*583*
*159*
*4MB*

*English*
*Pages 163*
*Year 2016*

- Author / Uploaded
- Jacqueline Perez (ed.)

MATERIALS SCIENCE AND TECHNOLOGIES

CERAMIC MATERIALS SYNTHESIS, PERFORMANCE AND APPLICATIONS

No part of this digital document may be reproduced, stored in a retrieval system or transmitted in any form or by any means. The publisher has taken reasonable care in the preparation of this digital document, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained herein. This digital document is sold with the clear understanding that the publisher is not engaged in rendering legal, medical or any other professional services.

MATERIALS SCIENCE AND TECHNOLOGIES Additional books in this series can be found on Nova’s website under the Series tab.

Additional E-books in this series can be found on Nova’s website under the E-book tab.

MATERIALS SCIENCE AND TECHNOLOGIES

CERAMIC MATERIALS SYNTHESIS, PERFORMANCE AND APPLICATIONS

JACQUELINE PEREZ EDITOR

New York

Copyright © 2017 by Nova Science Publishers, Inc. All rights reserved. No part of this book may be reproduced, stored in a retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic, tape, mechanical photocopying, recording or otherwise without the written permission of the Publisher. We have partnered with Copyright Clearance Center to make it easy for you to obtain permissions to reuse content from this publication. Simply navigate to this publication’s page on Nova’s website and locate the “Get Permission” button below the title description. This button is linked directly to the title’s permission page on copyright.com. Alternatively, you can visit copyright.com and search by title, ISBN, or ISSN. For further questions about using the service on copyright.com, please contact: Copyright Clearance Center Phone: +1-(978) 750-8400 Fax: +1-(978) 750-4470 E-mail: [email protected].

NOTICE TO THE READER The Publisher has taken reasonable care in the preparation of this book, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained in this book. The Publisher shall not be liable for any special, consequential, or exemplary damages resulting, in whole or in part, from the readers’ use of, or reliance upon, this material. Any parts of this book based on government reports are so indicated and copyright is claimed for those parts to the extent applicable to compilations of such works. Independent verification should be sought for any data, advice or recommendations contained in this book. In addition, no responsibility is assumed by the publisher for any injury and/or damage to persons or property arising from any methods, products, instructions, ideas or otherwise contained in this publication. This publication is designed to provide accurate and authoritative information with regard to the subject matter covered herein. It is sold with the clear understanding that the Publisher is not engaged in rendering legal or any other professional services. If legal or any other expert assistance is required, the services of a competent person should be sought. FROM A DECLARATION OF PARTICIPANTS JOINTLY ADOPTED BY A COMMITTEE OF THE AMERICAN BAR ASSOCIATION AND A COMMITTEE OF PUBLISHERS. Additional color graphics may be available in the e-book version of this book.

Library of Congress Cataloging-in-Publication Data Names: Perez, Jacqueline, editor. Title: Ceramic materials: synthesis, performance and applications / (editor) Jacqueline Perez. Description: Hauppauge, New York: Nova Science Publisher's, Inc., 2016. | Series: Materials science and technologies | Includes index. Identifiers: LCCN 2016035623 (print) | LCCN 2016038286 (ebook) | ISBN 9781634859653 (hardcover) | ISBN 9781634859806 Subjects: LCSH: Ceramic materials. Classification: LCC TA430 .C46 2016 (print) | LCC TA430 (ebook) | DDC 620.1/4--dc23 LC record available at https://lccn.loc.gov/2016035623

Published by Nova Science Publishers, Inc. † New York

CONTENTS Preface

vii

Chapter 1

Evaluation of Fly and Bottom Ash of Different Biomass Combustion as Raw Materials in Clay-Based Ceramics D. Eliche-Quesada, M. A. Felipe-Sesé and A. Infantes-Molina

Chapter 2

Nanostructured Ceramics for the Control of Heat Flows Evgenii I. Salamatov, Oksana V. Karban, Efim N. Khazanov and Andrey V. Taranov

33

Chapter 3

Analytical Model of Thermal Stresses in Multi-Component Materials with Cylindrical Particles Ladislav Ceniga

65

Chapter 4

Analytical Model of Thermal Stresses in Multi-Component Porous Materials Ladislav Ceniga

103

Chapter 5

An Update of Current Knowledge on Adhesion to Zirconia Dental Restorations M. L. P. D. Engler, E. Ruales, M. Özcan and C. A. M. Volpato

135

Index

1

153

PREFACE This book discusses the synthesis, performance and applications of ceramic materials. Chapter One presents the recycling of biomass ashes in the obtaining of clay bricks for possible use as construction material. Chapter Two summarizes the use of nanostructured ceramics for the control of heat flows. Chapter Three deals with analytical modelling of thermal stresses in a multiparticle-matrix system with isotropic cylindrical particles which are periodically distributed in an isotropic infinite matrix. Chapter Four deals with analytical modelling of thermal stresses which originate during a cooling process of an elastic solid continuum. Chapter Five provides recent information on the use of zirconia in dentistry, its characteristics and indications, with a particular emphasis on surface conditioning methods to promote adhesion of resin-based materials to zirconia. In Chapter 1, various fly and bottom biomass ash, such as: rice husk fly ash, wood bottom ash, fly and bottom pine-olive pruning ash, olive stone bottom ash, olive pomace bottom and fly ash, were individually blended with clay to produce ceramic bricks. The clay and biomass ash waste were characterized by X-ray fluorescence, elemental chemical analysis and thermogravimetric and differential thermal analysis. The bricks were manufactured by mixing clay and 20 wt% of ash. These bricks were fired at 900ºC. The influence of the type of biomass ash added on the linear shrinkage, bulk density, water absorption, apparent porosity and mechanical properties was investigated. The results indicated that the addition of biomass ash decreased the bulk density and the compressive strength (25% lower) although the incorporation of fly rice husk ash produced a maximum decreased of 60.8%. Instead it was observed an increment in water absorption from 4.0 to 17.3% with respect to the control bricks containing only clay. Heavy metal

viii

Jacqueline Perez

concentration in the leachates of the biomass ash-clay bricks was far lower than those recommended in the Spanish legislation (OM AAA/661/2013) and US-EPA standard. Therefore, fired bricks fulfill standard requirements for clay masonry units, offering, at the same time, good mechanical properties. The recycling of these biomass ashes in the obtaining of clay bricks for possible use as construction material is presented as a potentially feasible solution according to the technical qualities of the manufactured bricks, as well as, the economic and environmental benefits that implies its use in replacement of natural raw materials. As described in Chapter 2, nowadays considerable attention is paid to the creation of a new type of nanostructured materials in which one can control the heat flow. Since it is believed that the basic element of such thermocrystals should be phononic lattices with a wide forbidden gap, it is an urgent task to find new methods for their synthesis that strikes a balance between the thermocrystal efficiency and ease of fabrication. It is shown both theoretically and experimentally that the compacted ceramics can exhibit the properties of a phononic lattice, i.e., a forbidden gap may arise in the phonon spectrum. The position and width of the gap in such systems are determined by the average grain size of ceramics, as well as by the thickness and elastic properties of the grain boundaries. Inclusions of metal phase in dielectric matrix can create photonic traps for the nanocomposite materials and determine their diffusion ratio. The approach for the synthesis of nanocomposites by use of ceramics technology was introduced. It allows to create materials with required characteristics by the compaction and sintering process and to give a practical advice on synthesis of nanostructured ceramics with specified parameters. Chapter 3 deals with analytical modelling of thermal stresses in a multiparticle-matrix system with isotropic cylindrical particles which are periodically distributed in an isotropic infinite matrix. This multi-particlematrix system represents a model system which is applicable to real twocomponent materials of with precipitates of a cylindrical shape. The thermal stresses as functions of microstructural parameters (particle volume fraction, particle radius, inter-particle distance) originate during a cooling process as a consequence of the difference in thermal expansion coefficients of the cylindrical particle and the matrix. The analytical modeling is based on an application of suitable mathematical techniques on fundamental equations of mechanics of solid elastic continuum. The mathematical techniques thus result in analytical solutions for both the cylindrical particle and the infinite matrix.

Preface

ix

Finally, numerical values of the thermal stresses in a real two-component material with cylindrical precipitates are determined. Chapter 4 deals with analytical modelling of thermal stresses which originate during a cooling process of an elastic solid continuum. This continuum consists of an isotropic infinite matrix with isotropic spherical particles and spherical pores. The particles and pores are both periodically distributed in the infinite matrix which is imaginarily divided into identical cubic cells. Each cell contains either a central particle or a central pore. This porous multi-particle-matrix system represents a model system which is applicable to porous two-component materials of a precipitate-matrix type characterized by microstructural parameters, i.e. the cubic cell dimension; radii and volume fractions of both the particles and of the pores. The thermal stresses are a consequence of different thermal expansion coefficients of the isotropic matrix and isotropic particle. Resulting from fundamental equations of mechanics of an elastic solid continuum, the thermal stresses are determined within this cell, and thus represent functions of these microstructural parameters. Finally, numerical values for a real porous two-component material of the precipitate-matrix type are obtained. As explained in Chapter 5, Yttria-stabilized tetragonal zirconia polycrystal (Y-TZP) has been used in dentistry in order to manufacture prosthetic frameworks, monolithic crowns and implant abutments due to its superior mechanical properties, biocompatibility, chemical stability and appropriate aesthetics as opposed to other materials. The survival of dental ceramic restorations depends on durable bond strength between the restorative material, composite resin luting cement and the tooth surface. However, it is difficult to establish a durable mechanical or chemical adhesion in zirconiabased prostheses since yttrium-stabilized zirconia is an oxide ceramic that does not contain silicon dioxide (SiO2) phase in its microstructure. In order to achieve strong and reliable adhesion between resin composite luting cements and zirconia surfaces, it is crucial to employ a method that does not impair the mechanical properties and at the same time rendering it compatible with the luting cement. Furthermore, the chosen method should be practical, easy to perform and should not cause t→m phase transformation. Several methods and protocols for conditioning zirconia surfaces prior to adhesive cementation have been suggested in the literature such as physical, physicochemical and chemical methods. Typically, while physical surface conditioning methods are based on employing air-borne particle abrasion with alumina particles, physicochemical methods use silica-coated alumina particles followed by silanization. It is also possible to activate the zirconia surface chemically using

x

Jacqueline Perez

functional-monomer containing adhesive promoters in the form of adhesive cements or primers. Generally, combination of micromechanical and chemical surface conditioning methods are preferred to enhance adhesion to zirconia. As this ceramic demonstrates superior properties compared to other ceramics, it is essential to study the peculiar characteristics of dental zirconia after surface conditioning methods and suggest one that does not damage its favorable mechanical properties. Chapter 5 will provide the recent information on the use of zirconia in dentistry, its characteristics and indications, with a particular emphasis on surface conditioning methods to promote adhesion of resin-based materials to zirconia.

In: Ceramic Materials Editor: Jacqueline Perez

ISBN: 978-1-63485-965-3 © 2017 Nova Science Publishers, Inc.

Chapter 1

EVALUATION OF FLY AND BOTTOM ASH OF DIFFERENT BIOMASS COMBUSTION AS RAW MATERIALS IN CLAY-BASED CERAMICS D. Eliche-Quesada1,, M.A. Felipe-Sesé1 and A. Infantes-Molina2 1

Department of Chemical, Environmental, and Materials Engineering, Higher Polytechnic School of Jaén, University of Jaén, Jaén, Spain 2 Department of Inorganic Chemistry, Crystallography and Mineralogy (Associate Unit to the ICP-CSIC0, Faculty of Sciences, University of Malaga, Málaga, Spain

Abstract In this work, various fly and bottom biomass ash, such as: rice husk fly ash, wood bottom ash, fly and bottom pine-olive pruning ash, olive stone bottom ash, olive pomace bottom and fly ash, were individually blended with clay to produce ceramic bricks. The clay and biomass ash waste were characterized by X-ray fluorescence, elemental chemical analysis and thermogravimetric and differential thermal analysis. The bricks were manufactured by mixing clay and 20 wt% of

Address: Department of Chemical, Environmental, and Materials Engineering, Higher Polytechnic School of Jaén, University of Jaén, Campus Las Lagunillas s/n, 23071 Jaén, Spain (Corresponding author).

2

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina ash. These bricks were fired at 900ºC. The influence of the type of biomass ash added on the linear shrinkage, bulk density, water absorption, apparent porosity and mechanical properties was investigated. The results indicated that the addition of biomass ash decreased the bulk density and the compressive strength (25% lower) although the incorporation of fly rice husk ash produced a maximum decreased of 60.8%. Instead it was observed an increment in water absorption from 4.0 to17.3% with respect to the control bricks containing only clay. Heavy metal concentration in the leachates of the biomass ash-clay bricks was far lower than those recommended in the Spanish legislation (OM AAA/661/2013) and US-EPA standard. Therefore, fired bricks fulfill standard requirements for clay masonry units, offering, at the same time, good mechanical properties. The recycling of these biomass ashes in the obtaining of clay bricks for possible use as construction material is presented as a potentially feasible solution according to the technical qualities of the manufactured bricks, as well as, the economic and environmental benefits that implies its use in replacement of natural raw materials.

Keywords: fly and bottom biomass ash, recycling, ceramics, technological properties, sustainability

1. Introduction Economic and social development requires energy, in a manner that the need for energy consumption in developed countries is increasing at at a rate of nearly 1% a year, whereas the rate is higher in emerging countries, approximately 5% a year [1]. It is estimated that oil and gas reserves will only cover energy needs for the next 40 and 60 years, respectively. Furthermore, emissions generated as a result of fossil fuels combustion are responsible of serious environmental problems such as global warming. As a result, renewable energy seems to be one the most effective solution due to its renewable and environmentally sustainable nature [2] in order to ensure a high quality of life and the well-being of coming generations [3]. The energy generated from biomass is one of the most promising ways of reducing, in significant quantities, CO2 from the combustion of coal and natural gas. According to definition in Directive 2003/54/EC, “biomass” is the biodegradable fraction of products, waste and residues from biological origin from agriculture (including vegetal and animal substances), forestry and related industries including fisheries and aquaculture, as well as the biodegradable fraction of industrial and municipal waste (Directive 2003/54/EC) [4].

Evaluation of Fly and Bottom Ash …

3

Spain, following the ambitious European Union objectives has assumed the challenge to establish an ambitious energy model with the intention of promoting renewable resources like biomass to fulfill the energy targets. This is the aim of the “Plan de Acción Nacional de Energías Renovables” (PANER) (2010-2020) [5]. Andalusia (Spain) is the second-largest autonomous community in Spain, with wide forest and farmland surface and is the region that records the highest consumption in the country of the most promising source of renewable energy, biomass [6], with 18 generators of electricity from residual biomass which produce 257,48 MW [7]. Solid biomass is the best known type of biomass and can be included within this group: wood obtained from silviculture and forestry activities; wastes from industries dealing with any kind of solid biomass (e.g., carpentry, paper industry…); residues obtained from the pruning and cleaning of parks and gardens; energy crops; peat; agriculture and agro-industrial waste (such as pomace, sawdust, olive stones…); and organic fraction of solid urban wastes. Different sources of solid biomass are used in Andalusia to produce electric energy: olive pomace (218,3 Ktoe), energetic crops (190,4 Ktoe), forestry residues (106,7 Ktoe) and industrial wastes (175,6 Ktoe) depicted the main sources of solid biomass in 2013 of the total quantity (723,7 ktoe) [7]. The wastes generated from the olive sector in Andalusia, is the most important source of residual biomass for electric and thermal energy. Approximately 50% of biomass is olive tree residues; the other half is principally obtained from sunflowers, cotton and fruit trees [8]. It should be born in mind that Spain is the main world olive producer (4,577,800 tonnes) [9] and the production is mainly concentrated in Andalusia. The potential exploitation of solid olive wastes for energy purposes have been extensively researched [10-15]. However, an environmental and economic problem inherent to solid biomass combustion, stems from the large quantities of fly and bottom ashes generated from the process. Ash is usually accumulated in landfills which lead to a clear damage to the land and the surrounding area, contributing to air pollution and water contamination. In addition, the occupation of a territory stops it from being productive and the disposal in landfills is also problematic due to space limitations. The composition of the ash depends on the minerals absorbed or incorporated into the biomass during cultivation and harvesting. Likewise, ash is usually composed by organic material unburned during the usual inefficient processes [16]. Accordingly, the potential reuse of the ash is determined by its physical, chemical and environmental properties. Obviously, quality and quantity of the ash are directly influenced by the characteristics of the biomass and the combustion technology employed [17]. Regarding the type of ash, bottom ash is

4

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

the portion of residue that remains in the incinerator or furnace, while fly ash is the portion of ash that goes through the chimney and is retained to prevent it from being released into the atmosphere [18]. The management of the ashes produced in great quantity as a result of the combustion processes is a challenge. There have been an increasing number of studies in all over the world regarding the characterization and the establishing of appropriated processes in which ashes can be effectively reused. As a result of this research, different areas of application of ash were proposed, depending on its composition and properties. One of the most valuable components of the ash is amorphous silica, with a wide range of applications, such as manufacturing of silica gels, silicon chip, synthesis of activated carbon and silica, production of construction materials and insulation, zeolites, catalysts, ingredients for batteries, graphene, carbon capture, drug delivery vehicles [19]. In addition, biomass ashes have been studied focusing on applications as a construction material replacing, in part or completely, traditional construction materials. This has been fostered by the growing environmental awareness in the building industry due to the large quantities of raw materials needed for ceramic production [20, 21]. As a result, the incorporation of waste in place of traditional construction material, while requirements are fulfilled, is environmentally and economically attractive. Some authors have studied building materials using as raw materials ashes from different sources with satisfactory results. So, Cabrera et al. [16] studied the properties of biomass bottom ash from the combustion of wood and olive trees residues and determined that this bottom ashes had acceptable properties to be used as a filler material in the core of road embankments over 5 m in height without additional precautionary measures, such as the construction of road shoulders. Rauta et al. [22] studied brick samples prepared from paper pulp, rice husk ash and cement. The optimal composition with paper pulp (80 wt%), rice husk ash (10 wt%) and cement (10 wt%) had a higher strength and physicchemical characteristics than conventional burnt clay bricks. Zang et al. [23] studied the incorporation of municipal solid waste fly ash in clay bricks. The optimal mixture ratio of materials was, municipal fly ash: 20 wt%, red ceramic clay: 60 wt%, feldspar: 10 wt%, gang sand: 10 wt%. And the optimal sintering temperature was 950ºC. Other authors have studied the using of ash from coal power plants [24-29]. Eliche-Quesada and Leite-Costa [30] studied the using of bottom ash from olive pomace combustion to replace different amounts (10-50 wt%) of clay in brick manufacturing. The optimal amount of bottom ashes was 10 and 20 wt% of waste to produced bricks with lower bulk density and suitable compressive strength. Fired bricks fulfil standards requirements for clay masonry units, offering, at the same time, a reduction in thermal conductivity compared to

Evaluation of Fly and Bottom Ash …

5

control bricks (only clay). Cheeseman et al. [31] studied the use of sewage sludge incinerator ash to form new ceramic materials. Syed et al. [32] studied the incorporation of rice husk ash or sugarcane bagasse. Clay bricks incorporating with biomass ash exhibited lower compressive strength compared to that of clay bricks without waste. However, compressive strength of bricks with 5% of rice husk ash or sugarcane bagasse satisfied the standards. In the present study, clay bricks by means of conventional methods, using different types of biomass ashes have been manufactured. The samples of ashes were obtained from Andalusian biomass power plants that belong to the following companies: Tradema (Linares, Jaén), Herba Ricemills (San Juan de Aznalfarache, Sevilla), Aldebarán Energía del Gualdalquivir (Andújar, Jaén), Valoriza Energía and Energía La Loma S.A. (Villanueva del Arzobispo, Jaén). Tradema is a wooden board factory located in the town of Linares (Andalusia). The residues generated during the process constituted primarily of wood scraps from the bark of conifers (52%), wood dust and non-conforming products (48%) are used as fuel in the cogeneration plant in order to obtain electrical and thermal energy with 2 MW of power [7]. Herba Ricemills, is a factory located in San Juan de Aznalfarache (Andalusia) which produces energy from a power plant by the combustion of the rice husk, the external layer of the paddy grain that is separated from the rice grains during the milling process. In Andalusia 58,7 Ktn of rice husk were obtained derived from the industrial rice production [7], becoming an interesting source of biomass available in Andalusia, especially since one ton of rice husk can generate 800 Kw h [19]. Aldebarán Energía del Gualdalquivir uses biomass as a source of energy constituted of cereal straw and wastes from the maintenance and improvement treatments of the forests and olive groves. The cogeneration plant produces 6 MW of power. The forest waste depicted 1,34 Mt in Andalusia, while residues agricultural residues from olives groves, represented 2,52 Mt in 2013 [7]. Valoriza Energía Company is located in the Scientific and Technological Park Geolit at Mengibar (Jaen, Spain) provided air conditioning to the Park using as fuel olive stone. Olive pomace is a by-product resulting from the extraction of olive oil obtained directly from olives. From every ton of olive processed, 0,27 ton of olive oil and 0,73 ton of olive pomace will be produced. In turn, from olive pomace, oil is also recovered by a chemical process. The residue resulting from this last process is itself a potential source of renewable energy, with 4,200 kcal/kg as a calorific value. Furthermore, it should be taken into account that in a normal season, 840 Kt/year of this waste is obtained in Andalusia. On this basis, Energía La Loma S.A. uses this waste to generate 16 MW of electrical energy in its power plant [7].

6

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

In view of the above, the present work aims at providing further knowledge in the technological properties of clay bricks and biomass combustion bottom or fly ash (BA and FA) from the power plants previously mentioned. For this purpose, raw materials were characterized and clay-ash mixtures with 20 wt% of BA or FA were conformed. Green samples were fired at 900°C and the effect of type of ash was studied by physical, mechanicall and environmental properties.

2. Experimental 2.1. Preparation of the Samples Clay was supplied by a clay pit located in Bailen, Jaen (Spain). It was obtained by mixing three types of raw clay in the following percentages: 30 wt% red, 30 wt% yellow and 40 wt% black clay. To obtain uniform particle size, the clay was crushed and ground to yield a powder with a particle size suitable to pass through a 500 μm sieve. The rice husk fly ash was supplied by Herba Ricemills S.L., a rice-producing industry in San Juan de Aznalfarache (Seville, Spain). The ash was black because the burning temperature was not controlled. Wood bottom ash was supplied by the cogeneration plant belonging to Tradema S.L., a wooden board factory in Linares (Jaen, Spain). The raw materials are solid by-products generated during the process and composed primarily of wood scraps from conifer bark, wood dust, and non-conforming products. Pine-olive pruning fly and bottom ashes were supplied by the plant Aldebarán Energia del Guadalquivir S.L. located in Andújar (Jaen, Spain). This company generates renewable energy using as fuel biomass of the pruning of olive groves and forest pruning (pine). Olive stone bottom ash was supplied by Valoriza Energía company located in the Scientific and Technological Park Geolit at Mengibar (Jaen, Spain) provided air conditioning to the Park using as fuel olive stone. Olive pomace bottom and fly ash were supplied by the plant Energía de La Loma S.A. located in Villanueva del Arzovispo (Jaen, Spain). This company uses as a fuel, orujillo. 20 wt% of fly or bottom biomass ashes were added to the clay and mixed to obtain good homogenization. For comparative purposes, ten samples per series were prepared for the tests. The necessary amount of water (7-10 wt% moisture) was added to obtain an adequate plasticity and assess the absence of defects, mainly cracks, during the semi-dry compression moulding stage under 54.5 MPa of pressure, using an uniaxial laboratory-type pressing Mega KCK-30 A. Wastefree mixtures were also made as references. Solid bricks with 30 x 10 mm cross sections and a length of 60 mm were obtained. Samples were fired in a laboratory

Evaluation of Fly and Bottom Ash …

7

furnace at a rate of 3ºC/min up to 900ºC for 4 h. Samples were then cooled to room temperature by natural convection inside the furnace. The shaped samples were designated as C for the bricks without waste and C-20W for the mixtures, where W indicated the waste incorporated (RHFA (rice husk fly ash); WBA (wood bottom ash); POPFA (Pine-olive pruning fly ash); POPBA (pine-olive pruning bottom ash); OSBA (olive stone bottom ash); OPBA (olive pomace bottom ash) and OPFA (olive pomace bottom and fly ash)).

2.2. Characterization of Raw Materials A laser diffractometer Malvern Mastersizer 2000 was used to measure particle size distribution of different ash particles. Crystalline phases were evaluated in a X-ray diffractometry with a X´Pert Pro MPD automated diffractometer (PANanalytical) equipped with Ge (111) primary monochromator, using monochromatic Cu Kα radiation (λ= 1.5406 Å) and an X´Celerator detector. Chemical composition was determined by X-ray fluorescence (XRF) using the Philips Magix Pro (PW-2440). Thermal behavior was determined by thermogravimetric and differential thermal analysis (TGA-DTA) with a Mettler Toledo 851e device in oxygen. The total content of carbon, hydrogen, nitrogen, and sulphur was determined by combustion of samples in O2 atmosphere using the CHNS-O Thermo Finnigan Elementary Analyzer Flash EA 1112. The organic content was measured according to ASTM D-2974, Standard Test Method for Moisture, Ash, Organic Matter of Peat and Other Organic Soils [33]. The ignition temperature was 440°C. Carbonate content (expressed as calcium carbonate) was determined by calcimetry in a Bernard calcimeter.

2.3. Characterization of Clay-Ash Bricks Linear shrinkage was obtained by measuring the length of samples before and after the firing stage, using a caliper with a precision of ± 0.01 mm, according to ASTM standard C326 [34]. Water absorption values were determined from weight difference between the fired and water-saturated samples (immersed in boiling water for 2 h), according to ASTM standard C373 [35]. Open porosity (in vol.%) were determined from weight differences between saturated and dry mass with respect to exterior volume; and closed porosity (in vol.%) was calculated from weight difference between dry and suspended mass in water with respect to exterior volume according to ASTM standard C373 [35]. Bulk density was determined by the Archimedes method [35]. Water suction of a brick is the

8

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

volume of water absorbed during a short partial immersion. Tests to determine water suction was implemented according to standard procedure UNE-EN 772-1 [36]. An efflorescence study was carried out. To this end, the bricks were immersed in water for 24 h and dried in shade. After this treatment the presence of soluble salts in the bricks was determined. Compressive strength of bricks defined as their bulk unit charge against breakage under axial compressive strength. For this trial, six fired samples were studied. Tests on compressive strength were performed according to standard UNE-EN 772-1 [37] on a MTS 810 Material Testing Systems laboratory press. The area of both bearing surfaces was measured and the average taken. All samples were submitted to a progressively increasing normal strength, with the load applied on the center of the upper surface of the sample until breakage. The compressive strength of each sample was obtained by dividing the maximum load by the average surface of both bearing surfaces, expressed in MPa with 0.1 MPa accuracy. Table 1. Chemical composition of clay and biomass ash Oxide content (%) SiO2 Al2O3 Fe2O3 CaO MgO MnO Na2O K2O TiO2 P2O5 SO3 ZnO SrO ZrO2 Cl LOI

Clay

RHFA WBA

POPBA POPFA OPBA OPFA OSBA

54.4 12.36 4.58 8.76 2.46 0.03 3.37 0.60 0.11 0.68 0.026 0.027 0.033 12.51

76.7 0.183 0.233 0.821 0.654 2.03 1.62 0.035 17.78

48.1 9.3 3.2 17.7 2.73 0.10 3.83 0.473 1.01 0.023 0.023 0.047 12.73

48.6 5.94 3.26 18.1 3.2 0.051 0.92 1.85 1.39 0.52 0.14 0.281 0.0434 0.064 15.62

41.2 8.05 2.78 22.1 4.63 0.178 6.78 0.467 1.99 0.28 0.065 0.047 0.33 9.95

19.14 3.47 1.62 15.00 4.43 0.039 28.32 0.158 4.11 0.86 0.023 0.056 0.012 0.64 22.09

11.7 2.51 1.26 10.2 3.03 42.66 0.11 2.97 3.6 0.037 2.26 18.54

8.47 1.68 2.97 24.00 3.42 0.057 31.22 0.073 4.04 0.025 0.148 0.074 23.79

The development of porosity in samples was also evaluated by means of a scanning electron microscope (SEM), using the high-resolution transmission electron microscope JEOL SM 840, and the Energy Dispersive X-ray

Evaluation of Fly and Bottom Ash …

9

Spectroscopy (EDS) for chemical analysis (20 kV). Samples were placed on an aluminium grate and coated with carbon using the ion sputtering device JEOL JFC 1100. Leachability of heavy metals in the samples was studied using the toxicity characteristic leaching procedure (TCLP) according to EPA method 1311 [38]. The concentrations in the filtrate were measured with an Inductively Coupled Plasma-Atomic Emission Spectrometer (ICP-AES Agilent 7500).

3. Results and Discussion 3.1. Characterization of Raw Materials Table 1 shows the chemical composition of raw clay and different biomass ashes, determined by XRF. The raw clay had high amounts of SiO2 and Al2O3 as the predominant oxides, due mainly to the silicate in the clay. The content of CaO was significant and it is related to the abundance of carbonates. It had a relatively high content of Fe2O3, which confers the red colour. The rice husk ash contains a high proportion of pure silica (79.6%). The main components observed in the wood ash, and pine-olive pruning fly and bottom ashes were SiO2, CaO and Al2O3. The minor components were Fe2O3, K2O and MgO. On the other hand, K2O is the major oxide present followed by CaO and SiO2 in olive stone bottom ash and olive pomace bottom and fly ashes. High content in K2O is due to the oxide being a major component of the olive stone and pomace used as fuels. Chemical components of ceramic bodies can be classified into three groups: (1) skeleton components, which form the framework and surface of ceramic bodies, mainly consisting of SiO2 and Al2O3; (2) flux materials, which lowered the melting point, mainly containing alkaline metal oxide and alkaline-earth metal oxides such as CaO, Na2O, K2O and MgO; (3) gaseous components, which generate gases and bloat ceramic bodies during sintering at high temperature [39]. As indicated in Table 1, the total content of Si and Al (estimated as oxides) is higher in rise hush fly ash, wood bottom ash, pine-olive pruning fly and bottom ashes. High contents of fluxing oxides (K2O) and auxiliary fluxing oxides (CaO, MgO) in olive stone bottom ash and olive pomace bottom and fly ashes are suitable to lower the temperature of the firing process for brick preparation. The XRD patter of raw clay showed SiO2, CaCO3 as main crystalline phases and alumina-silicates of K-Mg or Fe-Mg in smaller proportion. X-ray diffraction patterns of the biomass ashes showed a series of crystalline phases within a glassy

10

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

matrix. In the X-ray diffraction pattern of WBA, POPBA and POPFA the major phases identified were SiO2 and CaCO3. The presence of tiny diffraction peaks indicated the presence of crystalline silicates of Al and Fe with alkaline earth elements (AlKSi3O8 and Ca5.74Fe0.26Si6O18) in WBA and some aluminosilicates such as Al0.5Ca2Mg0.75O7Si1.75, Al0.83Ca3.027Fe1.17O12Si3 and silicoaluminatesof Na and K in POPBA and POPFA. XRD patterns of OSBA, OPBA and OPFA are also complex and presenting a great number of diffraction peaks. These samples contain great quantities of potassium as observed from XRF analysis. Several diffraction peaks associated to K-crystalline phases were noticeable in all cases. As before, these samples are composed mainly of silicate, aluminosilicates of earth and alcalino-earth metals as well as carbonates. Some diffraction peaks were difficult to assign but pointed to the presence of phosphate and pyrophosphate compounds. Table 2. Carbonate content and CNHS analysis of raw materials Organic Carbonate matter contenta (%) content (%) Clay 2.29 ± 0.09 7.36 ± 0.33 RHFA 16.37 ± 0.17 5.61 ± 0.55 WBA 10.41 ± 0.09 17.25 ± 0.76 POPBA 5.10 ± 0.10 11.41 ± 0.10 POPFA 3.00 ± 0.08 18.95 ± 0.56 OPBA 7.80 ± 0.18 30.35 ± 0.75 OPFA 4.70 ± 0.27 31.20 ± 0.74 OSBA 11.83 ± 0.12 39.54 ± 0.89 a Determined according ASTM D-2974. Sample

%C

%H

%N

%S

2.25 ± 0.01 11.45 ± 0.04 6.15 ± 0.03 9.14 ± 0.18 4.79 ± 0.02 4.29 ± 0.01 3.34 ± 0.06 11.60 ± 0.01

0.34 ± 0.004 0.248 ± 0.005 0.622 ± 0.021 0.27 ± 0.022 0.05 ± 0.019 0.64 ± 0.005 0.47 ± 0.01 0.40 ± 0.02

0.05 ± 0.002 0.127 ± 0.0 0.204 ± 0.006 0.04 ± 0.006 0.04 ± 0.003 0.030 ± 0.00 0.043 ± 0.00 0.012 ± 0.0

0.032 ± 0.008 0.0 0.025 ± 0.001 0.0 0.018 ± 0.002 0.054 ± 0.009 0.211 ± 0.016 0.0

Oxides, such as quartz (SiO2) are produced at high temperature during the combustion process. Carbonates were also detected due to biomass fuel contains a high content of wood waste [40]. The detection of silica and calcite depends on the combustion temperature and the type of biomass used as fuel [41]. Traces of clay minerals were also detected. The mineralogical composition obtained for biomass ashes are consistent with other studies [42-44]. Also, according with background intensity, high content of glass phases indicated high activity of biomass ash to reduce the sintering temperature in the heating procedure. The average particle size, D50, was lower for POPFA and OPFA (fly ash), however RFHA presented an average particle size higher than the bottom ashes (Table 3). Therefore, POPHFA and OPFA have a higher reaction area per unit volume and higher surface energy per area, thus resulting in a higher activity [45].

Evaluation of Fly and Bottom Ash … Table 3. Average particle size D50 for fly and bottom biomass ashes Biomass ash RHFA WBA POPBA POPFA OPBA OPFA OEBA

Average particle size D50 (µm) 96,13 92,14 58,68 17,41 61,77 17,43 59,44

RHA

WBA

Figure 1. Continued on next page.

11

12

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina POPFA

Figure 1. XRD patterns of clay; RHFA; WBA; POPBA; POPFA; OPBA; OPFA and OSBA.

The CNHS analysis of biomass ashes (Table 2) showed that biomass ashes were composed mainly of carbon, hydrogen and a small quantity of nitrogen. OPFA, OPBA, WBA and POPFA also contained a small amount of sulphur. The carbon content is equivalent to the inorganic carbon derived from the decomposition of carbonates. Carbon content in ash usually depends on the efficiency of combustion technology. Large amounts of organic carbon in ash indicate incomplete combustion of biomass, which suggests inefficient fuel use [46]. The TGA/DTA curves of the clay and biomass ashes up to 900°C are shown in Figure 2. The weight loss of 1.0% between 30-150ºC of the raw clay, associated to the release of hydration water, showed an endothermic peak centered at 70°C. The weight loss of 2.2% between 150°C and 600°C can be attributed to the combustion of organic matter as indicates the exothermic effects centered at

Evaluation of Fly and Bottom Ash …

13

375 and 475ºC and to the silicate dehydroxylation as indicated the endothermic peak centered at 570ºC. Between 600°C and 800°C, the decomposition of calcium carbonate with the release of CO2 was indicated by the endothermic effect centered at 760°C with a mass loss of 8.2%.

47 45 43

41 39 37 35

7 6 5 4 3 2 1 0 -1 -2 -3

50 150 250 350 450 550 650 750 850

45 44 43 42 41 40 39 38 37 36 35

16 POPBA

12

10 8 6 4 2 0 -2

50 150 250 350 450 550 650 750 850

Temperature (ºC)

Temperature (ºC) 14

POPFA

42

10

40

8

38

6 4

36

OPB

12

A T (ºC)

Weight loss ( mg)

44

2 34

0

32

-2

30

14

T (ºC)

WBA

Weight loss ( mg)

Weight loss ( mg)

49

T (ºC)

Clay

-4 50 150 250 350 450 550 650 750 850

Temperature (ºC)

Figure 2. Continued on next page.

14

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

12

1 44

0,5

37 0

36 35

-0,5

34

-1

33

-1,5

32 31

-2

30

-2,5

50 150 250 350 450 550 650 750 850

Temperature (ºC)

Weight loss ( mg)

OPFA

T (ºC)

Weight loss ( mg)

38

OEBA

42

10

8

40

6

38

4

T (ºC)

39

36

2

34

0

32

-2

30

-4 50 150 250 350 450 550 650 750 850 Temperature (ºC)

Figure 2. DTA/TGA analysis of clay; RHFA; WBA; POPBA; POPFA; OPBA; OPFA and OSBA.

The TGA/DTA results of seven biomass ashes (Figure 2) indicated that weight loss curves are complex with gradual weight losses up to the final temperature 900ºC. The first weight loss at low temperature (30-200ºC) is due to, as indicated the endothermic peak, the presence of moisture in the sample. Release of organic matter (exothermic peak) and unburned elements (exothermic peak), such as residual carbon, occurred from 200-650ºC, indicating, in all cases, unburned carbon in the ash. Between 650-900ºC the decomposition of calcium carbonates (endothermic peak) emitting CO2 takes place. In all the biomass ashes except in the RHBA samples, several thermal effects occurred at higher temperatures. At 650ºC, an endothermic peak was observed due to elimination of structural water from the hydroxide ions in the biomass ash. The exothermic peak at 700ºC was probably ascribed to combustion reactions of the unburned elements in the ashes, while the endothermic effect at 750ºC may be due to carbonates decomposition.

3.2. Characterization of the Clay-Biomass Ash Bricks During firing process, changes of dimensions, mass and colour variations occurs into the clay-biomass ash bricks. It was observed that the bricks became darker, after firing at 900ºC the colour is reddish due to the iron content in clayed materials. No defects such as cracks, bloating or efflorescence were found after firing. Different technological properties of the biomass ash-clay bricks compared to the standard (only clay mixture) were studied.

Evaluation of Fly and Bottom Ash …

15

The linear shrinkage of the bricks reflects expansion/contraction behavior during thermal treatment. Shrinkage is a key parameter to evaluate the quality of fired bricks. The stress on the clay body increases as the shrinkage so does, therefore, large shrinkage may induce to tensions and even to broken pieces [47]. As indicated in Figure 3 addition of the biomass ash changed the linear shrinkage of the clay. The standard bricks had a linear shrinkage of -0.52 showing expansion behavior. Only the addition of RHFA produced contraction in the bricks. However, the addition the OSBA produced the highest increase in the linear shrinkage up to -1.88%. The addition of POPFA, OPFA and OPBA also produced an increased in this property showing values of -0.65%, -1.23% and -1.62% respectively. However the addition of POPBA waste does not change the linear shrinkage of the clay. Thus, clay samples, as well as samples containing biomass ash, except RHFA-clay bricks, expanded slightly when fired at 900ºC. This behavior could be due to the expansion in the ceramic body of the biomass ash amended bricks as a result of the gases released in the combustion of organic matter and carbonates decomposition, which caused the expansion. The addition of RHFA could reduce, at 900ºC, the liquid phase viscosity and the gases resulting from organic matter decomposition and CaCO3 could escape, producing shrinkage in the bricks. The values of linear shrinkage suggest that the introduction of 20 wt% of biomass ash showed linear shrinkage lower than 2.0%, within the safety limits for industrial production of clay bricks.

Figure 3. Linear shrinkage of clay bricks and clay–biomass ash bricks.

16

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

Figure 4 shows the weight loss of ignition of the brick samples. The control clay bricks present the lowest loss on ignition (9.2%). The addition of biomass ash increased the loss of ignition to values varying from 12% up to 15.2% with the addition of POPFA and OSBA respectively. The increase in the weight loss on ignition during the firing process could increase due to the contribution of organic matter and carbonate content as well as inorganic matter in clay and biomass ashes.

Figure 4. Loss of ignition of clay bricks and clay-biomass ash bricks.

Figure 5. Bulk density of the fired bricks as function of type of biomass ash addition.

Evaluation of Fly and Bottom Ash …

17

The addition of biomass ashes decreased the bulk densities of the fired bricks (Figure 5), which exhibited values ranging from 1,765to 1,520 kg/m3 lower than the values for control bricks of 1,832 kg/m3. The addition of 20 wt% of biomass ash decreased the bulk density in this order: WBA=OPFA>OPBA>POPFA>POPBA>OSBA>RHFA. The reduction in bulk density indicated that this type of wastes promotes an expansion reaction at firing temperature of 900ºC. In addition, the porosity increases with biomass ashes addition also playing an important role in reducing the weight of the bricks, declining labor and transportation costs.

Figure 6. Compressive strength of clay bricks and clay-biomass ash bricks.

The compressive strength is another important parameter to consider in order ensuring the engineering quality of the bricks. The results of compressive strength are shown in Figure 6. Test results showed that the standard bricks had higher compressive strength (53.4 MPa). The highest compressive strength is achieved with the addition of WBA, 46.7 MPa, a reduction of 12.5% compared to the bare clay. If OPFA and OPBA are added, the compressive strength is reduced by 2530%, respectively; and 37-39% with the addition of OSBA, POPBA and POPFA. The highest reduction in the compressive strength with respect to control bricks is obtained with the addition of RHFA, this parameter decreased up to a 60.8%. It should be pointed that the compressive strength of bricks mainly depends on their bulk density, amount and type of porosity, and pore size distributions [48-50]. A linear relationship between compressive strength and apparent porosity as well as compressive strength and water absorption was observed as shown in Figure 7.

18

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

Decomposition of organic matter and carbonates can lead to higher porosity. Samples containing biomass ash had lower bulk density and greater total porosity, having higher open porosity than control brick based on water absorption data. Open pores and other microscopic imperfections acted as stress concentrator notches and reduced the compressive strength. The high amount of silica present in RHFA can lead to higher porosity. Generally, silica content in clay bricks ranged between 50-60%, higher amount is undesirable [51], since reduces the mechanical properties of bricks. RHFA has a 76.7% of silica and explains the lower bulk density and higher apparent porosity and water absorption. According to ASTM C62-10 [52] and European Standard EN-772-1 [37], the compressive strength varies from 10 MPa for weather-resistant brick to 20 MPa in the case of severe weathering. Therefore, it can be used 20 wt% of biomass ashes to replace clay for sustainable bricks. Only samples with 20 wt% of RHFA content had compressive strength rates close to the minimum (20 MPa) required by the standard threshold value for severe weathering. Apparent porosity as a function of biomass ashes is shown in Figure 8. It can be observed that standard bricks have the lowest apparent porosity (31.0%) whereas RHFA bricks have highest apparent porosity values (43.0%). The addition of WBA and OPFA increased the apparent porosity by 10%, 17% for OPBA and OSBA, 25% for POPFA and POPBA and 39% for RHFA. Porosity is related to biomass residual combustion, carbonate decomposition and dehydroxilation reactions [53].

Figure 7. Relationship between compressive strength and apparent porosity and compressive strength and water absorption of clay-biomass ash bricks.

Evaluation of Fly and Bottom Ash …

19

Figure 8. Apparent porosity of clay bricks and clay-biomass ash bricks.

Figure 9. Effect of biomass ash addition on water absorption of the fired bricks.

Water absorption is an important factor affecting the durability of bricks. Low water absorption values indicate a greater life of ceramic specimens and resistance to external weather conditions. The test results of the water absorption increased with biomass ash incorporated in the bricks (Figure 9). Control bricks showed the minimum water absorption of 16.9% since they had the highest density and the lowest apparent porosity. It is noteworthy that C-20RHBA bricks showed the

20

D. Eliche-Quesada, M.A. Felipe-Sesé and A. Infantes-Molina

maximum water absorption value (28.4%), while the minimum water absorption value is obtained by incorporating WBA (19.5%). The open porosity increased in the following order: WBA 3, λ2 < −2 with respect to µ ∈ (0, 0.5). Considering Eq. (35), the partial differential equation (28) is transformed to the form 2 ∂ 2 u011 1 ∂u011 u011 1 − 2µ X (11) λ(11) −2 + − 2 =− Ci r i . ∂r 2 r ∂r r 2 (1 − µ)

(37)

i=1

Using the Wronskian’s method [25], the function u011q = u011q (r, ϕ) (see Eq. (26)) which represents a solution of Eq. (28) for the cylindrical particle (q = p) and the cell matrix (q = m) has the form 2 X

u011q =

(11)

Ciq

(11)

uiq .

(38)

i=1 (11)

(11)

The integration constant Ciq = Ciq (ϕ) (i = 1,2) as a function of the variable ϕ ∈ h0, π/2i is determined by the boundary conditions (see Eqs. (53), (58), (63)–(73)) for the cylindrical particle (q = p) and the cell matrix (q = m). (11) (11) (11) (11) The two solutions u1q = u1q (r), u2q = u2q (r) of the partial dif(11)

(11)

ferential equation (37), and consequently the coefficients ξ1q , ξ2q have the forms (11)

uiq

(11) λ(11) iq

= ξiq

(11)

ξiq (11)

where u1q

=−

(11)

r

(11)

(q = p,m)

(11)

, i = 1, 2; λ1q > 3, λ2q < −2

1 − 2µq h , i = 1, 2, i (11) 2 2 (1 − µq ) λiq −1 (11)

= u1q (r) and u2q

(39) (40)

(11)

= u2q (r) are increasing and decreasing

(11)

(11)

functions of the variable r due to λ1q > 3 and λ2q < −2, respectively. 4.2.2.

Function u033q = u033q (x3 )

The partial differential equation (32) can be solved provided that the following two conditions are required to be both valid ∂u031q 1 ∂ 1 ∂ 0 r u11q = 1 ∧ r = 1, (41) r u031q ∂r r u031q ∂r ∂r

76

Ladislav Ceniga

and consequently, these two conditions result in the following partial differential equation derived as ∂u031q = u011q . (42) ∂r With regard to Eq. (42), the partial differential equation (29) is transformed to the form ∂ 2 u013q 1 + 2µq ∂u033q . (43) = − 1 − 2µq ∂x3 ∂x23 and then we get ∂u013q 1 + 2µq 0 =− u . ∂x3 1 − 2µq 33q

(44)

With regard to Eqs. (42), (44), the partial differential equation (32) is derived as ∂ 3 u033q 2µq − u0 = 0. ∂x3 ∂x3 1 − 2µq 33q

(45)

If the function u033q = u033q (x3 ) (see Eq. (27)) is assumed in the form u033q = eλq x3 , then the solution u033q = u033q (x3 ) of the differential equation (32) has the form (33)

(33)

u033q = C1q eλq

x3

(33)

(33)

+ C2q e−λq

x3

,

(46)

(33)

where the integration constant Ci (i = 1,2) which is not a function of the (33) variables r, ϕ, x3 (see Eq. (2)), ϕ ∈ h0, π/2i (i.e. Ciq 6= f (r, ϕ, x3)) is determined by the boundary conditions (see Eqs. (54)–(56), (74)–(69)) for the (33) cylindrical particle (q = p) and the cell matrix (q = m). The exponent λq is derived as s 2µq (33) λq = , (47) 1 − 2µq where (1 − 2µq ) > 0, and then [2µq / (1 − 2µq )] > 0 due to µq ∈ (0, 0.5) for real materials [9].

Analytical Model of Thermal Stresses ... 4.2.3.

77

Function u013q = u013q (r, ϕ)

Finally, with regard to Eqs. (44), (47), the function u013q = u013q (r, ϕ) has the form h i (33) (33) 1 + 2µq (13) (13) (13) u013q = − p C1q eλq x3 − C2q e−λq x3 + C3q , (48) 2µq (1 − 2µq ) (13)

where the integration constant Ciq

(i = 1,2,3) which is not a function of the

(13) Ciq

variables r, ϕ, x3 (i.e. 6= f (r, ϕ, x3)) is determined by the boundary conditions (see Eq. (62)) for the cylindrical particle (q = p) and the cell matrix (q = m). 4.2.4.

Function u031q = u031q (r)

With regard to Eqs. (39), (42), the function u031q = u031q (r) is derived as (11)

u031q

=

(31)

ξ1q C1q (11) λ1q

+1

r

(11)

λ1q +1

(31)

where the integration constant Ciq

(11)

+

(31)

ξ2q C2q (11) λ2q

+1

(11)

r λ2q

+1

(31)

+ C3q ,

(49)

(i = 1,2,3) which is not a function of the

(31) Ciq

variables r, ϕ, x3 (i.e. 6= f (r, ϕ, x3)) is determined by the boundary conditions (see Eq. (60)) for the cylindrical particle (q = p) and the cell matrix (q = m).

5.

Reason of Thermal Stresses

The thermal stresses originate during a cooling process at the temperature T ∈ hTf , Tr i, where Tf and Tr [26] are final and relaxation temperature of the cooling process, respectively. As defined in [26], the relaxation temperature Tr is such temperature below that the stress relaxation as a consequence of thermalactivated processes does not occur in a material. The relaxation temperature is defined approximately by the relationship Tr = (0.35 − 0.4) × Tm [26] and exactly by an experiment, where Tm is a melting point of a two-component material. If precipitates are formed from a liquid matrix of the two-component material, then the melting point Tm represents minimum of the set {Tmp , Tmm},

78

Ladislav Ceniga

where Tmp and Tmm are melting points of the precipitate (particle) and the matrix [26], respectively. If the precipitates are formed from a solid matrix, then Tm represents a melting point of the two-component material [26]. The thermal stresses which originate at the temperature T ∈ hTf , Tr i are thus a consequence of the condition βm − βp 6= 0. The coefficient βq is derived as ZTr βq = αq dT, q = p, m, (50) T

where αq is a thermal expansion coefficient of the cylindrical particle (q = p) and the matrix (q = m). Within the analytical modelling presented in this chapter, this cooling process is characterized by a homogeneous temperature change. Using the cylindrical coordinates (r, ϕ, x3) (see Fig. 2), the homogeneous temperature change is then characterized by the condition ∂T /∂r = ∂T /∂ϕ = ∂T /∂x3 = 0.

6. 6.1.

Determination of Radial and Axial Displacements Analysis of Radial and Axial Displacements

With regard to the boundary conditions for the cylindrical particle and the cell matrix, the following analysis of displacements which is based on a concept of imaginary separation is required to be considered. As presented in Sec. 5, the thermal stresses originate at the temperature T ∈ hTf , Tr i. Let the cylindrical particles and the infinite matrix be imaginarily separated, and then cylindrical holes are periodically distributed in the infinite matrix at inter-hole distance (see Fig. 1). Let T ∈ hTf , Tr i represent temperature of the separated cylindrical particles and of the infinite matrix with the cylindrical holes. If the temperature T increases or decreases within the interval hTf , Tri, then the components which are imaginarily separated expand or contract, respectively. The expansion and contraction result in displacements of points in the components. Due to the imaginary separation, these displacements result from the temperature change, and not from the difference βm − βp 6= 0 (see Eq. (50)), where this difference is a reason of the thermal stresses. In other words, let the cylindrical particles be embedded in the infinite matrix. Let ∆T = T − Tr 6= 0 represent the temperature change. Let the condition βp = βm be considered. If βp = βm , then the thermal stresses do not originate

Analytical Model of Thermal Stresses ...

79

in the multi-particle-matrix system, and the infinitesimal cylindrical cap is thus shifted due to the temperature change ∆T only and not due to the difference βm − βp 6= 0 i.e. not due to (αm − αp) ∆T provided that αq (q = p,m) is not a function of the temperature T . This shift (displacement) of the infinitesimal cylindrical cap is not induced by the thermal stresses. Let Rr , Lr represent dimensions of both the cylindrical particle and the cylindrical hole at the temperature T = Tr . The radius Rq and the length Lq of both the cylindrical particle (q = p) and the cylindrical hole (q = m) at the temperature T < Tr are derived as Rq = Rq (1 − βq ) , T < Tr ,

(51)

Lq = Lr (1 − βq ) , T < Tr ,

(52)

where Rq is not a function of x3 ∈ h0, Lq /2i due to the fact that βq is not a function of x3 and Lq is not a function of r ∈ h0, Rq i due to the fact that βq is not a function of r, i.e. Rq 6= f (x3 ) and Lq 6= f (r) due to βq 6= f (r, x3), respectively. Additionally, let dr represent inter-particle distance (= inter-hole distance) at the temperature T = Tr , and then we get d = dr (1 − βm ) at the temperature T < Tr . The following analysis concerning the radial displacement u011q and the axial displacement u033q (q=p,m) (see Eqs. (26), (27)) explains a way how to put the separated cylindrical particle with the dimensions Rp, Lp into the cylindrical matrix hole with the dimensions Rm , Lm in a centre of the cubic cell on the condition βp < βm which results in Rp > Rm , Lp > Lm , i.e. how to put the bigger cylindrical particle into the smaller cylindrical matrix hole in a centre of the cubic cell. This analysis is also valid for the condition βp > βm which results in Rp < Rm. Additionally, due to the matrix infinity, the following analysis is valid for each cubic cell of the multi-particle-matrix system (see Fig. 1). Let the condition βp < βm be considered, and then we get Rp > Rm , Lp > Lm . To put a bigger cylindrical particle into a smaller cylindrical matrix hole in a centre of the cubic cell, the radii Rp , Rm are both required to be changed to R, as well as Lp , L m are both required to be changed to L. The radial displacement u01p r=R = R − Rp 6= f (x3 ) and (u01m )r=Rm = p R − Rm 6= f (x3 ) in the cylindrical particle and the cylindrical matrix hole, respectively, are not functions of x3 due to Rq 6= f (x3 ) (q = p,m). With regard to the Cartesian system (Ox01 x02 x03 ) as well as from a mathematical point of view,

80

Ladislav Ceniga

the radial displacement u01p is considered to be negative, i.e. u01p = − u01p , and accordingly, the absolute value is considered. Similarly, the axial displace 0 ment u3q x =L /2 = (L − Lq ) /2 6= f (r, ϕ) is not a function of both r and q 3 ϕ due to Lq 6= f (r, ϕ) (q = p,m). The same analysis is valid on the condition βp > βm . Numerical values of R and L are determined by experimental methods for a real two-component material of the precipitate-matrix type with cylindrical precipitates. Due to βq 1 for α ∝ 10−6 and (Tr − T ) ∝ 10 − 102 (see Eq. (50)) [26], the radius Rr and Lr at Tr ∝ 103 are replaced by R and L, respectively. Accordingly, we get (53) u01m r=R − u01p r=R = R (βm − βp) , L (βm − βp) . (54) 2 The condition (53) represent one of the boundary conditions (see Sec. 6.2) (1) (1) (1) for the determination of the integration constants C1p , C1m , C2m in Eqs. (57), (58), (61), (62). Similarly, the condition (54) represent one of the boundary (3) conditions (see Sec. 6.2) for the determination of the integration constants C1p , u03m

(3)

(3)

(3)

x3

− u03p =L/2

x3 =L/2

=

C2p , C1m , C2m in Eqs. (55), (56), (59), (60). With regard to βp < βm , the matrix cylindrical part with dimensions R and (d − L) /2 which is defined within the intervals r ∈ h0, Ri and x3 ∈ hL/2, d/2i is pushed along the axis +x03 by the cylindrical particle (see Fig. 2). On the contrary, the cylindrical particle is pushed by this matrix cylindrical part along the axis −x03 (see Fig. 2), i.e. along a direction which is opposite to the direction of the pushing of this the matrix cylindrical part. This pushing is homogeneous over the surface S3 of the particle-matrix boundary with the normal x03 and with the surface area A3 = πR2 , and then the axial displacement u03p = u03p (x3 ) as a function of x3 ∈ h0, L/2i and the axial displacement u03m = u03m (x3 ) as a function of x3 ∈ hL/2, d/2i are not functions of both r and ϕ, i.e. u03p = u03p (x3 ) 6= f (r, ϕ) for x3 ∈ h0, L/2i and u03m = u03m (x3 ) 6= f (r, ϕ) for x3 ∈ hL/2, d/2i. Accordingly, the absolute value u03p = f (x3 ) 6= f (r, ϕ) for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i is required to represent an increasing function of x3 , exhibiting a maximum value on the particle-matrix boundary, i.e. for x3 = L/2. Consequently, the absolute value |u03m | = f (x3 ) 6= f (r, ϕ) for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i is required to represent a decreasing

Analytical Model of Thermal Stresses ...

81

function of x3 , exhibiting a maximum value on the particle-matrix boundary, i.e. for x3 = L/2. With regard to Eqs. (27), (46), (49), the axial displacement u03p = 0 u3p (x3 ) 6= f (r, ϕ) in the cylindrical particle for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i and the axial displacement u03m = u03m (x3 ) 6= f (r, ϕ) in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i have the forms (3)

(33)

(3)

(33)

u03p = u03p (x3 ) = C1p eλp x3 + C2p e−λp D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , 2 2 (3)

(33)

(3)

x3

(55)

(33)

u03m = u03m (x3 ) = C1m eλm x3 + C2m e−λm D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , 2 2 2 (31)

(31)

(33)

,

(3)

x3

, (56) (33)

(33)

where C1q = C2q = 0, C3q 6= 0 (see Eq. (49)), and Ciq = Ciq C3q (q = p,m; i = 1,2). Similarly, this pushing is also homogeneous over the surface S1 of the particle-matrix boundary with the normal x01 and with the surface area S1 = 2πRL/2, and then the radial displacement u01p = u01p (r, ϕ) as a function of the variables r ∈ h0, Ri, ϕ ∈ h0, π/2i along with the radial displacement u01m = u01m (r) as a function of the variables r ∈ hR, rci, ϕ ∈ h0, π/2i (see Fig. 3, Eq. (2)) are not functions of x3 for x3 ∈ h0, L/2i, i.e. u01p = u01p (r, ϕ) 6= f (x3 ) for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i and u01m = u01m (r, ϕ) 6= f (x3 ) for r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i. The conditions (53), (54) and the analysis mentioned above are also valid on the condition βp > βm . With regard to βp > βm , the matrix cylindrical part which is defined within the intervals r ∈ h0, Ri and x3 ∈ hL/2, d/2i is pulled along the axis +x03 by the cylindrical particle (see Fig. 2). On the contrary, the cylindrical particle is pulled by this matrix cylindrical part along the axis −x03 (see Fig. 2). This pulling is also homogeneous over the surface S3 of the 0 particle-matrix boundary with the normal 0 x3 . Accordingly, the absolute value u1p = f (r, ϕ) 6= f (x3 ) for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i is required to represent an increasing function of r, exhibiting a maximum value on the particle-matrix boundary, i.e. for r = R. Consequently, the absolute value |u01m | = f (r, ϕ) 6= f (x3 ) for r ∈ hR, rci,

82

Ladislav Ceniga

ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i is required to represent a decreasing function of r, exhibiting a maximum value on the particle-matrix boundary, i.e. for r = R. With regard to Eqs. (26), (38), (48), the radial displacement u01p = u01p (r, ϕ) 6= f (x3 ) in the cylindrical particle for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i and the radial displacement u01m = u01m (r, ϕ) 6= f (x3 ) in the cell matrix for r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as u01p

=

u01p

(r, ϕ) =

(11) (1) (11) C1p ξ1p r λ1p ,

D πE L , x3 ∈ 0, , r ∈ h0, Ri , ϕ ∈ 0, 2 2 (57)

(1) (11)

(11)

(1) (11)

(11)

u01m = u01m (r, ϕ) = C1m ξ1m r λ1m + C2m ξ2m r λ2m , D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , 2 2 (33)

where C1q (33)

(11)

(33)

= C2q

(33)

= 0, C3q

(1)

(33)

(1)

(u01m )r→0 → ±∞ due to (11) C2p

(1)

6= 0 (see Eq. (48)), and C1p = C1p (ϕ) = (11)

C3p C1p (ϕ), Cim = C3m Cim (ϕ) for i = 1,2. (11) λ2p

(58)

(11)

If C2p

6= 0 then

< −2 (see Eqs. (36), (39)), and accordingly (11)

the coefficient is required to be C2p = 0. With regard to the axial displacement u03m = u033m (x3 ) × u031m (r) (see Eq. (27)) in the cell matrix for r ∈ hR, rci (see Fig. 3, Eq. (2)), the absolute value |u03m | is required to represent a decreasing function of r. Accordingly, the function u031m = u031m (r) (see Eq. (49)) is required to represent a decreasing function of r ∈ hR, rci (see Fig. 3, Eq. (2)), exhibiting a maximum value on the particle-matrix boundary, i.e. for r = R. With regard to Eq. (49), we get (31) (11) (31) (31) C1m = 0 due to λ1m > 3 (see Eqs. (36), (39)), C2m 6= 0 and C3m = 0. Additionally, with regard to the interval x3 ∈ h0, L/2i, the axial displacement u03m = u03m (r, x3 ) is required to fulfil the condition (u03m )r=R = u03p (x3 ) 6= f (r, ϕ) for ϕ ∈ h0, π/2i (see Eq. (55)). With regard to the interval x3 ∈ hL/2, d/2i, the axial displacement u03m = u03m (r, x3 ) for r = R (i.e. (u03m )r=R ) is required to be equal to the axial displacement u03m = u03m (x3 ) 6= f (r, ϕ) given by Eq. (56) which is defined for the intervals r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i. With regard to these boundary conditions, the axial displacement u03m = 0 u3m (r, x3) defined in the intervals x3 ∈ h0, L/2i and x3 ∈ hL/2, d/2i, both

Analytical Model of Thermal Stresses ...

83

for r ∈ hR, rci and ϕ ∈ h0, π/2i (see Fig. 3, Eq. (2)), has the forms h i r λ(11) (33) (33) 2m (3) (3) u03m = u03m (r, x3) = C1p eλp x3 + C2p e−λp x3 , R D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , 2 2

(59)

h i r λ(11) (33) (33) 2m (3) (3) u03m = u03m (r, x3) = C1m eλm x3 + C2m e−λm x3 , R D πE L d , x3 ∈ , , (60) r ∈ hR, rci , ϕ ∈ 0, 2 2 2 h i h i (11) (31) (11) (11) where C2m = λ2m + 1 / ξ2m Rλ2m for both intervals x3 ∈ h0, L/2i and x3 ∈ hL/2, d/2i. With regard to the radial displacement u01m = u011m (r, ϕ) × u031m (x3 ) (see Eq. (26)) in the cell matrix for ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i, the absolute value |u01m | is required to represent a decreasing function of x3 . Accordingly, the function u013m = u013m (x3 ) (see Eq. (48)) is required to represent a decreasing function of x3 ∈ hL/2, d/2i, exhibiting a maximum value on the particle(13) matrix boundary, i.e. for x3 = L/2. With regard to Eq. (48), we get C1m = 0 (33) (13) (13) due to λm > 3 (see (see Eq. (47))), C2m 6= 0 and C3m = 0. Additionally, with regard to the interval r ∈ h0, Ri, the radial displacement u01m = u01m (r, ϕ, x3) is required to fulfil the condition (u01m )x3 =L/2 = u01p (r, ϕ) 6= f (x3 ) (see Eq. (57)). With regard to the interval r ∈ hR, rci (see Fig. 3, Eq. (2)), the radial displacement u01m = u01m (r, ϕ, x3) for x3 = L/2 (i.e. (u01m )x3 =L/2 ) is required to be equal to the radial displacement u01m = u01m (r, ϕ) 6= f (x3 ) given by Eq. (58) which defined for the intervals r ∈ hR, rci and x3 ∈ h0, L/2i. With regard to these boundary conditions, the radial displacement u01m = u01m (r, ϕ, x3) defined in the intervals r ∈ h0, Ri and r ∈ hR, rci (see Fig. 3, Eq. (2)), both for ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i, has the forms (1) (11)

(11)

(33)

u01m = u01m (r, ϕ, x3) = C1p ξ1p r λ1p e−λm D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , 2 2 2

[x3 −(L/2)]

, (61)

84

Ladislav Ceniga » – (11) (11) (33) (1) (11) (1) (11) u01m = u01m (r, ϕ, x3 ) = C1m ξ1m rλ1m + C2m ξ2m rλ2m e−λm [x3 −(L/2)] , fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , , (62) 2 2 2

i hp (33) (13) where C2m = eλm L/2 2µm (1 − 2µm )/ (1 + 2µm ) for both intervals x3 ∈ h0, L/2i and x3 ∈ hL/2, d/2i. (1) (1) (3) The integration constants C1p , Cim , Ciq (i = 1,2; q = p,m) in Eqs. (55)– (62) are determined by the boundary conditions in Sec. 6.2.

6.2.

Boundary Conditions

The boundary conditions for the determination of the integration constants (1) (1) C1m , C2m in Eqs. (57), (58) have the forms 0 σ11p = −p1 , (63) r=R 0 = −p1 , (64) σ11p r=R (65) u01m r=rc = 0,

(1) C1p ,

and additionally, the boundary condition (53) is also considered for the determination of the radial stress p1 acting at the particle-matrix boundary for r = R, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i. With regard to Eqs. (17), (57), (58), (63)–(65), we get (1)

Cim = −

P1 , (11) (11) (11) (11) ξ im ξ2+im ξ4+im Rλim −1 P1

(1)

C1p = −

(11) (11) (11) ξ1p ξ3p Rλ1p −1

i = 1, 2,

,

(66)

(67)

(11)

where the coefficient ξ iq (i = 1,2; q = p,m) is given by Eq. (40), and the coeffi(11)

(11)

cients ξ2+iq , ξ4+im are derived as (11)

(11)

ξ2+iq = λiq (c1q + c2q ) − c2q , i = 1, 2; q = p, m, (11)

(11) ξ4+im

=1−

ξ5−im (11)

ξ2+im

R rc

(11) λ(11) 3−im −λim

, i = 1, 2.

(68) (69)

Analytical Model of Thermal Stresses ...

85

The boundary conditions for the determination of the integration constants (3) (3) (3) (3) C1p , C2p C1m , C2m in Eqs. (55), (56) are derived as u03p x =0 = 0, (70) 3

u03m

∂ 2 u03p ∂x23

!

x3 =d/2

=

x3 =L/2

= 0,

∂ 2 u03m ∂x23

(71)

,

(72)

x3 =L/2

and additionally, the boundary condition (54) is also considered. With regard to Eqs. (55), (56), the axial displacement ε033p = ε033p (x3 ) and ε033m = ε033m (x3 ), which are defined within the intervals r ∈ h0, Ri, ϕ ∈ h0, π/2i, represents functions of x3 ∈ h0, L/2i and x3 ∈ hL/2, d/2i, respectively. A connection of these functions for x3 = L/2 is assumed to be ’smooth’. Due to this assumption of the ’smooth’ connection for x3 = L/2, these dependences ε033p − x3 and ε033m − x3 for r ∈ h0, Ri, ϕ ∈ h0, π/2i are thus required not to mutually create a singular point for x3 = L/2. To fulfil this non-singularity assumption, a tangent of ε033p = ε033p (x3 ) for x3 = L/2 is equal of a tangent of ε033m = ε033m (x3 ) for x3 = L/2, i.e. ∂ε033p/∂x3 x =L/2 = (∂ε033m/∂x3 )x3 =L/2 . With regard to Eq. (5), the con3 dition ∂ε033p/∂x3 x =L/2 = (∂ε033m/∂x3 )x3 =L/2 results in the boundary con3 dition given by Eq. (72. With regard to Eqs. (55), (56), (70)–(72), we get (3)

Cim =

L (βm − βp ) (3)

2 ξi

(3)

(3)

C1p = −C2p =

, i = 1, 2,

L (βm − βp) (3)

2 ξ3

(73)

,

(74) (3)

(3)

(3)

where βm , βq are given by Eq (50), and the coefficients ξ1 , ξ2 , ξ3 have the forms h i h i (33) 2 (33) 2 h i (33) λp − λm (33) (3) ξ1 = 1 − eλm (d−L) eλm L/2 , (75) h i2 (33) λp (3)

(3)

(33)

ξ2 = ξ1 e−λm

d

,

(76)

86

(3)

ξ3

Ladislav Ceniga h i h i (33) 2 (33) 2 " # 2 λp − λm (33) L λp = sinh . h i 2 (33) 2 λm

(77)

The coefficient P1 = P1 (ϕ), and the radial stress p1 = p1 (ϕ) acting at the particle-matrix boundary for r = R, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as h i (33) (33) 0 L c λ cosh λ x p 2m p 3 (βm − βp ) ∂u3p βm − βp P1 = p1 −c2m = = p − , 1 (1) (3) ∂x3 ξ1 ξ3 (78) h i (33) (33) 1 L c2m λp cosh λp x3 p1 = (βm − βp ) + , (79) (3) ξ (1) ξ 1 3 (1)

where the coefficient ξ1 has the form " # (11) (11) (11) ξ1p ξ1m ξ2m (1) ξ1 = (11) − (11) (11) + (11) (11) . ξ3p ξ3m ξ5m ξ4m ξ6m

(80)

The boundary conditions for the determination of the axial stress p3 acting at the particle-matrix boundary for x3 = L/2 within the intervals ϕ ∈ h0, π/2i, r ∈ h0, Ri are derived as 0 σ33p = −p3 , (81) x3 =L/2 0 σ33m = −p3 . (82) x =L/2 3

With regard to Eqs. (19), (55)–(57), (61), (71), (75)–(69), the axial stress p3 acting at the particle-matrix boundary for x3 = L/2 within the intervals ϕ ∈ h0, π/2i, r ∈ h0, Ri has the form h i2 (33) (33) L (βm − βp) λp λm p3 = h i h i2 h i2 ff (11) (11) (33) (33) 2 ξ9p − ξpm λp − λm ( " # " #) (11) (33) (33) (11) ξ9p (c1m + c2m ) ξpm (c1p + c2p ) L λp (d − L) λm × coth + coth , (33) (33) 2 2 λp λm

(83)

(11)

where the coefficient ξpm is derived as h i (11) (11) ξpm = −c2m 1 + λ1p .

(84)

Analytical Model of Thermal Stresses ...

6.3. 6.3.1.

87

Radial and Axial Displacements Cylindrical Particle

The radial displacement u01p = u01p (r, ϕ) (see Eq. (57)) and the axial displacement u03p = u03p (x3 ) (see Eq. (55)) in the cylindrical particle both for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as (11)

r (βm − βp) r λ1p = =− (1) (11) R ξ1 ξ3p D πE L , x3 ∈ 0, , r ∈ h0, Ri , ϕ ∈ 0, 2 2

u01p

u01p (r, ϕ)

u03p = u03p (x3 ) =

L (βm − βp) (3)

−1

, (85)

h i sinh λ(33) x , 3 p

ξ3 D πE L , x3 ∈ 0, . r ∈ h0, Ri , ϕ ∈ 0, 2 2

6.3.2.

(86)

Cell Matrix

Intervals r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i. The radial displacement u01m = u01m (r, ϕ) (see Eq. (58)) and the axial displacement u03m = u03m (r, x3) (see Eq. (59)) in the cell matrix have the forms 2

u01m = u01m (r, ϕ) = −

r (βm − βp) X (1)

ξ1

1 (11)

(11)

i=1 ξ2+im ξ4+im D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , 2 2

r λ(11) im −1 R

, (87)

h i r λ(11) 2m (33) sinh λ x , 3 p (3) R ξ3 D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, . (88) 2 2

u03m = u03m (r, x3) =

L (βm − βp )

88

Ladislav Ceniga

Intervals r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i. The radial displacement u01m = u01m (r, ϕ, x3) (see Eq. (61)) and the axial displacement u03m = u03m (x3 ) (see Eq. (56)) in the cell matrix are derived as (11)

r (βm − βp) r λ1p = =− (1) (11) R ξ1 ξ3p D πE L d , x3 ∈ , , r ∈ h0, Ri , ϕ ∈ 0, 2 2 2 u01m

u01m (r, ϕ, x3)

−1

(33)

× e−λm

[x3 −(L/2)]

,

(89)

" (33) # (33) λ m x3 −λm x3 L (β − β ) e e m p u03m = u03m (x3 ) = + , (3) (3) 2 ξ1 ξ2 D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , . 2 2 2

(90)

Intervals r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i. The radial displacement u01m = u01m (r, ϕ, x3) (see Eq. (62)) and the axial displacement u03m = u03m (r, x3) (see Eq. (60)) in the cell matrix have the forms 2

u01m = u01m (r, ϕ, x3) = − (33)

e−λm

[x3 −(L/2)]

r (βm − βp) X (1)

ξ1

i=1

1 (11)

(11)

ξ2+im ξ4+im

r λ(11) im −1 R

,

πE r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 2 D

L d , 2 2

,

(91)

" (33) # (33) λ m x3 −λm x3 λ(11) L (β − β ) e e r 2m m p u03m = u03m (r, x3) = + , (3) (3) 2 R ξ1 ξ2 D πE L d r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ , . (92) 2 2 2

Analytical Model of Thermal Stresses ...

7. 7.1.

89

Thermal Strains and Stresses Cylindrical Particle

With regard to Eqs. (3)–(7), (85), (86), the thermal strains in the cylindrical particle for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as (11) (βm − βp) λ1p r λ(11) 1p −1 , (1) (11) R ξ1 ξ3p D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , 2 2

ε011p = ε11p (r, ϕ) = −

(93)

(11)

(βm − βp ) r λ1p −1 , (1) (11) R ξ1 ξ3p D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , 2 2

ε022p = ε22p (r, ϕ) = −

(33)

ε033p = ε33p (x3 ) =

L λp

(βm − βp ) (3)

ξ3

πE , x3 ∈ r ∈ h0, Ri , ϕ ∈ 0, 2 D

(94)

h i cosh λ(33) x 3 , p

L 0, , 2

# " (1) λ(11) −1 β − β r 1p ∂ξ m p 1 ε012p = ε021p (r, ϕ) = , h i2 ∂ϕ R (11) (1) ξ3p ξ1 D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , 2 2

(95)

(96)

where ε013 = ε031 = 0 due to u01p = u01p (r, ϕ) 6= f (x3 ), u03p = u03p (x3 ) 6= f (r) (see Eqs. (7), (85), (86)). With regard to Eqs. (17)–(21), (85), (86), the thermal stresses in the cylindrical particle for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i have the forms (

) (11) (33) h i 1 “ r ”λ1p −1 Lc2p λp (33) = (r, ϕ, x3 ) = − (βm − βp ) + cosh λp x3 , (1) (3) R ξ1 ξ3 fi fl D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , (97) 2 2 0 σ11p

0 σ11p

90

Ladislav Ceniga 0 0 σ22p = σ22p (r, ϕ, x3) = ) ( (11) (33) h r λ(11) i ξ7p Lc2pλp 1p −1 cosh λ(33) + , − (βm − βp) p x3 (1) (11) R (3) ξ1 ξ3p ξ3 D πE L , x3 ∈ 0, r ∈ h0, Ri , ϕ ∈ 0, , (98) 2 2

0 0 σ33p = σ33p (r, ϕ, x3) = ) ( (11) (33) r λ(11) h i ξ9p L (c1p + c2p ) λp 1p −1 (33) cosh λp x3 , + − (βm − βp ) (1) (11) R (3) ξ1 ξ3p ξ3 D πE L , x3 ∈ 0, , r ∈ h0, Ri , ϕ ∈ 0, 2 2 (99)

" # (1) λ(11) −1 ∂ξ β − β r 1p m p 0 0 1 σ12p = σ21p (r, ϕ) = , h i2 (11) (1) ∂ϕ R s44p ξ3p ξ1 D πE L , x3 ∈ 0, , (100) r ∈ h0, Ri , ϕ ∈ 0, 2 2

0 0 = σ31 = 0 due to u01p = u01p (r, ϕ) 6= f (x3 ), u03p = u03p (x3 ) 6= where σ13 (11)

(11)

f (r) (see Eqs. (21), (85), (86)). The coefficients ξ7p , ξ9p are derived as h i (11) (11) ξ6+iq = c1q + c2q 1 − λiq , i = 1, 2, q = p, m,

(101)

h i (11) (11) ξ8+iq = −c2q 1 + λiq , i = 1, 2, q = p, m.

(102)

Analytical Model of Thermal Stresses ...

7.2.

91

Cell Matrix

7.2.1.

Intervals r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i

With regard to Eqs. (3)–(7), (87), (88), the thermal strains in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i have the forms ε011m = ε011m (r, ϕ) = −

2 βm − βp X (1) ξ1

(11)

λim

im

(11) (11) i=1 ξ2+im ξ4+im

D πE L , x3 ∈ 0, , r ∈ hR, rci , ϕ ∈ 0, 2 2 ε022m

=

ε022m (r, ϕ)

=−

2 βm − βp X (1)

ξ1

1 (11)

R

, (103)

(11)

ξ ξ 2+im 4+im D πE L , x3 ∈ 0, , r ∈ hR, rci , ϕ ∈ 0, 2 2 i=1

r λ(11) −1

r λ(11) im −1 R

, (104)

(33)

h i r λ(11) 2m (33) cosh λ x , 3 p (3) R ξ3 D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, . (105) 2 2

ε033m = ε033m (r, x3) =

L (βm − βp ) λp

ε012m = ε021m (r, ϕ) = (βm − βp ) " # (11) 2 (1) r λ(11) X 1 im −1 (11) ∂ξ1 (1) ∂ξ4+im + ξ1 × , h i2 ξ4+im (11) (1) (11) ∂ϕ ∂ϕ R i=1 ξ2+im ξ1 ξ4+im D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , (106) 2 2 (11)

h i r λ(11) 2m −1 (33) , sinh λ x 3 p (3) R R ξ3 D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , (107) 2 2

ε013m = ε031m (r, x3) =

L (βm − βp ) λ2m

92

Ladislav Ceniga

where the formula for the shear strain ε013 = ε031 given by Eq. (7) is transformed to the form ε013 = ε031 = ∂u03m /∂r due to u01m = u01m (r, ϕ) 6= f (x3 ) (see Eqs. (87), (88)). With regard to Eqs. (17)–(21), (87), (88), the thermal stresses in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i have the forms 0 0 σ11m = σ11m (r, ϕ) = − (βm − βp ) ) ( (11) 2 (33) h i r λ(11) 2m 1 X 1 r λim −1 L c2m λp (33) , × + cosh λp x3 (1) (11) (3) R ξ1 i=1 ξ4+im R ξ3 D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , (108) 2 2

0 0 σ22m = σ22m (r, ϕ) = − (βm − βp ) ( ) (11) 2 (33) h i r λ(11) r λ(11) ξ6+im 1 X L c2m λp im −1 2m × + cosh λ(33) x3 , p (1) (11) (3) (11) R ξ1 i=1 ξ2+im ξ4+im R ξ3 D πE L , x3 ∈ 0, , (109) r ∈ hR, rci , ϕ ∈ 0, 2 2

0 0 σ33m = σ33m (r, ϕ) = − (βm − βp ) × ( ) (11) 2 i “ r ”λ(11) “ r ”λ(11) −1 L (c + c ) λ(33) h ξ8+im 1 X 2m im 1m 2m p (33) cosh λp x3 + , (1) (11) (11) (3) R ξ1 i=1 ξ2+im ξ4+im R ξ3 fi fl D πE L r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ 0, , (110) 2 2

0 0 σ12m = σ21m (r, ϕ) =

×

2 X

1

(βm − βp) s44m "

(1) (11) ∂ξ1 ξ4+im

(11) (1) ∂ξ4+im ξ1

+ h i ∂ϕ (11) (1) (11) 2 ξ2+im ξ1 ξ4+im D πE L r ∈ hR, rci , ϕ ∈ 0, , x3 ∈ 0, , 2 2 i=1

∂ϕ

#

r λ(11) im −1 R

,

(111)

Analytical Model of Thermal Stresses ...

93

(11)

h i r λ(11) 2m −1 (33) sinh λ , = x = 3 p (3) R R s44m ξ3 D πE L , x3 ∈ 0, r ∈ hR, rci , ϕ ∈ 0, , (112) 2 2

0 σ13m

0 σ31m (r, x3)

(11)

L (βm − βp ) λ2m

(11)

where the coefficients ξ6+im , ξ8+im (i = 1,2) are given by Eqs. (102), (103), and 0 0 the formula for the shear stress σ13 = σ31 given by Eq. (21) is transformed to 0 0 0 the form σ13 = σ31 = (1/s44m) (∂u3m /∂r) due to u01m = u01m (r, ϕ) 6= f (x3 ) (see Eqs. (87), (88)). 7.2.2.

Intervals r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i

With regard to Eqs. (3)–(7), (89), (90), the thermal strains in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as (11) (33) (βm − βp) λ1p “ r ”λ(11) 1p −1 × e−λm [x3 −(L/2)] , (1) (11) R ξ1 ξ3p fi fl D πE L d , x3 ∈ , r ∈ h0, Ri , ϕ ∈ 0, , (113) 2 2 2

ε011m = ε011m (r, ϕ, x3 ) = −

(11) (33) βm − βp r λ1p −1 × e−λm [x3 −(L/2)], = = − (1) (11) R ξ1 ξ3p D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , (114) 2 2 2

ε022m

ε022m (r, ϕ, x3)

" (33) # (33) (33) λ m x3 −λm x3 e L (β − β ) λ e m m p ε033m = ε033m (x3 ) = − , (3) (3) 2 ξ1 ξ2 D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , . (115) 2 2 2 " (1) # “ r ”λ(11) −1 (33) ∂ξ1 βm − βp 1p = (r, ϕ, x3 ) = × e−λm [x3 −(L/2)] , h i2 (11) (1) ∂ϕ R ξ3p ξ1 fi fl D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , (116) 2 2 2 ε012m

ε021m

94

Ladislav Ceniga

(33)

ε013m = ε031m (r, ϕ, x3) =

r (βm − βp ) λm (1) (11) ξ1 ξ3p

r λ(11) 1p −1 R

D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , 2 2 2

(33)

× e−λm

[x3 −(L/2)]

,

(117)

where the formula for the shear strain ε013 = ε031 given by Eq. (7) is transformed to the form ε013 = ε031 = ∂u01m /∂x3 due to u03m = u03m (x3 ) 6= f (r) (see Eqs. (89), (90)). With regard to Eqs. (17)–(21), (89), (90), the thermal stresses in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i have the forms 0 0 σ11m = σ11m (r, ϕ, x3 ) = − (βm − βp ) ( " (33) #) (33) (11) (33) “ ” (33) 1 r λ1p −1 Lc2m λm eλm x3 e−λm x3 −λm [x3 −(L/2)] × ×e + − , (1) (3) (3) R 2 ξ1 ξ1 ξ2 fi fl D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , (118) 2 2 0 0 σ22m = σ22m (r, ϕ, x3 ) = − (βm − βp) #) " (33) ( (33) (11) (33) “ r ”λ(11) (33) ξ7p e−λm x3 Lc2m λm eλm x3 1p −1 −λm [x3 −(L/2)] − , × e + × (1) (11) (3) (3) R 2 ξ1 ξ3p ξ1 ξ2 fi fl D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , (119) 2 2

0 σ33m

=

0 σ33m

(r, ϕ, x3 ) = − (βm − βp )

(

(11)

ξ9p (1) ξ1

(11) ξ3p

“ r ”λ(11) 1p −1 R

(33)

× e−λm

[x3 −(L/2)]

" (33) #) (33) (33) L (c1m + c2m ) λm eλm x3 e−λm x3 − , + (3) (3) 2 ξ1 ξ2 fl fi D πE L r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ 0, , 2 2 βm − βp = (r, ϕ, x3 ) = h i2 (11) (1) s44m ξ3p ξ1 fi fl D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , 2 2 2

0 σ12m

0 σ21m

"

(1)

∂ξ1 ∂ϕ

#

(120) “ r ”λ(11) 1p −1 R

(33)

× e−λm

[x3 −(L/2)]

,

(121)

Analytical Model of Thermal Stresses ...

(33)

0 0 σ13m = σ31m (r, ϕ, x3 ) =

r (βm − βp ) λm (1) s44m ξ1

(11) ξ3p

fi fl D πE L d r ∈ h0, Ri , ϕ ∈ 0, , x3 ∈ , , 2 2 2 (11)

“ r ”λ(11) −1 1p

R

95

(33)

× e−λm

[x3 −(L/2)]

,

(122)

(11)

where the coefficients ξ6+im , ξ8+im (i = 1,2) are given by Eqs. (102), (103), and the formula for the shear stress ε013 = ε031 given by Eq. (21) is transformed to 0 0 the form σ13 = σ31 = (1/s44m) ∂u01m /∂x3 due to u03m = u03m (x3 ) 6= f (r) (see Eqs. (89), (90)). 7.2.3.

Intervals r ∈ hR, rci, ϕ ∈ h0, π/2i, x3 ∈ hL/2, d/2i

With regard to Eqs. (3)–(7), (91), (92), the thermal strains in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i are derived as 2

ε011m = ε011m (r, ϕ, x3 ) = −

(11)

(βm − βp ) X (1) ξ1

λim

(11) i=1 ξ2+im

ε022m = ε022m (r, ϕ, x3 ) = −

2 βm − βp X (1) ξ1

D πE , x3 ∈ r ∈ hR, rc i , ϕ ∈ 0, 2

1

L d , 2 2

fl

R

(33)

× e−λm

[x3 −(L/2)]

,

(123)

(11) i=1 ξ2+im

fi

im

(11) ξ4+im

fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , , 2 2 2

“ r ”λ(11) −1

(11) ξ4+im

,

“ r ”λ(11) im −1 R

(33)

× e−λm

[x3 −(L/2)]

,

(124)

" (33) # (33) (11) (33) L (βm − βp ) λm eλm x3 e−λm x3 “ r ”λ2m = (r, x3 ) = − , (3) (3) 2 R ξ1 ξ2 fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , . (125) 2 2 2 ε033m

ε033m

ε012m = ε021m (r, ϕ, x3 ) = (βm − βp ) 2 3 (11) (1) 2 “ ” (11) X 1 (11) ∂ξ1 (1) ∂ξ4+im 5 r λim −1 −λ(33) 4 × + ξ1 × e m [x3 −(L/2)] , h i2 ξ4+im (11) (1) (11) ∂ϕ ∂ϕ R i=1 ξ ξ ξ 2+im

1

4+im

fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , , 2 2 2

(126)

96

Ladislav Ceniga

( 2 (33) “ r ”λ(11) (33) βm − βp X r λm im −1 × e−λm [x3 −(L/2)] = (r, ϕ, x3 ) = (1) (11) (11) 2 R i=1 ξ1 ξ2+im ξ4+im # ) " (33) (33) (11) (11) e−λm x3 “ r ”λ2m −1 L λ2m eλm x3 + + , (3) (3) 2R R ξ1 ξ2 fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , . (127) 2 2 2

ε013m

ε031m

With regard to Eqs. (17)–(21), (91), (92), the thermal stresses in the cell matrix for r ∈ h0, Ri, ϕ ∈ h0, π/2i, x3 ∈ h0, L/2i have the forms 0 σ11m

=

0 σ11m

(r, ϕ) = − (βm − βp )

(33)

L c2m λm + 2

"

(33)

eλm

x3

(33)

e−λm

( x3

2 1 X

(1) ξ1 i=1

#

1

“ r ”λ(11) 2m

− (3) (3) R ξ1 ξ2 fi fl D πE L r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ 0, , 2 2 0 σ22m

=

0 σ22m

(r, ϕ) = − (βm − βp)

(33)

L c2m λm + 2

"

(33)

eλm

x3

(33)

e−λm

( x3

2 1 X

(1) ξ1 i=1

#

0 σ33m

=

0 σ33m

(r, ϕ) = − (βm − βp)

(

2 1 X

(1) ξ1 i=1

(33)

e−λm

[x3 −(L/2)]

(128) (11)

(11) ξ2+im 2m

R

,

ξ6+im

“ r ”λ(11)

− (3) (3) R ξ1 ξ2 fi fl D πE L r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ 0, , 2 2

)

“ r ”λ(11) −1 im

(11) ξ4+im

)

(11) ξ4+im

“ r ”λ(11) −1 im

R

(33)

e−λm

[x3 −(L/2)]

, (129)

(11) ξ8+im (11) (11) ξ2+im ξ4+im

“ r ”λ(11) −1 im

R

" (33) # ) (33) (11) (33) L (c1m + c2m ) λm eλm x3 e−λm x3 “ r ”λ2m + − , (3) (3) 2 R ξ1 ξ2 fi fl D πE L r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ 0, , 2 2

(33)

e−λm

[x3 −(L/2)]

(130)

βm − βp s44m " # (11) (1) “ r ”λ(11) −1 (33) im (11) ∂ξ1 (1) ∂ξ4+im × e−λm [x3 −(L/2)] , + ξ1 i2 ξ4+im ∂ϕ ∂ϕ R

0 0 = σ21m (r, ϕ, x3 ) = σ12m

×

2 X

(11) i=1 ξ2+im

1 h

(1) ξ1

(11)

ξ4+im fi fl D πE L d r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , , 2 2 2

(131)

Analytical Model of Thermal Stresses ...

97

( 2 (33) “ r ”λ(11) −1 (33) βm − βp X r λm im × e−λm [x3 −(L/2)] = (r, ϕ, x3 ) = (1) (11) (11) 2s44m R i=1 ξ1 ξ2+im ξ4+im # ) " (33) (33) (11) (11) “ L λ2m eλm x3 r ”λ2m −1 e−λm x3 + , + (3) (3) 2R R ξ1 ξ2 fi fl D πE L d , r ∈ hR, rc i , ϕ ∈ 0, , x3 ∈ , (132) 2 2 2

0 σ13m

0 σ31m

(11)

(11)

where the coefficients ξ6+im , ξ8+im (i = 1,2) are given by Eqs. (102), (103).

8.

Application to SiC-Si3N4 Ceramics

This section presents illustrative examples of an application of this analytical model of thermal stresses in a two-component material with cylindrical particles to a real two-component material. These illustrative examples are numerically performed for the SiC-Si3 N4 ceramics. Table 1 presents material parameters of the SiC particle and the Si3 N4 matrix of the SiC-Si3 N4 ceramics representing a two-component material where the SiC particles can exhibit spherical and cylindrical shapes [26]. The relaxation temperature Tr = 665◦ C is determined by the formula Tr = 0.35 Tm [26], where Tm = Tmm is melting temperature of the SiC-Si3 N4 ceramics. Table 1. Material parameters of the SiC-Si3 N4 ceramics [26]

Eq [GPa] µq αq [10−6 K−1 ] Tmq [◦ C]

Particle (q = p) SiC 360 0.19 4.15 2730

Matrix (q = m) Si3 N4 310 0.235 2.35 1900

As shown in Fig. 4, the dependences p1 −v and p3 −v (see Eqs. (1), (2), (79), (83)) for the radial stress p1 = p1 (ϕ, v) and the axial stress p3 = p3 (v) both acting at the SiC-Si3 N4 boundary exhibit decreasing courses for v ∈ (0, vpmax) (see Eq. (1)), where L = 2R = 6 µm, Tr = 665◦ C, Tf = 20◦ C. With regard

98

Ladislav Ceniga

Figure 4. The functions p1 = p1 (v) (see Eq. (133)) and p3 = p3 (v) of the volume fraction v ∈ (0, vpmaxi (see Eq. (1)) of the SiC cylindrical particle, where L = 2R = 6 µm, Tf = 20◦ C, Tr = 665◦ C. The radial stress p1 = p1 (ϕ, v) and the axial stress p3 = p3 (v) (see Eqs. (79), (83)) act at the SiCSi3 N4 boundary. to the interval ϕ ∈ h0, π/2i, the mean value p1 = p1 (v) of the function p1 = p1 (ϕ, v) is numerically determined by the following formula 2 p1 = π

Zπ/2 n X p1 (ϕ) dϕ ≈ p1 (i × ∆ϕ) ∆ϕ, 0

(133)

i=0

where n is a integral part of the real number π/ (2 ∆ϕ). With regard to an experience of the author, the angle step ∆ϕ = 0.01 − 0.1 [deg] is sufficient to be considered within the numerical determination of the mean vale. Other applications of the final formulae (see Sec. 6) can be easily performed by a reader. This numerical determination can be performed by a computer software using suitable programming techniques. With regard to programming techniques within a suitable programming language (e.g. Fortran, Pascal), a derivative of the function ψ = ψ (ϕ) regarding the variable ϕ (see Eqs. (96), (100), (106), (111), (116), (121), (126), (131)) can be numerically determined by the formula ∂ψ ψ (ϕ + ∆ϕ) − ψ (ϕ) ≈ , (134) ∂ϕ ∆ϕ (1)

(11)

where ψ = ξ1 , ξ4+im (see Eqs. (96), (100), (106), (111), (116), (121), (126),

Analytical Model of Thermal Stresses ...

99

(131)). The angle step ∆ϕ is required to be taken as small as possible. With regard to an experience of the author, the angle step ∆ϕ = 10−6 [deg] is sufficient to be considered within the numerical determination.

Conclusion Results of this chapter are as follows. The analytical model of thermal stresses in a multi-particle-matrix system with isotropic components is determined (see Secs. 2, 7). The analytical model results from fundamental equations of mechanics of an elastic solid continuum (see Sec. 3). The multi-particle-matrix system consists of isotropic cylindrical particles which are periodically distributed in an isotropic infinite matrix (see Fig. 1). The thermal stresses are a consequence of different thermal expansion coefficients of the isotropic matrix and isotropic particle (see Eq. (50)). The infinite matrix is imaginarily divided into identical cubic cells (see Fig. 1), and the thermal stresses are thus investigated within the cubic cell (see Sec. 2). Each cell contains a central cylindrical particle. This multi-particlematrix system represents a model system which is applicable to two-component materials of a precipitate-matrix type. The radius and the volume fraction of the cylindrical particles along with the cubic cell dimension represent microstructural parameters of the two-component material. The thermal stresses are then functions of these microstructural parameters. Numerical values for a real twocomponent material of the precipitate-matrix type (SiC-Si3 N4 ceramics) are obtained.

Acknowledgments This work was supported by the Slovak Grant Agency under the contract VEGA 2/0081/16, 2/0120/15, 2/0113/16 and by the Slovak Research and Development Agency under the contract APVV-0147-11.

References [1] Greisel, M.; J¨ager, J.; Moosburger-Will, J.; Sause, M.G.R.; Mueller, W.M.; Horn, S. Composites: Part A 2014, 66, 117-127.

100

Ladislav Ceniga

[2] Meijer, G.; Ellyin, F.; Xia, Z. Composites: Part B 2000, 31, 29–37. [3] We¸glewski, W.; Basista, M.; Manescu, A.; Chmielewski, M.; Pietrzak, K.; and Schubert, Th. Composites: Part B 2014, 67, 119-124. [4] Nabavi, S.M.; Ghajar, R. Int. J. Eng. Sci. 2010, 48, 1811-1823. [5] Lee, J.; Hwang, K.-Y. Int. J. Eng. Sci. 1996, 34, 901–922. [6] Tanigawa, Y.; Osako, M.K. Int. J. Eng. Sci. 1986, 24, 309–321. [7] Abedian, A.; Szyszkowski, W.; Yannacopoulos, S. Compos. Sci. Technol. 1999, 59, 41–54. [8] Ceniga, L. Analytical Model of Thermal Stresses in Composite Materials I; Nova Science Publishers: New York, US, 2008, pp 66–67, 136– 137. [9] Mizutani, T. J. Mater. Sci. 1996, 11, 483–494. [10] Li, Sh.; Sauer, R.A.; Wang, G. J. Appl. Mech. 2007, 74, 770–783. [11] Li, Sh.; Sauer, R.A.; Wang, G. J. Appl. Mech. 2007, 74, 784–797. [12] Kushch, V.I. Prikladnaja Mekhanika 1985, 21, 18-27. [13] Kushch, V.I. Int. Appl. Mech. 2004, 40, 893-899. [14] Kushch, V.I. Int. Appl. Mech. 2004, 40, 1042-1049. [15] Wu, Y.; Dong, Z. Mater. Sci. Eng. 1995, 203, 314–323. [16] Sangani, A.S.; Mo, G. J. Mech. Phys. Sol. 1997, 45, 2001–2031. [17] Bidulsk´y, R.; Bidulsk´a, J.; Grande, M.A. Arch. Metallur. Mater. 2013, 58, 365–370. [18] Kvaˇckaj, T.; Koˇcisko, R.; Bidulsk´y, R.; Bidulsk´a, J.; Bella, P.; Lupt´ak, M.; Kov´acˇ ov´a, A.; Bacso, J. Mater. Sci. For. 2014, 782, 379– 383. [19] Bidulsk´y, R.; Bidulsk´a, J.; De Oro, R.; Hryha, E.; Maccarini, M.; Forno, I.; Grande, M.A. Act. Phys. Polon. A 2015, 128, 647–650.

Analytical Model of Thermal Stresses ...

101

[20] Mura, T. Micromechanics of Defects in Solids; Martinus Nijhoff Publishers: Dordrecht, NL, 1987, pp 1–3. [21] Ceniga, L. Analytical Models of Thermal Stresses in Composite Materials IV; Nova Science Publishers: New York, US, 2015, pp 34–37. [22] Brdiˇcka, M.; Samek, L.; Sopko, B. Mechanics of Continuum; Academia: Prague, CZ, 2000, pp 78–83. ˇ ca´ k, F.; Jurica, V. Elasticity and Strength I; Technical [23] Trebuˇna, F.; Simˇ University: Koˇsice, SK, 2005, pp 57–63. ˇ ca´ k, F.; Jurica, V. Examples and Problems of Elasticity [24] Trebuˇna, F,;, Simˇ and Strength I; Technical University: Koˇsice, SK, 2002, pp 134–138. [25] Rektorys, K. Review of Applied Mathematics; SNTL: Prague, CZ, 1973, pp 253–267. ˇ [26] Skoˇcovsk´y, P.; Bok˚uvka, O.; Palˇcek, P. Materials Science; EDIS: Zilina, SK, 1996, pp 35–48.

In: Ceramic Materials Editor: Jacqueline Perez

ISBN: 978-1-63485-965-3 c 2017 Nova Science Publishers, Inc.

Chapter 4

A NALYTICAL M ODEL OF T HERMAL S TRESSES IN M ULTI -C OMPONENT P OROUS M ATERIALS Ladislav Ceniga∗ Institute of Materials Research, Slovak Academy of Sciences, Koˇsice, Slovak Republic

Abstract This chapter deals with analytical modelling of thermal stresses which originate during a cooling process of an elastic solid continuum. This continuum consists of an isotropic infinite matrix with isotropic spherical particles and spherical pores. The particles and pores are both periodically distributed in the infinite matrix which is imaginarily divided into identical cubic cells. Each cell contains either a central particle or a central pore. This porous multi-particle-matrix system represents a model system which is applicable to porous two-component materials of a precipitatematrix type characterized by microstructural parameters, i.e. the cubic cell dimension; radii and volume fractions of both the particles and of the pores. The thermal stresses are a consequence of different thermal expansion coefficients of the isotropic matrix and isotropic particle. Resulting from fundamental equations of mechanics of an elastic solid continuum, the thermal stresses are determined within this cell, and thus represent ∗ E-mail addresses: [email protected], la[email protected], [email protected], [email protected]

104

Ladislav Ceniga functions of these microstructural parameters. Finally, numerical values for a real porous two-component material of the precipitate-matrix type are obtained.

PACS: 46.25.Cc, 46.25.Hf, 46.70.Lk Keywords: analytical modelling, thermal stress, composite material

1.

Introduction

Thermal stresses which originate as a consequence of different thermal expansion coefficients of components of multi-component materials represent an important phenomenon in multi-component materials. These stresses are usually investigated by computational and experimental methods [1]–[7] are still of interest to materials scientists and engineers. This chapter represents continuation of the author’s book [8] which deals with the analytical modelling of the thermal stresses in two-component materials of a precipitate-matrix type with isotropic precipitates (isotropic particles) and an isotropic matrix. In contrast to [8], the analytical model of the thermal stresses in this chapter is determined for a porous isotropic matrix with spherical pores. The thermal stresses originate during a cooling process at the temperature T ∈ hTf , Tr i, where Tf and Tr [9] are final and relaxation temperature of the cooling process, respectively. As defined in [9], the relaxation temperature Tr is such temperature below that the stress relaxation as a consequence of thermalactivated processes does not occur in a material. The relaxation temperature is defined approximately by the relationship Tr = (0.35 − 0.4) × Tm [9] and exactly by an experiment, where Tm is a melting point of a two-component material. If precipitates are formed from a liquid matrix of the two-component material, then the melting point Tm represents minimum of the set {Tmp , Tmm}, where Tmp and Tmm are melting points of the precipitate (particle) and the matrix [9], respectively. If the precipitates are formed from a solid matrix, then Tm represents a melting point of the two-component material [9]. The thermal stresses which originate at the temperature T ∈ hTf , Tr i are thus a consequence of the condition βm − βp 6= 0. The coefficient βq is derived

Analytical Model of Thermal Stresses in Multi-Component ... as βq =

ZTr

αq dT, q = p, m,

105

(1)

T

where αq is a thermal expansion coefficient of the isotropic spherical particle (q = p) and the isotropic matrix (q = m). Within the analytical modelling presented in this chapter, this cooling process is characterized by a homogeneous temperature change. Using the spherical coordinates (r, ϕ, ν), the homogeneous temperature change is then characterized by the condition ∂T /∂r = ∂T /∂ϕ = ∂T /∂ν = 0. With regard to materials engineering, experimental results are usually compared with the Selsing’s analytical model [10]–[23] which determines thermal stresses in a one-particle-matrix system with an isotropic spherical particle embedded in an isotropic infinite matrix. On the one hand, the Selsing’s analytical model does not consider neither the inter-particle distance d nor the particle volume fraction vp = Vp/Vm , where Vp and Vm is volume of the particle and the matrix, respectively, and then d → ∞, Vm → ∞, vp = 0 for the Selsing’s analytical model. On the other hand, in spite of this fact, the Selsing’s analytical model which was determined in 1961 is still used by materials scientists at present [16]–[23]. As a continuation of the Selsing’s analytical model, Mizutani [24] determined an analytical model for the thermal stresses for a multi-particle-matrix system with isotropic components. The Mizutani’s analytical model considers an imaginary division of the isotropic infinite matrix into identical spherical cells with a central isotropic spherical particle with the radius Rp. The thermal stresses which are investigated within this cell are then functions of the microstructural parameters d, vp , Rp. On the one hand, the influence of the thermal stresses of all cells on the thermal stresses in a certain cell as well as the influence of the thermal stresses of neighbouring cells on the thermal stresses in a certain cell can be hardly expressed by an exact mathematical solution. On the other hand, the analytical model of the thermal stresses which is determined within a cell is generally considered to represent more than sufficient mathematical solution for materials scientists and engineers. Using final mathematical formulae for the thermal stresses, materials scientists and engineers can then determine numerical values of the thermal stresses for a real two-component material. As presented in [24]–[31], this ’cell approach’ is used within mathematical

106

Ladislav Ceniga

procedures applied to analytical modelling of periodic model systems with an infinite matrix. The infinite matrix of the periodic model systems can be then imaginarily divided into e.g. spherical cells [24]–[26], cubic cells [27, 28], however, in contrast to cubic cells, two spherical cells are mutually connected in one point [24]–[26]. The matrix between two spherical cells is not considered, and accordingly, cubic cells which are considered in this chapter are preferable. Finally, as presented in [24, 32], to obtain analytical solutions, real twocomponent materials with finite dimensions and with aperiodically distributed particles (precipitates) are then replaced by a model system which consists of an infinite matrix with periodically distributed particles of a defined shape (e.g. spherical particles). Additionally, the case when an infinite matrix is considered within the analytical modelling is of particular interest for the mathematical simplicity of analytical solutions. As analysed in [32], such analytical solutions are assumed to exhibit sufficient accuracy due to the size of material components (e.g. precipitates) which is relatively small in comparison with the size of macroscopic material samples, macroscopic structural elements, etc.

2.

Cell Model

With regard to the analytical modelling, real porous two-component materials with isotropic components of finite dimensions are replaced by an infinite porous multi-particle-matrix system (see Fig. 1). The porous multi-particlematrix system represents a model system. The model system is represented by isotropic spherical particles which are periodically distributed in a porous isotropic infinite matrix with periodically distributed spherical pores. The porous infinite matrix is imaginarily divided into identical cubic cells with a central spherical particle and into identical cubic cells with a central spherical pore. The cubic cell represents such part of the porous multi-particle-matrix system which is related to one spherical particle (see the cubic cell 1234 in Fig. 1) and to one spherical pore (see the cubic cell 2567 in Fig. 1). Additionally, as presented in Fig. 1, one cubic cell with the central spherical pore (the cube 2567) is related to 26 cubic cells with the central spherical particle (see the cube 48910 in Fig. 1). The inter-particle distance d, the particle radius Rp, the pore radius Rv (pore=void), the particle volume fraction vp and the pore volume fraction vv , which represent parameters of the cubic cells with the spherical particle and with

Analytical Model of Thermal Stresses in Multi-Component ...

107

the spherical pore, are microstructural parameters of porous two-component materials of a precipitate-matrix type, where vp and vv have the forms 26Vp 104π = vp = 27Vc 81 vv =

Vv 4π = 27Vc 81

Rp d

Rv d

3

3

∈ (0, vpmaxi , vpmax =

∈ (0, vf maxi , vpmax =

vp = 26 vv

Rp Rv

3

13π , 81

π , 162

,

(2)

(3) (4)

where Vp = 4πR3p/3, Vv = 4πR3v /3 and Vc = d3 is volume of the spherical particle, the spherical pore and the cubic matrix, respectively. The maximum values vpmax and vf max result from the condition Rp = d/2 and Rv = d/2, respectively. In case of a real porous two-component material of the precipitate-matrix type, these microstructural parameters are obtained by experimental techniques. The thermal stresses are investigated within the cubic cell with the spherical particle and within the cubic cell with the pore, and thus represent functions of these microstructural parameters. Additionally, the surface of the cubic cell defines positions for which one of boundary conditions for the infinite matrix is determined (see Eq. (57)). The thermal stresses, as functions of the spherical coordinates [r, ϕ, ν], are derived in the Cartesian system (P x01 x02 x03 ) (see Fig. 2). The spherical coordinates (r, ϕ, ν) are used due to the spherical shapes of the particles and of the pores of the porous multi-particle-matrix system. The axes x 01 and x02 , x03 represent radial and tangential directions, respectively, and r = OP , where O is a centre of the spherical particle. Due to the symmetry of the cubic cell as well as due to the isotropy of the porous multi-particle-matrix system, the thermal stresses are sufficient to be investigated within one eighth of the cubic cell, i.e. for ϕ, ν ∈ h0, π/2i, where r ∈ h0, Rpi for the spherical particle and r ∈ hRp, rci for the cell matrix, respectively. ∗ The distance r∗c = rc (ϕ, ν) = OC3 for ν ∈ h0, ν ) and rc = rc (ϕ, ν) = OC1 for ν ∈ hν , π/2i (see Fig. 3) has the form [8] Rp fc rc = d fc = 3

104π 3vp

1/3

Rv fc = 3

4π 3vv

1/3

.

(5)

108

Ladislav Ceniga

Figure 1. The porous multi-particle-matrix system imaginarily divided into identical cubic cells with a central spherical particle (see the cubic cell 1234) and with a central spherical pore (see the cubic cell 2567) both in the point O of the Cartesian system (Ox1 x2 x3 ), where a dimension of the cubic cell is identical to the inter-particle distance d; Rp and Rv are radii of the particle and the pore, respectively. One cubic cell with the central spherical pore is related to 26 cubic cells with the central spherical particle (see the cube 2567). The function fc = fc (ϕ, ν) along with the coefficient cϕ and the angle ν ∗ (see Fig. 3) are derived as q 1 + c2ϕ fc = , ν ∈ (0, ν ∗ i , (6) 2 [cϕ cos (ν ∗ − ν) + sin (ν ∗ − ν)] D 1 πE , ν ∈ ν∗, , 2cϕ sin ν 2 D πE cϕ = cos ϕ, ϕ ∈ 0, , 4 π πE cϕ = sin ϕ, ϕ ∈ , , 4 2 1 ν ∗ = arctan . cϕ

fc =

(7) (8) (9) (10)

Analytical Model of Thermal Stresses in Multi-Component ...

109

Figure 2. The axes x01 = xr = OP and x02 = xϕ k x1 x2 , x03 = xν defining radial and tangential directions regarding the Cartesian system (P x01 x02 x03 ), respectively, and the arbitrary point P with a position determined by the spherical coordinates [r, ϕ, ν] regarding the Cartesian system (Ox1 x2 x3 ) (see Fig. 1). O is a centre of the spherical particle, and x02 , x03 are tangents to a surface of a sphere with the radius r = OP representing length of the abscissa |OP |.

The boundary condition for a surface of the cell with the spherical particle (see the cell 1234) given by Eq. (57), along with the formulae for the thermal stresses given by (24)–(27), (63) and with the boundary conditions given by Eqs. (54), Eq. (56) result in a dependence of the thermal stresses in the spherical particle and the cell matrix on the microstructural parameters Rp , d or Rp, vp (see Eqs. (2)).

3.

Fundamental Equations

The analytical modelling presented in this chapter results from fundamental equations of solid continuum mechanics. These fundamental equations are represented by the Cauchy’s equations, the equilibrium equations and the Hooke’s

110

Ladislav Ceniga

Figure 3. The points C3 (rc = OC3 ) and C1 (rc = OC1 ) as points of intersection of the axis x01 , representing a radial direction, with the surfaces 3657 and 1456 of one eighth of the cubic cell (see Fig. 1) for ν ∈ h0, ν ∗ ) and ν ∈ hν ∗ , π/2i, respectively. law for an isotropic elastic solid continuum. The Cauchy’s equations and the equilibrium equations for the infinitesimal spherical cap in the arbitrary point P with a position determined by the spherical coordinates [r, ϕ, ν] (see Fig. 4) regarding the Cartesian system (Ox1 x2 x3 ) are determined for the Cartesian system (P x01 x02 x03 ) (see Fig. 2). The Cauchy’s equations which represent geometric equations define relationships between strains and displacements of an infinitesimal part of a solid continuum. The equilibrium equations which are related to the axes x01 , x02 , x03 (see Fig. 2) are based on a condition of the equilibrium of forces which act on sides of this infinitesimal part. The infinitesimal spherical cap in the arbitrary point P (see Fig. 4) is described by the dimensions dr, rdϕ,rdν along the axes x01 , x02 , x03 of the Cartesian system (P x01 x02 x03 ), respectively. The axis x01 represents a normal of the surfaces Sr and Sr+dr with the surface area Ar = r 2 dϕ dν and Ar+dr = (r + dr)2 dϕ dν at the radii r and r + dr, respectively. As analysed in [33], this infinitesimal spherical cap exhibits the radial displacement u01 along the axis x01 . Accordingly, the Cauchy’s equations for the radial strain ε011 along the axis x01 , tangential strain ε0ii and the shear strains ε01i = ε0i1 along the axis x0i

Analytical Model of Thermal Stresses in Multi-Component ...

111

Figure 4. The infinitesimal spherical cap at the point P (see Fig. 2) with the surfaces Sr = A1 B1 C1 D1 and Sr+dr = A2 B2 C2 D2 at the radii r = OP and r + dr, respectively. Dimensions of the infinitesimal spherical cap are as follows: |A1 A2 | = |B1 B2 | = |C1 C2 | = |D1 D2 | = dr, |A1 D1 | = |B1 C1 | = r × dϕ, |A1 B1 | = |C1 D1 | = r × dν, |A2 D2 | = |B2 C2 | = (r + dr) × dϕ, |A2 B2 | = |C2 D2 | = (r + dr) × dν. (i = 2,3) are derived as [33] ∂u01 , ∂r u0 ε022 = ε033 = 1 , r 1 ∂u01 ε012 = ε021 = , r ∂ϕ ε011 =

(11) (12) (13)

1 ∂u01 , (14) r ∂ν 0 acting Consequently, the equilibrium equations for the radial stress σ11 0 0 0 0 acting along the axis x1 , tangential stresses σii and the shear stresses σ1i = σi1 along the axis x0i (i = 2,3) have the forms [33] ε013 = ε031 =

0 0 0 2σ11 − σ22 − σ33 +r

0 0 ∂σ11 ∂σ 0 ∂σ13 + 12 + = 0, ∂r ∂ϕ ∂ν

(15)

112

Ladislav Ceniga 0 ∂σ22 ∂σ 0 0 + 3σ12 + r 12 = 0, ∂ϕ ∂r

(16)

0 ∂σ33 ∂σ 0 0 + 3σ13 + r 13 = 0. (17) ∂ν ∂r With regard to the shear strain ε023 = ε032 ∝ [(∂u02 /∂ν) + (∂u03 /∂ϕ)] in the Cartesian system (P x01 x02 x03 ) (see Fig. 2) [34], we get ε023 = 0 due to u02 = 0, u03 = 0, where u02 and u03 represent displacements of the infinitesimal spherical cap along the axes x02 and x03 (see Fig. 2), respectively, i.e. along tangential directions. Similarly, with regard to the Hooke’s law for an isotropic elastic 0 (see Eq. (23)). [34], we get σ 0 = 0. solid continuum, i.e. ε023 = s44 σ23 23 0 0 Finally, with regard to ε23 = 0, σ23 = 0, the Hooke’s law for an isotropic elastic solid continuum is derived as [34]–[36] 0 0 0 ε011 = s11 σ11 + s12 σ22 + σ33 , (18) 0 0 0 + s11 σ22 , (19) ε022 = s12 σ11 + σ33 0 0 0 + s11 σ33 , (20) ε033 = s12 σ11 + σ22 0 ε013 = s44 σ13 ,

(21)

0 ε012 = s44 σ12 .

(22)

The elastic moduli s11 , s12 , s44 which represent functions of the Young’s modulus E and Poisson’s ratio µ have the forms [34]–[36] s11 =

1 µ 2 (1 + µ) , s12 = − , s44 = , E E E

(23)

The Young’ modulus E and the Poisson’s ratio µ are related to the spherical particle (q = p) and the cell matrix (q = m). Consequently, the transformations E → Eq , µ → µq (i, j = 1, . . . , 6; q = p,m) are required to be considered.

4.

Mathematical Procedures

Let the Cauchy’s equations (see Eqs. (11)–(14)) be substituted to the Hooke’s law for an isotropic solid elastic continuum (see Eqs. (18)–(23)). Con0 sequently, the radial stress σ11 acting along the axis x01 (see Fig. 2), the tangen0 0 acting along the tial stress σ22 acting along the axis x02 , the tangential stress σ33

Analytical Model of Thermal Stresses in Multi-Component ...

113

0 0 axis x03 , the shear stress σ12 acting along the axis x02 and the shear stress σ13 0 acting along the axis x3 have the forms 0 σ11 = (c1 + c2 )

∂u01 u0 − 2c2 1 , ∂r r

∂u01 u0 + c1 1 , ∂r r 0 1 ∂u1 = , s44 r ∂ϕ

(24)

0 0 σ22 = σ33 = −c2

(25)

0 σ12

(26)

0 σ13 =

∂u01 , s44 r ∂ν 1

(27)

0 = σ 0 (i, j = 1,2,3) [34]–[36], and the condition σ 0 = σ 0 results where σij 22 33 ji from the condition ε022 = ε033 (see Eqs. (12), (19), (20)). The coefficients c1 , c2 , c3 are derived as (see Eq. (23))

s11 E = , s11 (s11 + s12 ) − 2s212 (1 + µ) (1 − 2µ) s12 c1 µE s44 c1 + 2 c2 = =− , c3 = = −4 (1 − µ) . (28) s11 (1 + µ) (1 − 2µ) s44 c2 − 1 c1 =

In case of an isotropic elastic solid continuum, we get µ = 0.25 [34]. In case of a real isotropic material, we get µ < 0.5 [9], and then c3 < 0. The coefficient c3 is considered within the following mathematical procedures. Additionally, with regard to Eqs. (11)–(14), (24)–(27), the elastic energy density w [34]–[36] has the form w=

3 X

0 ε0ij σij =

i,j=1

+

1 s44

r2

"„

∂u01 ∂ϕ

∂u01 ∂r «2 #

1 (c1 + c2 ) 2

«2

+

„

∂u01 ∂ν

„

«2

−

` ´2 c1 u01 2c1 u01 ∂u01 + r ∂r r2

,

(29)

0 where ε023 = 0, σ23 = 0 (see Sec. 3). Let the equations (24)–(27) be substituted to Eq. (15) as well as to the sum [∂Eq.(16)/∂ϕ] + [∂Eq.(18)/∂ν]. The equilibrium equations (15)–(17) are thus transformed to the forms

r2

∂u01 U1 ∂ 2 u01 + 2r − 2u01 + = 0, ∂r 2 ∂r s44 (c1 + c2 )

(30)

114

Ladislav Ceniga

∂U1 = c3 U1 , ∂r where the function U1 is derived as r

U1 =

(31)

∂ 2 u01 ∂ 2 u01 + . ∂ϕ2 ∂ν 2

(32)

A solution of this system of the differential equations (30), (31) is determined by the following mathematical procedures which result in a solution for the radial displacement u01 (see Eqs. (38)–(40)) along the axis x01 (see Fig. 2). Performing r [∂Eq.(31)/∂r], we get r2

∂ 2 U1 ∂U1 + (1 − c3 ) r = 0. 2 ∂r ∂r

(33)

Substituting Eq. (31) to Eq. (33), we get r2

∂ 2 U1 + c3 (1 − c3 ) U1 = 0. ∂r 2

(34)

If the dependence U1 − r is assumed in the form U1 = r λ , then the solution U1 of the differential equation (34) has the form 2 X ∂ 2 u01 ∂ 2 u01 U1 = + = Ci r λi , ∂ϕ2 ∂ν 2

(35)

i=1

where C1 , C2 are integration constants which are related to the mathematical procedure 1. The exponent λi (i = 1,2) is derived as √ i 1h 1 + (δ1i − δ2i ) D , i = 1, 2, 2 D = 1 − 4 c3 (1 − c3 ) = 1 + 16 (1 − µ) [1 + 4 (1 − µ)] , λi =

(36)

Due to µ < 0.5 for a real isotropic material [9], and c3 < 0 (see Eq. (28)), we get D > 0, and the real exponents λ1 > 3, λ2 < −2. Considering Eq. (35), the differential equation (30) is transformed to the form 2 X ∂ 2 u01 2 ∂u01 2u01 1 + − = − Ci r λi −2 . (37) ∂r 2 r ∂r r2 s44 (c1 + c2 ) i= 1

Analytical Model of Thermal Stresses in Multi-Component ...

115

Using the Wronskian’s method [37], the radial displacement u01q = (r, ϕ, ν) in the spherical particle (q = p) and the cell matrix (q = m) has the form 2 X 0 u1q = Ciq ξiq uirq , q = p, m. (38)

u01q

i=1

The function uirq = uirq (r) and the coefficient ξiq (i = 1,2; q = p,m) have the forms uirq = r λiq , i = 1, 2; λ1q > 3, λ2q < −2; q = p, m, 1 1 1 ξiq = − , i = 1, 2; q = p, m, 3s44 (c1 + c2 ) λiq + 2 λiq − 1

(39) (40)

where u1rq = u1rq (r) and u2rq = u2rq (r) are increasing and decreasing functions of the variable r due to λ1q > 3 and λ2q < −2, respectively. With regard to Eqs. (11)–(14), (24)–(27), we get ε011q

=

2 X

Ciq ξiq λiq r λiq −1 ,

(41)

i=1

ε022q = ε033q =

2 X

Ciq ξiq r λiq −1 ,

(42)

i=1

ε012q

2 X ∂Ciq = ξiq r λiq −1 , ∂ϕ

(43)

i= 1

ε013q

2 X ∂Ciq = ξiq r λiq −1 , ∂ν

(44)

i= 1

0 σ11q =

2 X

Ciq ξiq ξ2+iq r λiq −1 ,

(45)

2 X

(46)

i=1 0 0 σ22q = σ33q =

Ciq ξiq ξ4+iq r λiq −1 ,

i=1 0 σ12q

2 1 X ∂Ciq = ξiq r λiq −1 , s44q ∂ϕ i=1

(47)

116

Ladislav Ceniga 0 σ13q =

2 1 X ∂Ciq ξiq r λiq −1 , s44q ∂ν

(48)

i=1

where the coefficients ξ2+iq , ξ4+iq (i = 1,2) are derived as ξ2+iq = λiq (c1q + c2q ) − 2c2q , i = 1, 2,

(49)

ξ4+iq = c1q − λiq c2q , i = 1, 2.

(50)

With regard to Eqs. (11)–(14), (24)–(27), (41)–(50), the thermal-stress induced elastic energy density wq [34]–[36] has the form 2 0 2 ∂u1q 2c1q u01q ∂u01q c1q u01q 1 wq = = (c1q + c2q ) − + 2 ∂r r ∂r r2 i,j=1 " 2 0 2 # ∂u01q ∂u1q 1 + + 2 s44q r ∂ϕ ∂ν 2 X 1 ∂Ciq ∂Cjq ∂Ciq ∂Cjq = ξ2+iq ξjq Ciq Cjq ξ4+i+2jq + + r λiq −λjq −2 , s44q ∂ϕ ∂ϕ ∂ν ∂ν 3 X

0 ε0ijq σijq

i,j=1

(51)

where the coefficient ξ4+i+2jq (i, j = 1,2) is derived as λjq (c1q + c2q ) − 2c2q , i, j = 1, 2. ξ4+i+2jq = λiq 2

(52)

The thermal-stress induced elastic energy Wq which is accumulated in the spherical particle (q = p), in the cell matrix around the particle (q = m) and in the cell matrix around the pore (=flaw, q = v) has the form Wq = 8

Zπ/2 Zπ/2 Z r2 0

0

r1

2

wq r dr dϕ dν = 8

Zπ/2 Zπ/2 Z r2 0

0

r1

3 1 X 0 0 ε σ 2 i,j=1 ijq ijq

!

r2 dr dϕ dν.

(53)

The boundaries r1 = 0, r2 = Rp; r1 = Rp, r2 = rc (see Eqs. (5)–(10)); and r1 = Rv , r2 = rc are valid for the spherical particle; for the cell matrix around the spherical particle; and for the cell matrix around the pore, respectively.

Analytical Model of Thermal Stresses in Multi-Component ...

5. 5.1.

117

Boundary Conditions Spherical Particle

The absolute value u01p is required to represent an increasing function of r ∈ h0, Rpi, exhibiting a maximum value on the particle-matrix boundary (i.e. 0 0 for r = Rp). Additionally, due to σiip ∝ r λp−1 , σ12+jp ∝ r λp−1 (i = 1,2,3; j = 0,1; see Eqs. (24)–(27)), the exponent λp is required to be λp > 1, otherwise (σiip )r→0 → ±∞, (σ12+jp )r→0 → ±∞. With regard to Eqs. (38), (39), u2rp = r λ2p is a decreasing function of the variable r due to λ2p < −2, and then we get C2p = 0. With regard to λ1p > 3 (see Eq. (39)), the boundary condition for the determination of the integration constant C1p (see Eq. (38)) has the form [8] 0 σ11p = −p, (54) r=R p

where the determination of the radial stress p acting at the particle-matrix boundary is analysed in Sec. 5.4. With regard to Eqs. (45), (54), we get C1p = −

5.2.

p λ −1

ξ1p ξ3p Rp 1p

(55)

Cell Matrix Around Particle

The absolute value |u01m | which exhibits a maximum value on the particlematrix boundary (i.e. for r = Rp) is required to represent a decreasing function of r ∈ hRp , rci, where rc is given by Eqs. (5)–(10). The decreasing course of the dependence |u01m | − r is ensured by the integration constants C1m , C2m in Eq. (38). The boundary conditions for the determination of the integration constants C1m , C2m are derived as 0 σ11m = −p, (56) r=Rp u01m

r=rc

= u01c = u1c0 fc .

(57)

where the function fc = fc (ϕ, ν) is given by Eqs. (6)–(10), and u1c0 is a radial displacement along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2).

118

Ladislav Ceniga

The determination of the radial stress p acting at the particle-matrix boundary and the determination of the radial displacement u1c0 are analysed in Secs. 5.4 and 5.5, respectively. With regard to Eqs. (38)–(40), (45), (56), (57), we get 1 u01c ξ5−im p Cim = − + rc ζ2+im ξim rcλim −1 ζim u1c0 ξ5−im 1 p + = − , i = 1, 2, (58) d ζ2+im ξim rcλim −1 ζim where u01c /rc = u1c0 /d (see Eqs. (2), (57)). The coefficients ζim , ξ4+2im (i = 1,2) have the forms ζim = ξ2+im

Rp rc

λim −1

ζ2+im = ξ2+im

5.3.

− ξ5−im

Rp rc

Rp rc

λim −λ3−im

λ3−im −1

, i = 1, 2,

− ξ5−im , i = 1, 2.

(59)

(60)

Cell Matrix Around Pore

The absolute value |u01v | is required to represent an increasing function of r ∈ hRv , rci, exhibiting a maximum value on the cell surface (i.e. for r = rc ). With regard to Eqs. (38), (39), u2rv = r λ2v is a decreasing function of the variable r due to λ2v < −2, and then we get C2v = 0. With regard to λ1v > 3 (see Eq. (39)), the boundary condition for the determination of the integration constant C1v (see Eq. (38)) has the form (61) u01v r=rc = −u01c = −u1c0 fc .

where the determination of the radial displacement u1c0 is analysed in Sec. 5.5. With regard to Eqs. (38), (39), (61), we get C1v = −

u01c ξ2m rcλ2m

=−

where u01c /rc = u1c0 /d (see Eqs. (2), (57)).

u1c0 d ξ2m rcλ2m −1

,

(62)

Analytical Model of Thermal Stresses in Multi-Component ...

5.4.

119

Determination of Radial Stress p

The thermal stresses in the porous multi-particle-matrix system (see Fig. 1) are a consequence of the radial stress p which acts at a particle-matrix boundary. The compressive or tensile radial stress, p > 0 or p < 0, results from the difference βm − βp > 0 or βm − βp < 0 (see Eq. (1)). As analysed in [8], the radial stress p is determined by the following formula ε022m r=Rp − ε022p r=R = βm − βp . (63) p

5.5.

Determination of u1c0

The radial displacement u1c0 along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) is determined by the following energy analysis. The thermal-stress induced elastic energy of the multi-particle-matrix system with pores (see Fig. 1) is represented by both the elastic energy Wv and by the elastic energy 26 (Wp + Wm ) accumulated in 26 cubic cells with particles. These 26 cubic cells are related to one porous cubic cell. Stresses acting in the porous cubic cell are induced by the thermal stresses acting in these 26 cubic cells. The stresses acting in both the 26 cubic cells and the porous cubic cell are required to fulfilled the following energy condition ∂ [26 (Wp + Wm ) − Wv ] =0 ∂u1c0

(64)

The condition (64) is considered for the determination of the radial displacement u1c0 .

6.

Thermal Stresses in Porous Multi-Particle-Matrix System

6.1.

Spherical Particle

With regard to Eqs. (41)–(48), (55), we get λ1p −1 pr r 0 u1p = − , ξ3p Rp λ1p −1 pλ1p r 0 ε11p = − , ξ3p Rp

(65)

(66)

120

Ladislav Ceniga λ1p −1 p r 0 0 , ε22p = ε33p = − ξ3p Rp λ1p −1 1 ∂p r 0 ε12p = − , ξ3p ∂ϕ Rp 1 ∂p r λ1p −1 0 ε13p = − , ξ3p ∂ν Rp λ1p −1 r 0 σ11p = −p , Rp λ1p −1 r pξ5p 0 0 , σ22p = σ33p = − ξ3p Rp λ1p−1 1 ∂p r 0 σ12p = − , s44p ξ3p ∂ϕ Rp 1 ∂p r λ1p −1 0 σ13p = − , s44p ξ3p ∂ν Rp

(67) (68) (69) (70) (71) (72) (73)

where the exponent λ1p and coefficients ξ3p , ξ5p are given by Eqs. (36) and (49), (50), respectively. The radial stress p acting at the particle-matrix boundary is given by Eqs. (92)–(95).

6.2.

Cell Matrix Around Particle

With regard to Eqs. (41)–(48), (58), we get u01m

λim −1 2 X p u1c0 ξ5−im r =− r + , ζim d ξ4+2im rc

(74)

i=1

ε011m

ε022m

=

=−

2 X

i= 1

ε033m

λim

p ζim

u1c0 ξ5−im + d ξ4+2im

r rc

λim −1

,

λim −1 2 X p u1c0 ξ5−im r =− + , ζim d ξ4+2im rc i= 1

(75)

(76)

Analytical Model of Thermal Stresses in Multi-Component ... ε012m

121

λim −1 2 X 1 − λ1p p u1c0 ξ5−im ∂rc r =− + rc ζim d ξ4+2im ∂ϕ rc i=1 λim −1 2 X ∂ p u1c0 ∂ ξ5−im r − + (77) ∂ϕ ζim d ∂ϕ ξ4+2im rc i=1

ε013m

λim −1 2 X 1 − λ1p p u1c0 ξ5−im ∂rc r =− + rc ζim d ξ4+2im ∂ν rc i=1 λim −1 2 X p u1c0 ∂ ξ5−im r ∂ + (78) − ∂ν ζim d ∂ν ξ4+2im rc i=1

0 σ11m

0 σ22m

0 σ12m

=− −

0 σ13m

=− −

=− =− 1

s44m 1 s44m

1 s44m 1 s44m

2 X

ξ2+im

ξ4+im

i=1 2 X

i=1

p ζim p ζim

u1c0 ξ5−im + d ξ4+2im

r rc

λim −1

,

(79)

u1c0 ξ5−im + d ξ4+2im

r rc

λim −1

,

(80)

λim −1 2 X 1 − λ1p p u1c0 ξ5−im ∂rc r + rc ζim d ξ4+2im ∂ϕ rc i=1 λim −1 2 X ∂ p u1c0 ∂ ξ5−im r + ∂ϕ ζim d ∂ϕ ξ4+2im rc i=1 (81)

λim −1 2 X 1 − λ1p p u1c0 ξ5−im ∂rc r + rc ζim d ξ4+2im ∂ν rc i=1 2 X ∂ p u1c0 ∂ ξ5−im r λim −1 + (82) . ∂ν ζim d ∂ν ξ4+2im rc i=1

where the exponent λ2m and the coefficient ξ2+im (i = 1, . . . , 4), ζjm (i = 5, . . . , 8) are given by Eqs. (36) and (49), (50), (59), (60), respectively. The radial stress p acting at the particle-matrix boundary and the radial displacement u1c0 along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) are given by Eqs. (92)–(95) and (126)–(128).

122

Ladislav Ceniga

6.3.

Cell Matrix Around Pore

With regard to Eqs. (41)–(48), (62), we get u01v

u1c0 r =− d

r rc

λ2m −1

,

u1c0 λ2m r λ2m −1 = λ2m − , d rc u1c0 r λ2m −1 0 0 ε22v = ε33v = − , d rc u1c0 (1 − λ2m ) ∂fc r λ2m −1 0 ε12v = − , d fc ∂ϕ rc u1c0 (1 − λ2m ) ∂fc r λ2m −1 0 , ε13v = − d fc ∂ν rc u1c0 ξ4m r λ2m −1 0 σ11v = − , d rc u1c0 ζ4m r λ2m −1 0 σ22v = − , d rc u1c0 (1 − λ2m) ∂fc r λ2m −1 0 σ12v = − , d s44m fc ∂ϕ rc u1c0 (1 − λ2m) ∂fc r λ2m −1 0 σ13v = − , d s44m fc ∂ν rc ε011v

(83)

(84) (85) (86) (87) (88) (89) (90) (91)

where the exponent λ2m and the coefficients ξ4m, ζ4m (i = 1,2) are given by Eqs. (36) and (49), (50), respectively. The radial displacement u1c0 along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) is given by Eqs. (126)–(128).

Analytical Model of Thermal Stresses in Multi-Component ...

6.4.

123

Radial Stress p

With regard to Eqs. (43), (63), (67), the radial stress p acting at the particlematrix boundary has the form u1c ζ6m u1c0 ζ6m p = ζpm + βm − βp = ζpm + βm − βp , (92) rc d where the coefficients ζpm , ζ5m , ζ6m are derived as ζpm =

ζ5m = ξ3m

ζ6m

ξ3p , 1 − ξ3p ζ5m

Rp λ1m −1 rc Rp λ1m −1 rc

−

Rp rc

− ξ4m

(93)

λ2m −1

Rp λ2m −1 rc

λ1m −1 R (ξ3m + ξ4m ) rcp = . λ1m −λ2m R ξ3m rcp − ξ4m

,

(94)

(95)

The exponent λim and the coefficient ξ3p , ξ2+im (i = 1,2) are given by Eqs. (36) and (49), respectively. The radial displacement u1c0 along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) is given by Eqs. (126)– (128).

6.5.

Radial Displacement u1c0

With regard to Eqs. (51), (55), (58), (62), the elastic energy density wq (q = p,m,v) has the form u 2 2ω u (β − β ) r 2λ1p−2 1c0 2p 1c0 m p 2 wp = ω + + ω (β − β ) , 1p 3p m p 2 d d ξ3p (96) u 2 ω u (β − β ) 1c0 2m 1c0 m p 2 wm = ω1m + + ω3m (βm − βp) , (97) d d u 2 r λ2m −2 1c0 wv = ωv , (98) d rc

124

Ladislav Ceniga

where the coefficients ωiq (i = 1,2,3; q = p,m), ωv along with the coefficients ζ1p , ξim (i = 7, . . . , 36) are derived as ( 2 2 ) ∂ (ζ ζ ) ∂ (ζ ζ ) 1 pm 6m pm 6m 2 2 ω1p = ζ1p ζ6m ζpm + + , (99) s44p ∂ϕ ∂ν 2 ω2p = ζ1p ζ6m ζpm +

1 s44p

(

) ∂ζpm ∂ (ζpm ζ6m ) 2 ∂ζpm ∂ (ζpm ζ6m ) 2 + , ∂ϕ ∂ϕ ∂ν ∂ν (100)

ω3p =

ω1m

2 ζ1p ζpm

+

1 s44p

"

∂ζpm ∂ϕ

2

+

∂ζpm ∂ν

2 #

,

(101)

λim +λjm −2 2 X ζ26+i+2jm Rp = ξ4+i+2jm ζ4+i+2jm + , (102) s44m rc i,j=1

ω2m =

λim +λjm −2 2 X ζ30+i+2jm Rp ξ4+i+2jm ζ8+i+2jm + , (103) s44m rc

i,j=1

ω3m

λim +λjm −2 2 X ζ32+i+2jm Rp = ξ4+i+2jm ζ12+i+2jm + , (104) s44m rc i,j=1

ωv = c1m + λ2m

»

– „ «2 "„ «2 „ «2 # λ2m λ2m − 1 ∂fc ∂fc (c1m + c2m ) − 2c2m + + , 2 fc ∂ϕ ∂ν

(105) ζ1p = ζ4+i+2jm =

λ21p (c1p + c2p ) − 2λ1p c2p + c1p, 2

2 2 ζ6m ζpm ξ5−im ξ5−jm + + ζ6m ζpm ζim ζjm ζ2+im ζ2+jm

i, j = 1, 2,

„

(106)

ξ5−im ξ5−jm + ζ2+im ζjm ζim ζ2+jm

«

,

(107) ζ8+i+2jm =

2 2 ζ6m ζpm + ζpm ζim ζjm

ξ5−im ξ5−jm + ζ2+im ζjm ζim ζ2+jm

, i, j = 1, 2, (108)

Analytical Model of Thermal Stresses in Multi-Component ... ζ12+i+2jm = ζ18+im =

2 ζpm , i, j = 1, 2, ζim ζjm

ζ6m ζpm ξ5−im + , i = 1, 2, ζim ζ2+im

∂ ζ18+im d ζ18+im (λim − 1) − ∂ϕ rc ζpm d ζpm (λim − 1) ∂ = − ∂ϕ ζim rc ζim

125 (109) (110)

ζ19+2im =

∂fc , i = 1, 2, ∂ϕ

(111)

ζ20+2im

∂fc , i = 1, 2, ∂ϕ

(112)

ζ23+2im =

∂fc , i = 1, 2, ∂ν

(113)

ζ24+2im

∂fc , i = 1, 2, ∂ν

(114)

ζ26+2im = ζ19+2im ζ19+2jm + ζ23+2im ζ23+2jm , i = 1, 2,

(115)

∂ ζ18+im d ζ18+im (λim − 1) − ∂ν rc d ζpm (λim − 1) ∂ ζpm = − ∂ν ζim rc ζim

ζ30+2im = ζ20+2im ζ19+2jm + ζ19+2im ζ20+2jm + ζ24+2im ζ23+2jm + ζ23+2im ζ24+2jm , i = 1, 2, (116) ζ32+2im = ζ20+2im ζ20+2jm + ζ24+2im ζ24+2jm , i = 1, 2,

(117)

With regard to Eqs. (53), (96)–(99), the thermal-stress induced elastic energy Wq accumulated in the spherical particle (q = p), in the cell matrix around the spherical particle (q = m), and in the cell matrix around the spherical pore (q = v) has the form Wp =

» – “ u ”2 2u Ω (β − β ) 8R3p 1c0 1c0 2p m p 2 Ω + + Ω (β − β ) , 1p 3p m p 2 ξ3p (2λ1p + 1) d d

(118) h i Wm = 8d u21c0 Ω1m + u1c0 d Ω2m (βm − βp ) + d2 Ω3m (βm − βp)2 , (119) 2 Wv = 8 d u1c0 Ωv , (120)

where the coefficients Ωiq (i = 1,2,3; q = p,m), Ωv are derived as Zπ/2 Zπ/2 Ωip = ωip dϕ dν, i = 1, 2, 3, 0

0

(121)

126

Ladislav Ceniga Ω1m =

Zπ/2 Zπ/2 X 2 0

Ω2m =

Zπ/2 Zπ/2 X 2 0

Ω3m =

0

fc3 ζ26+i+2jm ξ4+i+2jm ζ4+i+2jm + λ + λjm + 1 s44m i,j=1 im " λim +λjm +1 # Rp × 1− dϕ dν, (122) rc

0

ζ30+i+2jm fc3 ξ4+i+2jm ζ8+i+2jm + λ + λjm + 1 s44m i,j=1 im " λim +λjm +1 # Rp × 1− dϕ dν, (123) rc

Zπ/2 Zπ/2 X 2 0

0

Ωv =

fc3 ζ32+i+2jm ξ4+i+2jm ζ12+i+2jm + λim + λjm + 1 s44m i,j=1 " λim +λjm +1 # Rp × 1− dϕ dν, (124) rc Zπ/2 Zπ/2 0

0

" 2λ2m+1 # Rv ωv fc3 1− dϕ dν. 2λ2m + 1 rc

(125)

With regard to Eqs. (64), (118)–(120), the radial displacement u1c0 along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) has the form u1c0 =

d ζ1 (βm − βp ) , ζ2

(126)

where the coefficients ζ1 , ζ2 are derived as 3 2Ω2p Rp ζ1 = Ω2m + 2 , ξ3p (2λ1p + 1) d " 3 # Ω1p Rp Ωv ζ2 = − 2 Ω1m + 2 . 13 ξ3p (2λ1p + 1) d

(127)

(128)

Analytical Model of Thermal Stresses in Multi-Component ...

7.

127

Application to SiC-Si3N4 Ceramics

This section presents illustrative examples of applications of final formulae for the thermal stresses (see Sec. 6) to a real porous two-component material of the precipitate-matrix type. These illustrative examples are numerically performed for the SiC-Si3 N4 ceramics. Other applications of the final formulae (see Sec. 6) can be easily performed by a reader. This numerical determination can be performed by a computer software using suitable programming techniques. With regard to programming techniques within a suitable programming language (e.g. Fortran, Pascal), a derivative of the function ψ = ψ (η) regarding the variable η = ϕ, ν (see e.g. Eqs. (77), (78)) can be numerically determined by the formula ∂ψ ψ (η + ∆η) − ψ (η) ≈ , ∂η ∆η

(129)

where ψ = rc , ξ, ζ, and η = ϕ, ν. The angle steps ∆ϕ, ∆ν are required to be taken as small as possible. With regard to an experience of the author, the angle steps ∆ϕ = ∆ν = 10−6 [deg] are sufficient to be considered within the numerical determination. Similarly, a definite integral (see Eqs. (121)–(125)) can be numerically determined by the formula ! Zπ/2 Zπ/2 m n X X ω dϕ dν ≈ (130) Ω= ω (i × ∆ϕ; j × ∆ν) ∆ϕ ∆ν, 0

j=0

0

i=0

where n, m are integral parts of the real numbers π/ (2 ∆ϕ), π/ (2 ∆ν), respectively. With regard to an experience of the author, the angle steps ∆ϕ = ∆ν = 0.01 − 0.1 [deg] are sufficient to be considered within the numerical determination. Considering the same conditions concerning the angle steps ∆ϕ, ∆ν as related to Eq. (130), the average value κ of the function κ = κ (ϕ, ν) of the variables ϕ, ν ∈ h0, π/2i can be numerically determined by the formula π/2 Z π/2 „ «2 Z „ «2 X m 2 2 κ = κ dϕ dν ≈ π π j=0 0

0

n X i=0

!

κ (i × ∆ϕ; j × ∆ν) ∆ϕ ∆ν,

(131)

0 ) where κ = p, u1c0, (σ11v r=rc . Table 1 presents material parameters of the SiC particle and the Si3 N4 matrix of the SiC-Si3 N4 ceramics. The SiC-Si3 N4 ceramics represents a porous

128

Ladislav Ceniga

two-component material of a precipitate-matrix type. Pores in the Si3 N4 matrix are a consequence of powder metallurgy processes [9]. The relaxation temperature Tr = 665◦ C is determined by the formula Tr = 0.35 Tm [9], where Tm = Tmm is melting temperature of the SiC-Si3 N4 ceramics. Table 1. Material parameters of the SiC-Si3 N4 ceramics [9].

Eq [GPa] µq αq [10−6 K−1 ] Tmq [◦ C]

Particle (q = p) SiC 360 0.19 4.15 2730

Matrix (q = m) Si3 N4 310 0.235 2.35 1900

As shown in Fig. 5, the dependence p−vp (see Eq. (131)) for the radial stress p = p (ϕ, ν) acting at the SiC-Si3 N4 boundary exhibits a decreasing course for vp ∈ (0, vpmax) (see Eq. (2)) in contrast to an increasing course of the radial displacement u1c0 = u1c0 (v) (see Fig. 6) along the axis xi (i = 1,2,3) on the cubic cell surface (i.e. for r = d/2) (see Eqs. (126)–(128)), where Rp = 3 µm, Rv = 0.1 µm, Tr = 665◦ C, Tf = 20◦ C. With regard to βp > βm (see Eq. (1), Tab. 1), the dimension d of the cubic cell with the spherical particle is changed to d − u1c) due to the thermal stresses. Consequently, the dimension d of the cubic cell with the spherical pore is changed to d + u1c) due to the thermal stresses. 0 Finally, the increasing dependence σ11v − vp (see Eq. (131)) for the r=rc

0 ) radial stress (σ11v r=rc = p (ϕ, ν) acting on a surface of the cubic cell with the spherical pore (i.e. for r = rc , see Eqs. (5)–(10)) is shown in Fig. 7

Conclusion Results of this chapter are as follows. The analytical model of thermal stresses in a porous multi-particle-matrix system with isotropic components is determined (see Secs. 2, 6). The analytical model results from fundamental equations of mechanics of an elastic solid continuum (see Sec. 3).

Analytical Model of Thermal Stresses in Multi-Component ...

129

Figure 5. The function p = p (vp ) of the volume fraction vp ∈ (0, vpmaxi (see Eqs. (2), (131)) of the SiC particle, where Rp = 3 µm, Rv = 0.1 µm, Tf = 20◦ C, Tr = 665◦ C. The radial stress p = p (ϕ, ν, v) (see Eqs. (92)–(95)) acts at the SiC-Si3 N4 boundary.

Figure 6. The radial displacement u1c0 = u1c0 (vp ) along the axis xi (i = 1,2,3) on a surface of the cubic cell with the spherical pore (i.e. for r = d/2) (see Eqs. (126)–(128)) as a function of the volume fraction vp ∈ (0, vpmaxi (see Eq. (2)) of the SiC particle, where Rp = 3 µm, Rv = 0.1 µm, Tf = 20◦ C, Tr = 665◦ C. The porous multi-particle-matrix system consists of isotropic spherical particles and spherical pores which are both periodically distributed in an isotropic infinite matrix (see Fig. 1). The thermal stresses are a consequence of different

130

Figure 7. The dependence

Ladislav Ceniga

0 σ11v

r=rc

− vp on the volume fraction vp ∈

0 (0, vpmaxi (see Eqs. (2), (131)) for the radial stress (σ11v )r=rc = p (ϕ, ν) acting on a surface of the cubic cell with the spherical pore (i.e. for r = rc , see Eqs. (5)–(10), (88)), where Rp = 3 µm, Rv = 0.1 µm, Tf = 20◦ C, Tr = 665◦ C.

thermal expansion coefficients of the isotropic matrix and isotropic particle (see Eq. (1)). The infinite matrix is imaginarily divided into identical cubic cells (see Fig. 1), and the thermal stresses are thus investigated within the cubic cell. Each cell contains either a central particle or a central pore (see Sec. 2). This porous multi-particle-matrix system represents a model system which is applicable to porous two-component materials of a precipitate-matrix type. Radii and volume fractions of both the particles and of the pores along with the cubic cell dimension represent microstructural parameters of the porous two-component material. The thermal stresses are then functions of these microstructural parameters. Numerical values for a real porous two-component material of the precipitate-matrix type (SiC-Si3 N4 ceramics) are obtained.

Acknowledgments This work was supported by the Slovak Grant Agency under the contract VEGA 2/0081/16, 2/0120/15, 2/0113/16 and by the Slovak Research and Development Agency under the contract APVV-0147-11.

Analytical Model of Thermal Stresses in Multi-Component ...

131

References [1] Greisel, M.; J¨ager, J.; Moosburger-Will, J.; Sause, M.G.R.; Mueller, W.M.; Horn, S. Composites: Part A 2014, 66, 117-127. [2] Meijer, G.; Ellyin, F.; Xia, Z. Composites: Part B 2000, 31, 29–37. [3] We¸glewski, W.; Basista, M.; Manescu, A.; Chmielewski, M.; Pietrzak, K.; and Schubert, Th. Composites: Part B 2014, 67, 119-124. [4] Nabavi, S.M.; Ghajar, R. Int. J. Eng. Sci. 2010, 48, 1811-1823. [5] Lee, J.; Hwang, K.-Y. Int. J. Eng. Sci. 1996, 34, 901–922. [6] Tanigawa, Y.; Osako, M.K. Int. J. Eng. Sci. 1986, 24, 309–321. [7] Abedian, A.; Szyszkowski, W.; Yannacopoulos, S. Compos. Sci. Technol. 1999, 59, 41–54. [8] Ceniga, L. Analytical Model of Thermal Stresses in Composite Materials I; Nova Science Publishers: New York, US, 2008, pp 66–67, 136– 137. ˇ [9] Skoˇcovsk´y, P.; Bok˚uvka, O.; Palˇcek, P. Materials Science; EDIS: Zilina, SK, 1996, pp 35–48. [10] Selsing, J. J. Amer. Cer. Soc. 1961, 44, 419–419. [11] Davidge, R.W.; Green, T.J. J. Mater. Sci. 1968, 3, 629–634. [12] Mastelaro, V.R.; Zanotto, E.D. J. Non-Crystal. Sol. 1996, 194, 297–304. [13] Mastelaro, V.R.; Zanotto, E.D. J. Non-Crystal. Sol. 1999, 247, 79–86. [14] Diko, P. Supercond. Sci. Technol. 1998, 11, 68–72. [15] Diko, P.; Fuchs, G.; Krabbes, G. Physica C 2001, 363, 60–66. [16] Diko, P. Supercond. Sci. Technol. 2004, 17, R45–R58. [17] Diko, P. Int. J. Mater. Product Technol. 2014, 49, 97-128. ˇ na, I.;, Peˇsiˇcka, J. J. Eur. Ceram. Soc. 2011, [18] Chmel´ık, F.; Trn´ık, A.; Stubˇ 31, 2205-2209.

132

Ladislav Ceniga

[19] Serbena, F.C.; Zanotto, E.D. J. Non-Crystal. Sol. 2012, 358, 975–984. [20] Bidulsk´y, R.; Bidulsk´a, J.; Grande, M.A. Arch. Metallur. Mater. 2013, 58, 365–370. [21] Kvaˇckaj, T.; Koˇcisko, R.; Bidulsk´y, R.; Bidulsk´a, J.; Bella, P.; Lupt´ak, M.; Kov´acˇ ov´a, A.; Bacso, J. Mater. Sci. For. 2014, 782, 379– 383. [22] Bidulsk´y, R.; Bidulsk´a, J.; De Oro, R.; Hryha, E.; Maccarini, M.; Forno, I.; Grande, M.A. Act. Phys. Polon. A 2015, 128, 647–650. ˇ na, I.; Str´ask´a, J.; [23] Knapek, M.; H´ulan, T.; Min´arik, P.; Dobroˇn, P.; Stubˇ Chmel´ık, F. J. Eur. Ceram. Soc. 2016, 36, 221-226. [24] Mizutani, T. J. Mater. Sci. 1996, 11, 483–494. [25] Li, Sh.; Sauer, R.A.; Wang, G. J. Appl. Mech. 2007, 74, 770–783. [26] Li, Sh.; Sauer, R.A.; Wang, G. J. Appl. Mech. 2007, 74, 784–797. [27] Kushch, V.I. Prikladnaja Mekhanika 1985, 21, 18-27. [28] Kushch, V.I. Int. Appl. Mech. 2004, 40, 893-899. [29] Kushch, V.I. Int. Appl. Mech. 2004, 40, 1042-1049. [30] Wu, Y.; Dong, Z. Mater. Sci. Eng. 1995, 203, 314–323. [31] Sangani, A.S.; Mo, G. J. Mech. Phys. Sol. 1997, 45, 2001–2031. [32] Mura, T. Micromechanics of Defects in Solids; Martinus Nijhoff Publishers: Dordrecht, NL, 1987, pp 1–3. [33] Ceniga, L. Analytical Models of Thermal Stresses in Composite Materials IV; Nova Science Publishers: New York, US, 2015, pp 34–37. [34] Brdiˇcka, M.; Samek, L.; Sopko, B. Mechanics of Continuum; Academia: Prague, CZ, 2000, pp 78–83. ˇ ca´ k, F.; Jurica, V. Elasticity and Strength I; Technical [35] Trebuˇna, F.; Simˇ University: Koˇsice, SK, 2005, pp 57–63.

Analytical Model of Thermal Stresses in Multi-Component ...

133

ˇ ca´ k, F.; Jurica, V. Examples and Problems of Elasticity [36] Trebuˇna, F,;, Simˇ and Strength I; Technical University: Koˇsice, SK, 2002, pp 134–138. [37] Rektorys, K. Review of Applied Mathematics; SNTL: Prague, CZ, 1973, pp 253–267.

In: Ceramic Materials Editor: Jacqueline Perez

ISBN: 978-1-63485-965-3 © 2017 Nova Science Publishers, Inc.

Chapter 5

AN UPDATE OF CURRENT KNOWLEDGE ON ADHESION TO ZIRCONIA DENTAL RESTORATIONS M. L. P. D. Engler1, E. Ruales1, M. Özcan2 and C. A. M. Volpato1,* 1

Department of Dentistry, Federal University of Santa Catarina, Florianópolis, Brazil 2 Dental Materials Unit, Center for Dental and Oral Medicine, Clinic for Fixed and Removable Prosthodontics and Dental Materials Science, University of Zurich, Zurich, Switzerland

Abstract Yttria-stabilized tetragonal zirconia polycrystal (Y-TZP) has been used in dentistry in order to manufacture prosthetic frameworks, monolithic crowns and implant abutments due to its superior mechanical properties, biocompatibility, chemical stability and appropriate aesthetics as opposed to other materials. The survival of dental ceramic restorations depends on durable bond strength between the restorative material, composite resin luting cement and the tooth surface. However, it is difficult to establish a durable mechanical or chemical adhesion in zirconia-based prostheses since yttrium-stabilized zirconia is an oxide ceramic that does not contain silicon dioxide (SiO2) phase in its microstructure. In order to achieve strong and reliable adhesion between resin composite luting cements *

E-mail address: [email protected] (Corresponding author).

136

M. L. P. D. Engler, E. Ruales, M. Özcan et al. and zirconia surfaces, it is crucial to employ a method that does not impair the mechanical properties and at the same time rendering it compatible with the luting cement. Furthermore, the chosen method should be practical, easy to perform and should not cause t→m phase transformation. Several methods and protocols for conditioning zirconia surfaces prior to adhesive cementation have been suggested in the literature such as physical, physicochemical and chemical methods. Typically, while physical surface conditioning methods are based on employing air-borne particle abrasion with alumina particles, physicochemical methods use silica-coated alumina particles followed by silanization. It is also possible to activate the zirconia surface chemically using functional-monomer containing adhesive promoters in the form of adhesive cements or primers. Generally, combination of micromechanical and chemical surface conditioning methods are preferred to enhance adhesion to zirconia. As this ceramic demonstrates superior properties compared to other ceramics, it is essential to study the peculiar characteristics of dental zirconia after surface conditioning methods and suggest one that does not damage its favorable mechanical properties. This chapter will provide the recent information on the use of zirconia in dentistry, its characteristics and indications, with a particular emphasis on surface conditioning methods to promote adhesion of resin-based materials to zirconia.

Keywords: zirconia, adhesion, prosthetic restorations, dentistry

1. Introduction The science of ceramic materials is evolving, including the development and introduction of new ceramic materials with high mechanical strength that allows for new indications and applications in dentistry. During the last few decades, new materials have been introduced in dentistry that could be used in conjunction with CAD/CAM technologies in order to solve dental problems that used to be limited to metal-ceramic restorations (Özcan & Volpato, 2015). Among many other ceramics, zirconia (ZrO2) received more attention of dentists and researchers due to the its favourable mechanical properties (Miyazaki et al., 2013; Ferrari, Vichi & Zarone, 2015), offering long term durability (Piascik et al., 2009) and versatility of aplications such as fixed dental prosthesis (FDPs), root posts, orthodontic brackets, implants and implant abutments (Özcan & Bernasconi, 2015).

An Update of Current Knowledge on Adhesion …

137

1.1. Main Caracteristics of Zirconia Zirconium dioxide (hereafter: zirconia) is an allotrope meaning that it can be found in more than one crystalline phase with the same chemical composition, namely monoclinic, tetragonal and cubic phases (Curtis, Wright & Fleming, 2006). However, in order to maintain zirconia in the tetragonal state at low temperatures (below 1770°C to room temperature), it is necessary to use a stabilizer such as yttrium, magnesium, cerium and calcium oxides, all of which could lead zirconia to a metastable state (Guan, Zhang & Liu, 2015). Yttriastabilized tetragonal zirconia polycrystal is composed of ZrO2 crystals and contains 2.5 to 3.5% yttrium oxide (Y2O3) (Vagkopoulou et al., 2009). As a biomaterial in medicine, zirconia stabilized by yttrium oxide is the only material with an ISO standard (13356.2008) (International Standards Organization, 2008). Because of its metastable state, the Y-TZP can undergo a process called “transformation toughening”. This phenomenon is a phase transformation induced by external forces. The impact of a magnitude of force could create a crack on the surface of the material but the metastable particles convert from tetragonal to monoclinic phase resulting in volumetric expansion of approximately 5% (Lughi & Sergo, 2010). This peculiar characteristic increases mechanical properties of zirconia (Passos et al., 2014). YTZP has fracture strength of >1000 MPa and toughness of 5-7 MPa m0.5, being the highest reported for a dental ceramic (Castro et al., 2012). Apart from mechanical properties, its aesthetic properties, biocompatibility, chemical stability and low thermal conductivity are determinant factors in order to choose this ceramic for several dental applications (Sciasci et al., 2015). Y-TZP is a chemically inert material and no local or systemic adverse effects have been reported. When it comes to cytotoxic, oncogenic or mutagenic properties, no adverse effects were observed on neither on fibroblasts nor on blood cells (Vagkopoulou et al., 2009). In vitro tests showed that zirconia ceramics have similar cytotoxicity levels with alumina (Piconi & Maccauro, 1999), and the in vivo behavior of zirconia compared with alumina did not show differences as regards to tissue reaction (Garvie & Nicholson, 1972). From optical point of view, being white, it is considered as an aesthetic material. Despite its high refractive index, it is still more translucent than metal (Vagkopoulou et al., 2009). With the purpose of enhancing aesthetics, some manufacturers offer coloured zirconia frameworks but limited information is available on the long-term colour stability (Reich & Hornberger, 2002). Recently, high-translucent zirconia has been introduced that contains smaller particles in the microstructure, having higher

138

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

density and cubic zirconia in the composition, making a hybrid of tetragonal-cubic zirconia (Zhang & Kim, 2009).

2. Adhesive Bonding for Zirconia Adhesive bonding of zirconia on dental tissues using resin based luting cements were recommended for improved retention (Blatz, Sadan & Kern, 2003), marginal adaptation (Derand et al., 2005) and the possibility of achieving more conservative dental restorations. Also, longevity of ceramic restorations is highly dictated by the adhesive bonding procedures. Likewise, long-term success is highly affected by the surface conditioning methods employed on the intaglio surfaces of zirconia-based reconstructions (Senyilmaz et al., 2007; Blatz, Sadan & Kern, 2003; Ozcan, Nijhuis & Valandro, 2008). Several luting cements have been proposed to be used with zirconia reconstructions, including glass ionomer (Blatz et al., 2007), conventional composite resin and self-etching cements (Attia, 2011). Nonetheless, adhesion between resin-based materials and zirconia is compromised as zirconia is an oxide ceramic without silica phase in its composition that is also acid-resistant (Kern & Wegner, 1998; Derand & Derand, 2000; Blatz, Sadan & Kern, 2003; Thompson et al., 2011). Hence, it is not possible to condition the surface of this material with hydrofluoric acid etching to create micromechanical retention (Della Bona et al. 2007). On the contrary, in silica based ceramics the use of hydrofluoric acid removes the vitreous matrix, increasing the surface roughness and energy in order to achieve a micromechanical bonding with resin-based luting cement. Also, in silica-based ceramics, the use of silane coupling agents allows the union of silicon dioxide (SiO2) present in the ceramic surface with the organic matrix of the resin composite luting cements (Mattiello et al., 2013). In the absence of SiO2 on the surface of the zirconia, silane coupling agents are ineffective in adhesive bonding procedures (Tsuo, Atsuta & Yoshida, 2006). Additionally, zirconia is an inert substrate with low surface energy and wettability (Özcan & Vallitu, 2003). It is virtually a flat material, free of roughness without a pattern of detectable microretention as it is composed of very small crystals (Janda et al., 2003) with minimum space between particles (Duran & Moure, 1984).

An Update of Current Knowledge on Adhesion …

139

2.1. Surface Conditioning Methods for Zirconia Surfaces Since zirconia surface does not favour durable adhesive bonding, numerous surface conditioning methods have been proposed in order to improve the interaction between resin-based luting cements and the zirconia surface (Sciasci et al., 2015; Burke et al., 2002; Derand, Molin & Kvam, 2005; Subaşı & İnan, 2014). Among all methods proposed, the simplest, functional and widely employed method used is air-borne particle abrasion using Al2O3 particles. In this method, particles ranging from 25 to 120 µm have been indicated while shear bond strength values reported statistically similar results independent of the particle size (Sciasci et al., 2015). Also, when bigger particles are used, possible ditching between the resin composite luting cement and zirconia surface could occur (Özcan, Nijhuis & Valandro, 2008). For this reason, particles of 50 µm are commonly accepted for air-abrasion protocols used for zirconia (Özcan, Nijhuis & Valandro, 2008; Blatz et al., 2010). Air-abrasion is typically performed using an intraoral air-abrasion device at a pressure between 2.3 and 3 bar for 12 to 15 seconds, maintaining a distance of 10 mm from the zirconia surface (Blatz et al., 2010; Özcan, Nijhuis & Valandro, 2008; Michida et al., 2015). This type of mechanical conditioning method could also remove contamination from cementation surfaces, clean the desired area and produce a rough surface on zirconia that increase the surface area and improve its surface energy (Özcan, Nijhuis & Valandro, 2008; Souza et al., 2013). Despite such advantages of air-abrasion protocols, air-particle abrasion without the use of primers could result in initial high bond strength to zirconia surface but the bond decreases drastically after long-term aging conditions (Kern, Barloi & Yang, 2009; Özcan et al., 2013). One other suggested physicochemical conditioning method is tribochemical silica coating, a procedure usually applied in dental laboratories using Al2O3 particles coated with silica layer (30 - 110 µm) (Burke et al., 2002; Sarmento et al., 2014). This conditoning method not only creates micro-roughness on the surface but also chemically activates the surface to react with the silane coupling agents (Özcan, Nijhuis & Valandro, 2008; Atsu et al., 2006; Kern & Wegner, 1998). The silanol groups (Si-OH) and later their reaction with the silica surface form siloxane (-Si-O-Si-O-) network (Özcan, Nijhuis & Valandro, 2008) that is capable of achieving covalent bonds at resin cement/silica-coated ceramic interface (Matinlinna et al., 2006; Valandro et al., 2007; Xible et al., 2006), justifying the use of this conditioning method.. Yet, poor silicon surface could suffer from after hydrothermal aging and impair the achieved adhesion

140

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

(Matinlinna et al., 2006). Therefore, tribochemical silica coating with the use of appropriate primers seems mandatory (Kern, Barloi & Yang, 2009). The optimum protocol for silica coating of zirconia surface was described as follows: (Özcan, 2013; Özcan, 2014) 1. 2. 3. 4.

Check the fit of the restoration using silicone based materials. Mark the area to be air-abraded with a pencil. Protect the outer surface of the restoration utilizing glycerin gel. Air abrade the cementation surface with silica coated alumina particles or silica particles only, using a chairside air-abrasion device. The particles size should range between 30 to 50µm at a pressure of 0.5 to 2.5 bar for 20 seconds, maintaining a distance of 10 mm from zirconia surface in circling motions. 5. Ultrasonic cleaning of the restoration in ethanol for 10 min. After this surface conditioning protocol, the intaglio surfaces should be able to interact with silane coupling agents and thereafter with the resin-based luting cements. Current evidence indicates superior performance of tribochemical silica coating in improving adhesion to zirconia when compared to air-abrasion with alumina (Özcan & Vallitu 2003; Atsu et al. 2006; El-Korashy & El-Refai, 2014; Erdem et al., 2014; Özcan & Bernasconi 2015). Despite the fact that the most widely used methods to improve adhesion to zirconia is air-abrasion with alumina and tribochemical silica coating, other conditioning methods are also being studied to induce increased surface bond area, surface energy and wettability (Mattiello et al., 2013; Kim et al., 2011). One such method is plasma coating with hexamethyldisiloxane, a rapid process performed at low temperatures by a reactor that generates an ionized gas when deposited on the zirconia surface. Although in part the reaction is explained by covalent bonds, adhesion mechanism of this surface modification remains unclear (Derand, Molin & Kvam, 2005). The application of micropearls of low fusing porcelain or vapor deposition of silicone tetrachloride (SiCl4) has also been investigated to obtain a silica layer on the zirconia surface (Derand, Molin & Kvam, 2005; Cura et al., 2012; Castro et al., 2012; Derand et al., 2008). This method have shown improved bond strength of resin composite luting cements but glass deposition could interfere with the internal adaptation of restorations. Other mechanical conditioning methods contemplate the use of erbium-doped yttrium aluminum garnet (Er:YAG) laser to modify zirconia through the removal of particles by micro explosions and vaporization, in a process named ablation

An Update of Current Knowledge on Adhesion …

141

(Cavalcanti et al., 2009). Er:YAG laser appears to have minimal impact on surface modifications as opposed to air-abrasion protocols that is attributed to lower laser energy absorption due to the fact that it is a water-free material (Subaşı & İnan, 2014). This procedure might damage the surface of zirconia due to severe temperature modifications that could be responsible for phase transformation (Guazzato et al., 2005). On the other hand, CO2 laser showed improved adhesion as a result of microcracks created on the zirconia surface allowing resin penetration. Unfortunately, this could yield to subsurface damage of zirconia that eventually weakens the material (Kasraei et al., 2014). Nevertheless, results are still contradictory for improving bond strength of resin materials to zirconia with the use of laser technologies (Subaşı & İnan, 2014; Mattiello et al., 2013). One other interesting method in this respect is selective infiltration etching (SIE) that transforms the relatively smooth zirconia surface into a 3-dimensional network of inter-grain porosity, making it a highly retentive surface (Aboushelib et al., 2009). Principally, heat-induced maturation and grain boundary diffusion that consist a low temperature fused glass ceramic layer is selectively applied to the surface and subsequently etched with 5% hydrofluoric acid (Aboushelib et al., 2009; Aboushelib, 2011). Despite the increased initial bond strength, a stable bond promoted with this method after long-term aging is still questionable (Mattiello et al., 2013; Cheung & Botelho, 2015). Other attempts to enhance adhesion of resin materials to zirconia involve the use of acidic agents (Liu et al. 2015)), namely etching zirconia with an acidic solution at 100ºC for 25 minutes or etching with hydrofluoric acid (48%) at 100ºC for 25 minutes. After both methods, the specimens were sintered following the manufacturer`s protocol. With such acid etching protocols it is claimed that zirconia grains are removed or dislodged, creating a rough surface that could result in an enhanced resin to zirconia interlocking.

3. Composite Resin Cements Adhesion to zirconia could also be improved with the use of resin cements containing functional monomers due to their special affinity to metal oxides (Kern & Wegner, 1998; Blatz et al., 2010; Passos et al., 2010; Mattiello et al., 2013). Phosphate ester monomers in such resin cements, such as 10methacryloyloxydecyl-dihydrogenphosphate (MDP) could bond directly to metal oxides (Kern & Wegner, 1998). Thus, the presence of hydroxyl groups on the zirconia surface could activate the reaction with the phosphate ester monomers of

142

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

MDP (Oyagüe et al., 2009; Özcan & Bernasconi, 2015). The use of such monomers is responsible for water-resistant chemical bond with zirconia that is significantly higher compared to the bond strength with conventional bis-GMA resin cements. This chemical bond seems stable even after aging in water storage or the decrease of bond strength is not statistically significant (Kern & Wegner, 1998). The use of MDP based resin cements is indispensable for achieving proper adhesion to zirconia surface (Kern & Wegner, 1998; Blatz et al., 2010; Oyagüe et al., 2009). The bond strength could even be further improved with the use of MDP-containing silane coupling agents after silica-coating (Özcan & Bernasconi, 2015) (Figure 1).

Figure 1. 1-4. 1) Tribochemical silica coating of the zirconia surface; 2) Silane coupling agent application; 3) Resin luting cement application; 4) Cemented zirconia restoration.

Since application of surface conditioning methods are rather cumbersome and require additional armamentarium in the clinical practice, self-adhesive resin cements are introduced that require no initial surface conditioning of zirconia or the dental tissues with the advantages of simplified clinical steps, low incidence of postoperative sensitivity (Blatz et al, 2010). Manufacturers promote the use of self-adhesive resin cements as a chemical conditioning method for zirconia, dismissing any other mechanical or chemical conditioning methods that would be mandatory with conventional resin cements (Özcan & Volpato, 2015). Such resin cements show adequate adhesion to different substrates, including zirconia (Passos et al., 2010; Sciasci et al., 2015; Ehlers et al., 2015). The presence of functional acidic monomers in their composition allows for chemical bond with

An Update of Current Knowledge on Adhesion …

143

the metal oxides on the zirconia surface (Blatz et al., 2010). Nevertheless, limitations of self-adhesive resin cements are referred as low degree of conversion, low diffusion level into dentin and less hydrolytic stability (Monticelli et al., 2008; Vrochari et al., 2009; Özcan & Bernasconi, 2015). A comparison ceramics indicated for frameworks, their different characteristics and the corresponding surface conditioning methods are summarized in Table 1. Table 1. Overview of ceramics indicated for frameworks, their different characteristics and the corresponding surface conditioning methods Type of ceramic Lithium dissilicate

Alumina

Zirconia

Indication

Limitation

Single crowns, Not indicated anterior and for extended posterior FDP’s prostheses up 3 unit Not indicated for areas with Ceramic high aesthetic infrastructures demand up to 4 units involving translucently

Anterior and posterior FDPs, implant abutments and root posts

Not indicated for areas with high aesthetic demand involving translucently

Flexural Hydrofluoridric Surface treatments resistance acid sensivity 350MPa

600MPa

Acid sensitive

- Hidrofluoridric acid etching - Silane application

Acid resistance

- Silica coating or airparticle abrasion with aluminium oxide - Silane application

1000MPa Acid resistance

-Air-particle abrasion with aluminum oxide -Tribochemical silica coating - Hexamethyldisiloxane plasma spray - Micropearls of low fusing porcelain application - Silicon tetrachloride vapor deposition - Er:YAG laser CO2 laser - Heated HF 48% - Heated acid solution

3.1. Adhesive Interface Stability Based on the currently available data in the literature, some concerns are present regarding the zirconia-resin adhesive interface in that the process of aging conditions, simulating the oral environment, decreases the hydrolytic stability or the mechanical resistance of zirconia (Tzanakakis et al., 2016; Lung & Matinlinna, 2012). The main reasons for approximately 50% of reduction from

144

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

baseline to aged conditions are the hydrolytic effect of water and the moisture of the environment (Abousheilib et al., 2009). Typically, thermocycling aging method is used to simulate the worst-case oral environment and aging of adhesive interfaces where water at alternating temperatures between 5 and 55°C causes thermal expansion and contraction of the bonded materials, aging the bonded interface (Liu et al., 2014). In fact, the increase in surface area with the air-particle abrasion with different particles (silica, alumina, zirconia) for adhesion can help to improve the resistance against the hydrolytic effects on the resin-zirconia adhesive interface (Liu et al., 2014; Liu et al., 2015; Tzanakakis et al., 2016). However, even with silica coating, although the initial bond strength is doubled compared to the non-conditioned control group, after aging conditions the mean bond strength also decrease. This was partially attributed to the loosening of the attached silica and the hydrolytic degradation of the siloxane interface layer (Liu et al. 2013). Unfortunately, findings regarding this subject are difficult to compare between the studies since different zirconia materials, experimental tests, size of specimens and aging conditions greatly affect the results (Özcan & Bernasconi, 2015). However, at least it can be stated that there is practically no adhesion on zirconia when no surface conditioning method is employed, providing that the achieved results after all types conditioning methods tend to show poor long-term stability (Tzanakakis et al., 2016).

4. Phase Transformation The possibility to optimize the adhesion between resin luting composite and zirconia with surface conditioning methods is essential. However, especially mechanical surface conditioning methods could alter the zirconia microstructure (Karacoca & Yilmaz, 2009; Thompson et al., 2011). In this regard, the higher the amounts of monoclinic phase in zirconia, the higher the chances for failure. Accordingly, air-abrasion methods increase the monoclinic content in the zirconia microstructure (Kosmac et al., 1999) since the particle organization changes and fragile areas are created on the surface of the material. It has to be however noted that air-abrasion could be performed using different particle sizes (e.g., 30 – 250 µm) and deposition duration (e.g., 5, 15 and 30 seconds) that have direct affect on the amount of monoclinic content (Turp et al. 2013). The results of XRD analysis demonstrate higher amounts of monoclinic phase with the increase in the particle size and durations. There is thus concern on the possible impact of air-abrasion protocols that could create slow crack growth of zirconia, producing surface

An Update of Current Knowledge on Adhesion …

145

defects, reduce the mechanical strength and consequently affecting its long-term performance (Zhang et al. 2004; Zhang et al., 2006). Interestingly however, air-particle abrasion with 110 µm particle size can create a thin compressive layer on the zirconia surface and even increase the strength of zirconia as it initiates transformation when the material is subjected to stresses (Kosmac et al., 1999; Kosmac et al., 2000). Yet, this compressive layer and the amount of monoclinic phase content are highly dictated by the deposition duration and pressure (Turp et al., 2013). Since surface conditioning methods commonly introduce defects on the zirconia microstructure, fused glass infiltration method was suggested on the top and bottom surface of zirconia (Zhang & Kim, 2009). This process resulted in a graded glass/ceramic/glass material with an outer surface having residual glass layer, a dense ceramic core in the middle and a graded glass ceramic layer internally. These characteristics are claimed to improve optical properties and overcome adhesion related problems. In this graded material, glass content is relatively high at the residual glass layer interfaces and gradually transforms to a dense Y-TZP in the interior regions. With this architecture, a network of glasscoated zirconia grains are exposed that serve for ideal surface morphology for silanization and adhesive resin penetration. The graded material approach needs to be etched with hydrofluoric acid and silanized that could eventually eliminate the need for surface conditioning using air-abrasion technologies required for pure YTZP (Zhang & Kim, 2009). However, studies in this regard are limited.

Conclusion A lack of consensus exists on the unique method to bond resin-based luting cements to zirconia resulting in confusion in the dental community. Yet, the available evidence is in favour of micromechanical retention achieved through airabrasion protocols, especially using tribochemical silica coating, followed by MDP containing silane coupling agents and MDP based resin luting cements.

References Aboushelib, M.N. (2011). Evaluation of zirconia/resin bond strength and interface quality using a new technique. J. Adhes. Dent. 13, 255-60.

146

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

Aboushelib, M.N., Mirmohamadi, H., Matinlinna, J.P., Kukk, E., Ounsi, H.F., Salameh, Z. (2009). Innovations in bonding to zirconia-based materials. Part II: Focusing on chemical interactions. Dent.Mater. 25, 989-93. Atsu, S.S., Kilicarslan, M.A., Kucukesmen, H.C., Aka, P.S. (2006). Effect of zirconium-oxide ceramic surface treatments on the bond strength to adhesive resin. J. Prosthet. Dent. 95, 430-6. Attia, A. (2011). Bond strength of three luting agents to zirconia ceramic-influence of surface treatment and thermocycling. J. Appl. Oral Sci.19, 388-395. Blatz, M.B., Chiche, G., Holst, S., Sadan, A. (2007). Influence of surface treatment and simulated aging on bond strengths of luting agents to zirconia. Quintessence Int. 38, 745-753. Blatz, M.B., Phark, J.H., Ozer, F., Mante, F.K., Saleh, N., Bergler, M., Sadan, A. (2010). In vitro comparative bond strength of contemporary self-adhesive resin cements to zirconium oxide ceramic with and without air-particle abrasion. Clin. Oral. Investig. 14, 187-92. Blatz, M.B., Sadan, A., Kern, M. (2003) Resin-ceramic bonding: a review of the literature. J. Prosthet. Dent. 89, 268-274. Burke, F.J., Flemming, G.I., Nathanson, D., Marquis, P.M. (2002). Are adhesive technologies needed to support ceramics? An assessment of the current evidence. J. Aesthet. Dent. 4, 7-22. Castro, H.L., Corazza, P.H., Paes-Júnior, T.A., Della Bona, A. (2012). Influence of Y- TZP ceramic treatment and different resin cements on bond strength to dentin. Dent. Mater. 28, 1191-7. Cavalcanti, A.N., Foxton, R.M., Watson, T.F., Oliveira, M.T., Giannini, M., Marchi, G.M. (2009). Bond strength of resin cements to a zirconia ceramic with different surface treatments. Oper. Dent. 34, 280-287. Cheung, G.J., Botelho, M.G. (2015). Zirconia Surface Treatments for Resin Bonding. J. Adhes. Dent. 17, 551-558. Cura, C., Özcan, M., Isik, G., Sracoglu, A. (2012). Comparison of alternative adhesive cementation concepts for zirconia ceramic: glaze layer vs zirconia primer. J. Adhes. Dent. 14, 75-82. Curtis, A.R., Wright, A. J., Fleming, G.J.P. (2006). The influence of surface modification techniques on the performance of a Y-TZP dental ceramic. J. Dent. 3, 195-206. Della Bona, T.A., Donassollo, F.F., Demarco, A.A., Barrett, A.A., Mecholsky Jr, J.J. (2007). Characterization and surface treatment on topography of a glassinfiltrated alumina/zirconia- reinforced ceramic. Dent. Mater. 23, 769-775.

An Update of Current Knowledge on Adhesion …

147

Derand, T., Molin, M., Kleven, E., Haag, P., Karlsson, S. (2008). Bond strength of luting materials to ceramic crowns and different surface treatments. Eur. J. Prosthod. Restor. Dent. 16, 35-38. Derand, T., Molin, M., Kvam, K. (2005) Bond strength of composite luting cement to zirconia ceramic surfaces. Dent. Mater. 21, 1158-1162. Derand. P., Derand, T. (2000). Bond strength of luting cements to zirconium oxide ceramics. Int. J. Prosthod. 13, 131-5. Duran, P., Moure, C. (1984). Sintering at near theoretical density and properties of PZT ceramics chemically prepared. J. Mater. Sci. 20, 827-833. Ehlers, V., Kampf, G., Stender, E., Willershausen, B., Ernst, C.P. (2015). Effect of thermocycling with or without 1 year of water storage on retentive strengths of luting cements for zirconia crowns. J. Prosthet. Dent.113, 609-615. El-Korashy, D.I., El-Refai, D.A. (2014). Mechanical properties and bonding potential of partially stabilized zirconia treated with different chemomechanical treatments. J. Adhes. Dent. 16, 365-76. Erdem, A., Akar, G.C., Erdem, A., Kose, T. (2014). Effects of different surface treatments on bond strength between resin cements and zirconia ceramics. Oper. Dent. 39, e118-e127. Ferrari, M., Vichi, A., Zarone, F.(2015). Zirconia abutments and restorations: from laboratory to clinical investigations. Dent. Mater. 31, e63-76. Garvie, R.C., Nicholson, P.S. (1972). Structure and thermomechanical properties of partially stabilized zirconia in the CaO-ZrO2 system. J. Amer. Ceram. Soc. 55, 152-157. Guan, S.H., Zhang, X.J., Liu, Z.P. (2015). Energy landscape of zirconia phase transitions. J. Am. Chem. Soc., 137, 8010-8013. Guazzato, M., Quach, L., Albakry, M., Swain, M.V. (2005). Influence of surface and heat treatments on the flexural strength of Y-TZP dental ceramic. J. Dent. 33, 9-18. International Standards Organization: Implants for surgery. Ceramic materials based on yttria-stabilized tetragonal zirconia. 2008. Janda, R. Roulet, J.F., Wulf, M., Tiller, H.J. (2003). A new adhesive technology for all-ceramics. Dent. Mater. 19, 567-573. Karakoca, S., Yilmaz, H. (2009). Influence of surface treatments on surface roughness, phase transformation, and biaxial flexural strength of Y-TZP ceramics. J. Biomed. Mater. Res. Part B: App. Biomater. 91B, 930-937. Kasraei, S., Rezaei-Soufi, L., Heidari, B., Vafaee, F. (2014). Bond strength of resin cement to CO2 and Er:YAG laser-treated zirconia ceramics. Restor. Dent. Endod. 39, 296-302.

148

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

Kern, M., Barloi, A., Yang, B. (2009). Surface conditioning influences zirconia ceramic bonding. J. Dent. Res. 88, 817-822. Kern, M., Wegner, S.M. (1998). Bonding to zirconia ceramic: adhesion methods and their durability. Dent. Mater. 14, 64-71. Kim, S.T., Cho, H.J., Lee, Y.K., Choi, S.H., Moon, H.S. (2010). Bond strength of Y-TZP-zirconia ceramics subjected to various surface roughening methods and layering porcelain. Surf. Inter. Analysis 42, 576-80. Kosmac, T., Oblak, C., Jevnikar, P., Funduk, N., Marion L. (2000). Strength and reliability of surface treated Y-TZP dental ceramics. J. Biomed. Mater. Res. 53, 304-313. Kosmac, T., Oblak, C., Jevnikar, P., Funduk, N., Marion, L. (1999). The effect of surface grinding and sandblasting on flexural strength and reliability of YTZP zirconia ceramic. Dent. Mater. 15, 426-433. Liu, D., Pow, E.H., Tsoi, J.K.H., Matinlinna, J.P. (2014). Evaluation of four surface coating treatments for resin to zirconia bonding. J. Mech. Behav. Biomed. Mater., 32, 300-309. Liu, D., Tsoi, J.K.H., Matinlinna, J.P., Wong, H.M. (2015). Effects of some chemical surface modifications on resin zirconia adhesion. J. Mech. Behav. Biomed. Mater., 46, 23-30. Lughi, V., Sergo, V. (2010). Low temperature degradation -aging- of zirconia: A critical review of the relevant aspects in dentistry. Dent. Mater. 26, 807-820. Lung, C.Y.K., Matinlinna, J.P. (2012). Aspects of silane coupling agents and surface conditioning in dentistry: an overview. Dent. Mater. 28, 467-477. Matinlinna, J.P., Heikkinen, T., Özcan, M., Lassila, L.V., Vallittu, P.K. (2006). Evaluation of resin adhesion to zirconia ceramic using some organosilanes. Dent. Mater. 22, 824-31. Mattiello, R.D.L., Coelho, T.M.K., Insaurralde, E., Coelho, A.A. K., Terra, G.P., Kasuya, B., Favar I.N, Gonçalvez, L.S., Fonseca, R. B. (2013). A review of surface treatment methods to improve the adhesive cementation of zirconiabased ceramics. ISRN Biomaterials, 2013. Michida, S.M., Kimpara, E.T., dos Santos, C., Souza, R.O., Bottino, M.A., Özcan, M. (2015). Effect of air-abrasion regimens and fine diamond bur grinding on flexural strength, Weibull modulus and phase transformation of zirconium dioxide. J. Appl. Biomater. Func. Mater. 16, e266-273. Miyazaki, T., Nakamura, T., Matsumura, H., Ban, S., Kabayashi, T. (2013). Current status of zirconia restoration. J. Prosthodont. Res. 57, 236-261. Monticelli, F., Osorio, R., Mazzitelli, C., Ferrari, M., Toledano, M. (2008). Limited decalcification / diffusion of self-adhesive cements into dentin. J. Dent. Res.87, 974-979.

An Update of Current Knowledge on Adhesion …

149

Oyagüe, R.C., Monticelli, F., Toledano, M., Osorio, E., Ferrari, M., Osorio, R. (2009). Influence of surface treatments and resin cement selection on bonding to densely sintered zirconium-oxide ceramic. Dent. Mater. 25, 172-179. Özcan, M. (2013). Air abrasion of zirconia resin-bonded fixed dental prostheses prior to adhesive cementation: why and how. J. Adhes. Dent, 15, 394. Özcan, M. (2014). Airborne particle abrasion of zirconia fixed dental prostheses. J. Esthet. Restor. Dent. 26, 359-362. Özcan, M., Bernasconi, M. (2015). Adhesion to zirconia used for dental restorations: a systematic review and meta-analysis. J. Adhes. Dent. 17, 7–26. Özcan, M., Melo, R.M., Souza, R.O., Machado J.P., Valandro L., Botttino M.A (2013). Effect of air-particle abrasion protocols on the biaxial flexural strength, surface characteristics and phase transformation of zirconia after cyclic loading. J. Mech. Behav. Biomed. Mater. 20, 19-28. Özcan, M., Nijhuis, H., Valandro, L.F. (2008). Effect of various surface conditioning methods on the adhesion of dual-cure resin cement with MDP functional monomer to zirconia after thermal aging. Dent. Mater. J. 27, 99-104. Özcan, M., Vallittu, P.K. (2003). Effect of surface conditioning methods on the bond strength of luting cements to ceramics. Dent. Mater. 19:825-831.
Özcan, M.; Volpato, C.A.M. (2015). Adhesion to zirconium dioxide used for dental reconstructions: surface conditioning concepts, challenges and future prospects. Cur. Oral Health Rep. 2, 190-194. Passos, S.P., May, L.G., Barca, D.C., Özcan, M., Bottino, M.A., Valandro, L.F. (2010). Adhesive quality of self-adhesive and conventional adhesive resin cement to Y-TZP ceramic before and after aging conditions. Oper. Dent. 35, 689-696. Passos, S.P., Nychka, J.A., Major, P., Linke, B., Flores-Mir, C. (2015). In vitro fracture toughness of commercial Y-TZP ceramics: A systematic review. J Prosthodont. 24, 1-11. Piascik, J.R., Swi, E.J., Thompson, J.Y., Grego, S., Stoner, B.R. (2009). Surface modification for enhanced silanation of zirconia ceramics. Dent. Mater. 25, 1116-1121. Piconi, C., Maccauro, G. (1999). Zirconia as a ceramic biomaterial. Biomaterials 20, 1-25. Reich, S., Hornberger, H. (2002). The effect of multicolored machinable ceramics on the esthetics of all-ceramic crowns. J. Prosthet. Dent. 88, 44-49. Sarmento, H.R., Campos, F., Souza, R.S., Machado, J.P., Souza, R.O., Bottino, M.A., Özcan, M. (2014). Influence of air-particle deposition on the surface topography and adhesion of resin cement to zirconia. Acta Odontolol. Scand. 72, 346-353.

150

M. L. P. D. Engler, E. Ruales, M. Özcan et al.

Sciasci, P., Abi-Rached, F.O., Adabo, G.L., Baldissara, P., Fonseca, R.G. (2015). Effect of surface treatments on the shear bond strength of luting cements to Y-TZP ceramic. J. Prosthet. Dent. 113, 212-219. Senyilmaz, D.P., Palin, W.M., Shortall, A.C., Burke, F.J. (2007) The effect of surface preparation and luting agent on bond strength to a zirconium-based ceramic. Oper. Dent. 32, 623-630. Souza, R.O., Valandro, F.L., Melo, R.M., Machado, J.P., Bottino,M.A., Özcan, M.(2013). Air-particle abrasion on zirconia ceramic using different protocols: effects on biaxial flexural strength after cyclic loading, phase transformation and surface topography. J. Mech. Behav. Biomed. Mater. 26, 155-63. Subaşı, M.G., Özgür, I. (2014). Influence of surface treatments and resin cement selection on bonding to zirconia. Lasers Med. Sci. 29, 19-27. Thompson, J.Y., Stoner, B.R., Piascik, J.R., Smith, R. (2011). Adhesion/ cementation to zirconia and other non-silicate ceramics: where are we now? Dent. Mater. 27, 71-82. Tsuo, Y., Yoshida, K., Atsuta, M. (2006). Effects of alumina-blasting and adhesive primers on bonding between resin luting agent and zirconia ceramics. Dent. Mater. J. 25, 669-674. Turp, V., Sen, D., Tuncelli, B., Goller, G., Özcan, M. (2013). Evaluation of airparticle abrasion of Y-TZP with different particles using microstructural analysis. Austr. Dent. J. 58, 183-191. Tzanakakis, E.G.C., Tzoutzas, I.G., Koidis, P.T. (2016). Is there a potential for durable adhesion to zirconia restorations? A systematic review. J. Prosthet. Dent., 115, 9-19. Vagkopoulou, T. Koutayas, S.O., Koidis, P., Strub, J.R. (2009). Zirconia in dentistry: Part 1. Discovering the nature of an upcoming bioceramic. Eur. J. Esthet. Dent. 4, 130-151. Valandro, L.F., Özcan, M., Amaral, R., Leite, F.P., Bottino, M.A. (2007). Microtensile bond strength of a resin cement to silica-coated and silanized InCeram zirconia before and after aging. Int. J. Prosthodont. 20, 70-72. Vrochari, A.D., Eliades, G., Hellwig, E., Wrbas, K.T. (2009). Curing efficiency of four self-etching, self-adhesive resin cements. Dent. Mater. 25, 1104-1108. Xible, A.A., Jesus Tavarez, R.R., Araujo, C.R., Bonachela, W.C. (2006). Effect of silica coating and silanization on flexural and composite-resin bond strengths of zirconia posts: an in vitro study. J. Prosthet. Dent. 95, 224-229. Zhang, Y., Kim, J.W. (2009). Graded structures for damage resistant and aesthetic all-ceramic restorations. Dent. Mater. 25, 781-790.

An Update of Current Knowledge on Adhesion …

151

Zhang, Y., Lawn, B.R., Rekow, E.D., Thompson, V.P. (2004). Effect of sandblasting on the long-term performance of dental ceramics. J. Biomed. Mater. Res. Part B: Appl. Biomater. 15, 381-386. Zhang,Y., Lawn, B.R., Malament, K.A., Thompson, V.P., Rekow, E.D. (2006). Damage accumulation and fatigue life of particle-abraded ceramics. Int. J. Prosthodont. 19, 442-448.

INDEX A acid, 138, 141, 143 acidic, 141, 142 activated carbon, 4 adaptation, 138, 140 adhesion, vii, ix, x, 20, 51, 135, 136, 138, 139, 140, 141, 142, 144, 145, 148, 149, 150 adhesion force, 51 adsorption, 22 adverse effects, 137 aesthetic, ix, 135, 137, 143, 150 AFM, 52, 53 agriculture, 2, 3 Al2O3 particles, 139 alumina particles, ix, 136, 140 aluminium, 9, 51, 143 aluminum oxide, 53, 143 analytical modelling, vii, viii, ix, 65, 66, 67, 70, 78, 103, 104, 105, 106, 109 annealing, 48 aquaculture, 2 asymptotics, 40 atoms, 35

B band gap, 34, 35 batteries, 4 biocompatibility, ix, 135, 137 biodiesel, 30 bioenergy, 25

biomass, vii, viii, 1, 2, 3, 4, 5, 6, 8, 9, 10, 11, 12, 14, 15, 16, 17, 18, 19, 20, 21, 22, 23, 24, 25, 26, 27, 28 biomass ash-clay bricks, viii, 2, 14, 24 biotechnological applications, 25 BOE, 29 bonding, 138, 139, 146, 147, 148, 149, 150 bottom and fly ash, vii, 1, 7, 9 bottom ash, vii, 1, 3, 4, 6, 7, 9, 10, 26, 27, 28, 29 bottom pine-olive pruning ash, vii, 1 by-products, 6, 25

C CAD, 136 calcium, 7, 13, 14, 137 calcium carbonate, 7 CAM, 136 capillary, 27 carbon, 4, 7, 9, 12, 14 cell surface, 117, 118, 121, 122, 123, 126, 128 ceramic, vii, ix, x, 1, 4, 5, 9, 15, 19, 22, 24, 26, 28, 29, 30, 31, 35, 36, 38, 42, 43, 44, 46, 50, 59, 61, 135, 136, 137, 138, 139, 141, 143, 145, 146, 147, 148, 149, 150 ceramic bricks, vii, 1, 22, 29, 31 ceramic materials, vii, 5, 24, 35, 42, 136 ceramics, viii, x, 2, 28, 29, 30, 31, 33, 34, 35, 36, 37, 40, 43, 47, 49, 50, 51, 54, 55, 58, 61, 62, 63, 97, 99, 127, 128, 130, 136, 137, 138, 143, 146, 147, 148, 149, 150, 151 cerium, 137

154

Index

chemical, vii, ix, x, 1, 3, 4, 5, 9, 27, 35, 50, 135, 136, 137, 142, 146, 148 chemical characteristics, 4 chemical interaction, 146 chemical stability, ix, 135, 137 clay bricks, vii, viii, 2, 4, 5, 6, 15, 16, 17, 18, 19, 21, 22, 23, 24, 27, 28, 29, 30 cleaning, 3, 140 cleavages, 52, 53 clusters, 35 CO2, 2, 13, 14, 141, 143, 147 coal, 2, 4, 26, 27, 28 cogeneration, 5, 6 colour stability, 137 combustion, 2, 3, 4, 5, 6, 7, 10, 12, 14, 15, 18, 26, 27, 28, 29 combustion processes, 4 compaction, viii, 34, 61 composite material, 50, 66, 104 composite resin, ix, 135, 138 composites, 34, 43, 48, 50, 51, 61 composition, 3, 4, 7, 8, 9, 10, 23, 27, 51, 54, 137, 138, 142 compounds, 10 conditioning, vii, ix, x, 5, 6, 136, 138, 139, 140, 142, 143, 144, 145, 148, 149 conduction, 34 conductivity, 4, 22, 43, 54, 137 construction, vii, viii, 2, 4, 24, 29 contamination, 3, 139 cooling, vii, viii, ix, 52, 65, 77, 78, 103, 104, 105 cooling process, viii, ix, 77, 78, 103, 104, 105 covalent bond, 139, 140 cracks, 6, 14, 20 critical value, 61 crowns, ix, 135, 143, 147, 149 crystalline, 9, 10, 137 crystallites, 51 crystals, 35, 61, 137, 138 cytotoxicity, 137

D decomposition, 12, 13, 14, 15, 18 defects, 6, 14, 35, 49, 145 degradation, 144, 148 dental ceramics, 148, 151

dental restorations, 138, 149 dentin, 143, 146, 148 dentistry, vii, ix, x, 135, 136, 148, 150 deposition, 42, 140, 143, 144, 145, 149 derivatives, 37 differential equations, 114 diffraction, 10 diffusion, viii, 33, 34, 36, 37, 40, 43, 44, 49, 54, 55, 56, 57, 58, 59, 61, 141, 143, 148 dispersion, 34, 36, 37, 39, 40, 57 dispersity, 59 displacement, 70, 79, 80, 81, 82, 83, 85, 87, 88, 110, 114, 115, 117, 118, 119, 121, 122, 123, 126, 128, 129 distribution, 7, 50, 55, 57 drug delivery, 4 DTA curve, 12 durability, 19, 136, 148

E economic problem, 3 education, 25 elastic continuum, viii, 65, 72, 112 electron, 8, 35, 50, 55, 57 endothermic, 12, 13, 14 energy, 2, 3, 5, 24, 25, 50, 51, 113, 116, 119, 123, 125, 138, 141 energy consumption, 2 energy density, 116, 123 engineering, 17, 105 entrapment, 55, 57, 58 environment, 22, 143, 144 environmental awareness, 4 environmental impact, 22 environmental issues, 28 Environmental Protection Agency (EPA), viii, 2, 9, 22, 24, 27 equilibrium, 70, 71, 72, 73, 109, 110, 111, 113 erbium, 140 ester, 141 etching, 138, 141, 143, 150 ethanol, 140 evolution, 21 exothermic effects, 12 experimental condition, 55, 57 extraction, 5, 30, 31 extrusion, 31

155

Index

F fibroblasts, 137 filtration, 31 fire resistance, 26 fisheries, 2 fluorescence, vii, 1, 7 fly and bottom biomass ash, vii, 1, 2, 11 fly ash, 1, 4, 6, 7, 9, 10, 26, 27, 28 forbidden gap, viii, 33, 34, 61 force, 52, 53, 137 formation, 43, 44, 51, 52 formula, 38, 40, 57, 92, 93, 94, 95, 97, 98, 119, 127, 128 fracture toughness, 149 fragments, 35, 50 friction, 51

G global warming, 2 glycerin, 140 grades, 20 grain boundaries, viii, 33, 35, 36, 40, 54, 56, 61 grain size, viii, 33, 34, 36, 42, 43, 44, 51, 56 growth, 21, 34, 50, 51, 61, 144

H harmful effects, 22 harvesting, 3 hazardous waste, 22 health, 22 heat flow, vii, viii, 33, 34, 35, 61 heavy metals, 9, 22 helium, 34, 35, 42, 54, 58, 61 hydrofluoric acid, 138, 141, 145 hydrogen, 7, 12 hydrolytic stability, 143 hydroxide, 14 hydroxyl groups, 141

I images, 52, 53 immersion, 8

immobilization, 22 implant abutments, ix, 135, 136 implants, 136 incomplete combustion, 12 industrial wastes, 3 industry, 2, 3, 4, 6, 25, 30, 31 inequality, 55 ingredients, 4 insulation, 4, 22, 24 integration, 74, 75, 76, 77, 80, 84, 85, 114, 117, 118 interface, 34, 51, 139, 143, 144, 145 interference, 42 intervals, 87, 88, 91, 93 ions, 14 iron, 14, 50, 51, 52, 53, 55, 56, 58, 59, 60 isotropic cylindrical particles, vii, viii, 65, 66, 99

L landfills, 3, 22, 29 landscape, 147 lattices, viii, 33, 34 layering, 148 leachates, viii, 2 leaching, 9, 22, 24, 27 linear dependence, 36 liquid phase, 15 low temperatures, 35, 50, 140

M macropores, 21 magnesium, 137 magnetic field, 43 magnitude, 54, 57, 58, 137 manufacturing, 4, 35 mass, 7, 13, 14, 40, 55 mass loss, 13 materials, vii, viii, ix, x, 4, 9, 14, 23, 24, 26, 29, 31, 33, 35, 50, 61, 65, 66, 67, 68, 74, 76, 99, 103, 104, 105, 106, 107, 130, 135, 136, 138, 140, 141, 144, 146, 147 matrix, vii, viii, ix, 10, 33, 35, 36, 37, 40, 48, 50, 56, 57, 58, 59, 60, 61, 65, 66, 67, 68, 69, 70, 71, 75, 76, 77, 78, 79, 80, 81, 82, 83, 84, 86, 87, 88, 91, 92, 93, 94, 95,

156

Index

96, 97, 98, 99, 103, 104, 105, 106, 107, 108, 109, 112, 115, 116, 117, 118, 119, 120, 121, 123, 125, 127, 128, 129, 130, 138 matrix system, vii, viii, ix, 65, 66, 67, 69, 70, 79, 98, 99, 103, 105, 106, 107, 108, 119, 129, 130 matter, 10, 15, 16, 27 measurement, 43, 57 mechanical properties, vii, viii, ix, x, 2, 18, 22, 28, 135, 136, 137 medicine, 137 melting, 9, 77, 78, 97, 104, 128 melting temperature, 97, 128 meta-analysis, 149 metal oxides, 141, 143 metallurgy, 128 metal-oxide composites, 34 metals, 10, 22, 24 microscope, 8 microstructural parameters, viii, ix, 65, 68, 99, 103, 104, 105, 107, 109, 130 microstructure, ix, 27, 135, 137, 144, 145 mixing, vii, 1, 6, 31 model system, viii, ix, 65, 66, 67, 99, 103, 106, 130 modelling, vii, viii, ix, 65, 66, 67, 70, 78, 103, 104, 105, 106, 109 modifications, 141 modulus, 36, 71, 112, 148 moisture, 6, 14, 27, 144 monolithic crowns, ix, 135 monomers, 141, 142 morphology, 145 MTS, 8 municipal solid waste, 4

N nanocomposites, viii, 33, 50 nanoparticles, 51 nanostructured ceramics, vii, viii, 34, 43 nanostructured materials, viii, 33, 34 neglect, 58 nitrogen, 7, 12 NMR, 28 nonequilibrium, 34, 35, 42, 43

O olive oil, 5, 25, 30 olive pomace, vii, 1, 3, 4, 5, 7, 9 olive stone bottom ash, 1, 7, 9 opacity, 40 optical properties, 145 ores, 40 organic matter, 12, 14, 15, 18 organic soils, 27 oxidation, 52, 61

P partial differential equations, 73 peat, 3, 27 phase boundaries, 61 phase transformation, ix, 136, 137, 147, 148, 149, 150 phonon spectroscopy, 34, 35 phononic lattice, viii, 33, 34 phonons, 34, 35, 36, 37, 38, 40, 41, 42, 43, 46, 47, 48, 49, 50, 54, 58, 61 phosphate, 10, 141 photonic traps, viii, 33 physical and mechanical properties, 23 physical properties, 35, 50 physicochemical methods, ix plasticity, 6 porosity, vii, 2, 7, 8, 17, 18, 19, 20, 21, 22, 24, 141 potassium, 10 power plants, 4, 5, 6, 28 preservation, 61 programming, 98, 127 project, 26, 62 propagation, 35, 42, 43, 57 properties, vii, viii, ix, x, 2, 3, 4, 6, 14, 18, 22, 23, 24, 28, 30, 31, 33, 34, 35, 36, 40, 50, 51, 54, 57, 61, 135, 136, 137, 145, 147 prostheses, ix, 135, 143, 149 prosthesis, 136 prosthetic restorations, 136 protection, 26 pruning, vii, 1, 3, 6, 7, 9 pulp, 4 pyrophosphate, 10

157

Index

Q quartz, 10

R radiation, 7 radius, viii, 35, 36, 40, 55, 65, 67, 68, 79, 80, 99, 105, 106, 109 RAS, 33 raw materials, viii, 2, 4, 6, 10, 24 reactions, 14, 18 reactivity, 31 real numbers, 127 reception, 29 reconstruction, 37 recycling, vii, viii, 2 red mud, 27 redistribution, 51 relaxation, 77, 97, 104, 128 reliability, 148 renewable energy, 2, 3, 5, 6, 28 renormalization, 37, 61 requirement, 24, 61 requirements, viii, 2, 4 residues, 2, 3, 4, 5, 26, 28 resin composite, ix, 135, 139, 140 resistance, 19, 20, 143, 144 resolution, 8 resources, 3 restoration, 140, 142, 148 restorative material, 135 restructuring, 54 rice husk, vii, 1, 2, 5, 6, 7, 9, 26, 27, 28 room temperature, 7, 137 root, 136, 143 roughness, 138, 139, 147

S salts, 8 sawdust, 3 scattering, 35, 36, 37, 38, 39, 40, 41, 42, 43, 44, 49, 50, 54, 55, 57, 58, 61 science, 29, 30, 31, 136 SEM micrographs, 22, 24 sewage, 5, 27 shade, 8

shape, viii, 53, 65, 67, 69, 106 shear, 70, 71, 72, 92, 93, 94, 95, 110, 111, 112, 113, 139, 150 Si3N4, 97, 99, 127, 128, 129, 130 silane, 138, 139, 140, 142, 145, 148 silanol groups, 139 silica, ix, 4, 9, 10, 18, 24, 136, 138, 139, 140, 142, 143, 144, 145, 150 silicon, ix, 4, 135, 138, 139 silicon dioxide, ix, 135 sintering, viii, 4, 9, 10, 34, 40, 50, 51, 52, 54, 59, 61 SiO2, ix, 8, 9, 10, 23, 135, 138 sludge, 5, 27, 30 social development, 2 solid matrix, 78, 104 solid solutions, 57 solid waste, 25 solution, viii, 2, 24, 43, 66, 67, 74, 75, 76, 105, 114, 141, 143 specific heat, 35, 43, 57, 58, 61 spectroscopy, 34, 35 stability, 144 stabilization, 47 storage, 142, 147 stress, 15, 18, 66, 71, 72, 77, 84, 86, 93, 95, 97, 98, 104, 111, 112, 113, 116, 117, 118, 119, 120, 121, 123, 125, 128, 129, 130 structure, 34, 35, 44, 48, 50, 51, 58 substrates, 138, 142 sugarcane, 5, 27, 28 sulphur, 7, 12 surface area, 70, 80, 81, 110, 139, 144 surface conditioning, vii, ix, x, 136, 138, 139, 140, 142, 143, 144, 145, 148, 149 surface energy, 10, 138, 139, 140 surface modification, 140, 141, 148 surface properties, 31 surface treatment, 146, 147, 148, 149, 150 survival, ix, 135 sustainable development, 24 symmetry, 35, 69, 70, 107 synthesis, vii, viii, 4, 33, 34, 35, 44, 50, 51, 61

T techniques, viii, 25, 65, 68, 98, 107, 127, 146

158

Index

technological, 2, 6, 14, 28, 54, 61 technology(ies), viii, 3, 12, 29, 33, 34, 136, 141, 145, 146, 147 temperature, 4, 6, 7, 9, 10, 14, 17, 34, 35, 40, 42, 43, 46, 50, 51, 53, 54, 55, 57, 58, 61, 77, 78, 79, 97, 104, 105, 128, 141, 148 temperature dependence, 43, 54, 55, 58 tensions, 15 TGA, 7, 12, 14 thermal aging, 149 thermal analysis, vii, 1, 7 thermal energy, 3, 5 thermal expansion, viii, ix, 65, 66, 78, 99, 103, 104, 105, 129, 144 thermal properties, 61 thermal stability, 50 thermal stress, vii, viii, ix, 65, 66, 67, 68, 69, 77, 78, 79, 89, 92, 94, 96, 97, 98, 99, 103, 104, 105, 107, 109, 119, 127, 128, 129, 130 thermal stresses, vii, viii, ix, 65, 66, 67, 68, 69, 77, 78, 79, 89, 92, 94, 96, 97, 98, 99, 103, 104, 105, 107, 109, 119, 127, 128, 129, 130 thermal treatment, 15 thermocrystal efficiency, viii, 33 thermocrystals, viii, 33, 34, 51 titanium, 27 toxicity, 9, 23, 26, 28 trace elements, 28 transformation, 71, 112, 137, 141, 145 transport, 34, 35, 42, 50, 54, 57 treatment, 8, 25, 50, 146 treatment methods, 25

U ultrasound, 60

V vapor, 42, 140, 143

velocity, 43, 55 vibration, 50 viscosity, 15

W waste, vii, 1, 2, 3, 4, 5, 7, 15, 21, 23, 25, 26, 27, 28, 29, 30 waste incineration, 26, 28 waste management, 25 wastewater, 31 water absorption, vii, 2, 17, 18, 19, 20, 21, 24, 27 wavelengths, 35 weight loss, 12, 14, 16 wettability, 138, 140 wood, vii, 1, 3, 4, 5, 6, 7, 9, 10

X X-ray diffraction (XRD), 9, 10, 12, 23, 144

Y yield, 6, 141 Yttria-stabilized tetragonal zirconia polycrystal (Y-TZP), 135 yttrium, ix, 135, 137, 140

Z zeolites, 4 zirconia, vii, ix, x, 135, 136, 137, 138, 139, 140, 141, 142, 143, 144, 145, 146, 147, 148, 149, 150 zirconium, 146, 147, 148, 149, 150 ZnO, 8